Modification of Dynamic Modulus Predictive Models for Asphalt ...

**Modification** **of** **Dynamic** **Modulus** **Predictive** **Models** **for** **Asphalt** Mixtures Containing

Recycled **Asphalt** Shingles

by

Jianhua Yu

A thesis submitted to the graduate faculty

in partial fulfillment **of** the requirements **for** the degree **of**

MASTER OF SCIENCE

Major: Civil Engineering (Civil Engineering Materials)

R. Christopher Williams, Major Pr**of**essor

Vernon R. Schaefer

W. Robert Stephenson

Iowa State University

Ames, Iowa

2012

Copyright © Jianhua Yu, 2012. All rights reserved.

TABLE OF CONTENT

LIST OF TABLES ................................................................................................................... iii

LIST OF FIGURES .................................................................................................................. v

ACKNOLEDGEMENTS ....................................................................................................... viii

ABSTRACT ............................................................................................................................. ix

CHAPTER 1: INTRODUCTION ........................................................................................... 10

CHAPTER 2: LITERATURE REVIEW ................................................................................ 15

Shingle Recycling ............................................................................................................. 16

Previous Researches and Practices **of** RAS Utilization .................................................... 17

**Dynamic** **Modulus** Testing ................................................................................................ 21

**Dynamic** **Modulus** Master Curve ...................................................................................... 22

Witczak E* **Predictive** Model ........................................................................................... 24

Hirsch E* **Predictive** Model .............................................................................................. 27

Previous Evaluation **of** the Witczak and Hirsch E * **Predictive** **Models** ............................ 30

Effects **of** Fibers on **Asphalt** Concrete Mixture **Dynamic** **Modulus** ................................. 40

CHAPTER 3: EXPERIMENTAL PLAN AND TESTING METHODS ............................... 41

Minnesota DOT Demonstration Project ........................................................................... 42

Iowa DOT Demonstration Project .................................................................................... 46

Missouri DOT Demonstration Project .............................................................................. 48

Indiana DOT Demonstration Project ................................................................................ 50

**Dynamic** **Modulus** Test ..................................................................................................... 53

Direct Shear Rehometer (DSR) Test ................................................................................. 54

CHAPTER 4: EVALUATION AND MODIFICATION OF WITCZAK AND HIRSCH

MODELS ................................................................................................................................ 57

Model Input Parameters .................................................................................................... 67

Witczak Model .................................................................................................................. 74

Hirsch Model .................................................................................................................... 88

Model Efficiency Evaluation ............................................................................................ 94

Parameter Evaluation **of** **Models** ..................................................................................... 113

i

CHAPTER 5: CONCLUSIONS AND RECOMMENDATIONS ........................................ 125

Prediction Accuracies **of** the Original E* **Predictive** **Models** ......................................... 126

Modified E* **Predictive** **Models** ...................................................................................... 127

Influences **of** RAS on Parameters **of** the E* **Predictive** **Models** ..................................... 130

Recommendations ........................................................................................................... 130

REFERENCES ..................................................................................................................... 132

APPENDIX A: DYNAMIC MODULUS RESULTS........................................................... 135

APPENDIX B: DSR TEST RESULTS ................................................................................ 148

APPENDIX C: DSR FREQUENCY SWEEP TEST RESULTS ......................................... 150

ii

LIST OF TABLES

Table 1: Typical Shingle Composition [11] ............................................................................ 16

Table 2: Shingle Aggregate Compositions and Size [11] ....................................................... 16

Table 3: Material Properties [29] ............................................................................................ 30

Table 4: Mixture Gradation [29] ............................................................................................. 31

Table 5: Experimental Plan ..................................................................................................... 42

Table 6: Minnesota Demonstration Project Sieve Analysis Results ....................................... 45

Table 7: Iowa Demonstration Project Sieve Analysis Results ................................................ 48

Table 8: Missouri Demonstration Project Sieve Analysis Results ......................................... 50

Table 9: Indiana Demonstration Project Sieve Analysis Results............................................ 52

Table 10: Subjective Classification **of** the Goodness-**of**-Fit Statistical Parameters [37] ........ 58

Table 11: ANOVA Table **for** Witczak 1999 Model with Predicted E*/Lab E* as the

Response ........................................................................................................................... 63

Table 12: ANOVA Table **for** Witczak 2006 Model with Predicted E*/Lab E* as the

Response ........................................................................................................................... 63

Table 13: ANOVA Table **for** Hirsch Model with Predicted E*/Lab E* as the Response ...... 64

Table 14: Mean **of** Model Prediction Accuracy ...................................................................... 65

Table 15: Student-t Test Results **for** Model Prediction Accuracy .......................................... 65

Table 16: Volumetric Properties **of** Compacted Sample Cylinder ......................................... 68

Table 17: VTS Coefficients **of** Recovered **Asphalt** Binder .................................................... 70

Table 18: G* Shift Factors **for** Recovered Binders at Reference Temperature **of** 37 ºC ........ 73

Table 19: Phase Angle Shifting Factors **for** Recovered Binders at Reference Temperature **of**

37 ºC .................................................................................................................................. 74

Table 20: Regression Results **of** 0%-RAS-Effect Calibration Parameters **for** the 1999

Witczak Model .................................................................................................................. 79

Table 21: Regression Results **of** 0%-RAS-Effect Calibration Parameters **for** the 2006

Witczak Model .................................................................................................................. 80

Table 22: Regression Results **of** RAS-Effect Calibration Parameters **for** the 1999 Witczak

Model ................................................................................................................................ 86

Table 23: Regression Results **of** RAS-Effect Calibration Parameters **for** the 2006 Witczak

Model ................................................................................................................................ 87

Table 24: Regression Results **of** 0%-RAS-Effect Calibration Parameters **for** Hirsch 2006

Model ................................................................................................................................ 90

Table 25: Regression Results **of** RAS-Effect Calibration Parameters **for** Hirsch Model ....... 92

Table 26: Coefficient **of** Determination **of** the Witczak **Models** .......................................... 106

Table 27: Coefficient **of** Determination **of** the Hirsch Model ............................................... 113

Table 28: Coefficient Correlation Chart **for** the 1999 Witczak Model ................................. 118

Table 29: Coefficient Correlation Chart **for** the 1999 Witczak Model ................................. 118

Table 30: 2006 Witczak **Modification** Coefficient Correlation Table .................................. 122

Table 31: 2006 Witczak **Modification** Coefficient Correlation Table .................................. 122

Table 32: Project Effect Calibration Parameters **for** the Modified 1999 Witczak Model .... 128

Table 33: RAS Content Calibration Parameters **for** the Modified 1999 Witczak Model ..... 128

Table 34: Project Effect Calibration Parameters **for** the Modified 2006 Witczak Model .... 129

Table 35: RAS Content Calibration Parameters **for** the Modified 2006 Witczak Model ..... 129

iii

Table 36: Project Effect Calibration Parameters **for** the Modified Hirsch Model ................ 130

Table 37: RAS Content Calibration Parameters **for** the Modified Hirsch Model................. 130

Table 38: **Dynamic** **Modulus** Test Results **for** Mix BC-21 ................................................... 135

Table 39: **Dynamic** **Modulus** Test Results **for** Mix BC-22 ................................................... 136

Table 40: **Dynamic** **Modulus** Test Results **for** Mix BC-23 ................................................... 137

Table 41: **Dynamic** **Modulus** Test Results **for** Mix BC-24 ................................................... 138

Table 42: **Dynamic** **Modulus** Test Results **for** Mix BC-25 ................................................... 139

Table 43: **Dynamic** **Modulus** Test Results **for** Mix BC-26 ................................................... 140

Table 44: **Dynamic** **Modulus** Test Results **for** Mix BC-27 ................................................... 141

Table 45: **Dynamic** **Modulus** Test Results **for** Mix BC-28 ................................................... 142

Table 46: **Dynamic** **Modulus** Test Results **for** Mix BC-29 ................................................... 143

Table 47: **Dynamic** **Modulus** Test Results **for** Mix BC-30 ................................................... 144

Table 48: **Dynamic** **Modulus** Test Results **for** Mix BC-31 ................................................... 145

Table 49: **Dynamic** **Modulus** Test Results **for** Mix BC-32 ................................................... 146

Table 50: **Dynamic** **Modulus** Test Results **for** Mix BC-33 ................................................... 147

Table 51: DSR Test Results .................................................................................................. 148

Table 52: DSR Frequency Sweep Test Results **for** Mixes BC-21, 23, 24, and 25 ............... 150

Table 53: DSR Frequency Sweep Test Results **for** Mixes BC-27, 28, 29, and 30 ............... 152

Table 54: DSR Frequency Sweep Test Results **for** Mixes BC-31, 32, and 33 ..................... 154

iv

LIST OF FIGURES

Figure 1: States in the United States Allowing Using **of** RAS [7].......................................... 11

Figure 2: Stress and Strain **of** Typical Viscoelastic Material under Sinusoidal Loading ....... 21

Figure 3: Master Curve Construction ..................................................................................... 24

Figure 4: Schematic Representation **of** Hirsch Model and Four Modified Versions [10] ...... 28

Figure 5: Master Curve Comparison **for** Cell 21 [29] ............................................................. 31

Figure 6: Master Curve Comparison **for** Cell 33 [29] ............................................................. 32

Figure 7: Master Curve Comparison **for** Cell 34 [29] ............................................................. 32

Figure 8: Master Curve Comparison **for** Cell 35 [29] ............................................................. 33

Figure 9: Summary **of** Percent Error in **Dynamic** Moduli **for** Witczak’s Prediction [30] ...... 34

Figure 10: Summary **of** Percent Error in **Dynamic** Moduli **for** Hirsch’s Prediction [30] ....... 34

Figure 11: Predicted and Measured E* Values [10] ............................................................... 35

Figure 12: Measured Values vs. Predicted Values **of** **Dynamic** **Modulus** on log-log Scale

(RTFO Condition, Viscosity from Brookfield Test) [31] ................................................. 36

Figure 13: Measured Values vs. Predicted Values **of** **Dynamic** **Modulus** on log-log Scale

(RTFO Condition, Viscosity from DSR Test) [31] .......................................................... 36

Figure 14: Measured Values vs. Predicted Values **of** **Dynamic** **Modulus** on log-log Scale

(Mix/Laydown condition) [31] ......................................................................................... 37

Figure 15: Comparison **of** Values Using the Witczak **Predictive** Equation [32] .................... 38

Figure 16: Comparison **of** Values Using the Hirsch Model [32] ............................................ 38

Figure 17: Comparison **of** Values Using the Witczak **Predictive** Equation [32] .................... 39

Figure 18: Comparison **of** Values Using the Hirsch Model [32] ............................................ 39

Figure 19: Plan View **of** MnROAD Test Cells [35] ............................................................... 44

Figure 20: Aggregate Gradation 0.45 Power Chart **for** Minnesota Demonstration Project

Gradations ......................................................................................................................... 45

Figure 21: RAS Content and Virgin Binder Replacement **for** Iowa Demonstration Project

Test Sections ..................................................................................................................... 46

Figure 22: Plan View **of** Iowa Demonstration Project Test Sections [35] .............................. 47

Figure 23: Aggregate Gradation 0.45 Power Chart **for** Iowa Demonstration Project ............ 48

Figure 24: Plan View **of** Missouri Demonstration Project Test Sections [35] ....................... 49

Figure 25: Aggregate Gradation 0.45 Power Chart **for** Missouri Demonstration Project ...... 50

Figure 26: Plan View **of** Indiana Demonstration Project Test Sections [35] .......................... 51

Figure 27: Aggregate Gradation 0.45 Power Chart **for** Indiana Demonstration Project ........ 52

Figure 28: Universal Testing Machine and Environmental Chamber .................................... 54

Figure 29: AR1500 **Dynamic** Shear Rheometer ..................................................................... 55

Figure 30: Lab Tested vs. Witczak Model (1999) Predicted E* Values on Normal Scale ..... 59

Figure 31: Lab Tested vs. Witczak Model (1999) Predicted E* Values on Logarithm Scale 59

Figure 32: Lab Tested vs. Witczak Model (2006) Predicted E* Values on Normal Scale ..... 60

Figure 33: Lab Tested vs. Witczak Model (2006) Predicted E* Values on Logarithm Scale 61

Figure 34: Lab Tested vs. Hirsch Model Predicted E* Values on Normal Scale ................... 62

Figure 35: Lab Tested vs. Hirsch Model Predicted E* Values on Logarithm Scale .............. 62

Figure 36: VTS Curves **of** Recovered **Asphalt** Binder ........................................................... 71

Figure 37: Lab Tested G* Values **of** **Asphalt** Binder Recovered from Iowa 0% RAS Mix ... 72

v

Figure 38: G* Master Curve **for** **Asphalt** Binder Recovered from Iowa 0% RAS Mix

(Reference Temperature is 37ºC ) ...................................................................................... 72

Figure 39: Shift Factors **for** Mix BC-25 ................................................................................. 73

Figure 40: Phase Angle Master Curves **for** **Asphalt** Binder Recovered from Iowa 0% RAS

Mix .................................................................................................................................... 74

Figure 41: Lab Tested vs. 1999 Witczak Model Predicted E* Values Calibrated **for** 0%-RAS-

Effect on Logarithm Scale ................................................................................................ 81

Figure 42: Lab Tested vs. the 1999 Witczak Model Predicted E* Values Calibrated **for** 0%-

RAS-Effect on Normal Scale ............................................................................................ 81

Figure 43: Lab Tested vs. the 2006 Witczak Model Predicted E* Values Calibrated **for** 0%-

RAS-Effect on Logarithm Scale ....................................................................................... 82

Figure 44: Lab Tested vs. the 2006 Witczak Model Predicted E* Values Calibrated **for** 0%-

RAS-Effect on Normal Scale ............................................................................................ 82

Figure 45: Lab Tested vs. Modified 1999 Witczak Model Predicted E* Values on Logarithm

Scale .................................................................................................................................. 83

Figure 46: Lab Tested vs. Modified 1999 Witczak Model Predicted E* Values on Normal

Scale .................................................................................................................................. 84

Figure 47: Lab Tested vs. Modified 2006 Witczak Model Predicted E* Values on Logarithm

Scale .................................................................................................................................. 84

Figure 48: Lab Tested vs. Modified 2006 Witczak Model Predicted E* Values on Normal

Scale .................................................................................................................................. 85

Figure 49: Lab Tested vs. Hirsch Predicted E* Values Calibrated **for** 0%-RAS-Effect ........ 91

Figure 50: Lab Tested vs. Predicted E* Values **of** Modified Hirsch Model........................... 93

Figure 51: Witczak Model Master Curves **for** Minnesota 5% Mfr. RAS Mix (Mix BC21) .. 95

Figure 52: Witczak Model Master Curves **for** Minnesota 5% Tear-**of**f RAS Mix (Mix BC22)

........................................................................................................................................... 96

Figure 53: Witczak Model Master Curves **for** Iowa 4% RAS Mix (Mix BC25) .................... 96

Figure 54: Witczak Model Master Curves **for** Iowa 5% RAS Mix (Mix BC26) .................... 97

Figure 55: Witczak Model Master Curves **for** Iowa 6% RAS Mix (Mix BC27) .................... 97

Figure 56: Witczak Model Master Curves **for** Missouri 5% Fine RAS Mix (Mix BC29) ..... 98

Figure 57: Witczak Model Master Curves **for** Missouri 5% Coarse RAS Mix (Mix BC30) . 98

Figure 58: Witczak Model Master Curves **for** Indiana 3% RAS&HMA Mix (Mix BC32) ... 99

Figure 59: Witczak Model Master Curves **for** Indiana 3% RAS&WMA Mix (Mix BC33) .. 99

Figure 60: Lab E* vs. Predicted E* **of** Witczak 1999 Model ............................................... 102

Figure 61: Lab E* vs. Predicted E* **of** Witczak 2006 Model ............................................... 105

Figure 62: Hirsch Model Master Curves **for** Mix BC21 ....................................................... 107

Figure 63: Hirsch Model Master Curves **for** Mix BC25 ....................................................... 107

Figure 64: Hirsch Model Master Curves **for** Mix BC27 ....................................................... 108

Figure 65: Hirsch Model Master Curves **for** Mix BC29 ....................................................... 108

Figure 66: Hirsch Model Master Curves **for** Mix BC30 ....................................................... 109

Figure 67: Hirsch Model Master Curves **for** Mix BC32 ....................................................... 109

Figure 68: Hirsch Model Master Curves **for** Mix BC33 ....................................................... 110

Figure 69: Lab E* vs. Predicted E* **of** Hirsch Model ........................................................... 113

Figure 70: δ Calibration Coefficient **for** the 1999 Witczak Model ....................................... 114

Figure 71: α Calibration Coefficient **for** the 1999 Witczak Model ....................................... 115

vi

Figure 72: b Calibration Coefficient **for** the 1999 Witczak Model ....................................... 115

Figure 73: g 1 Calibration Coefficient **for** the 1999 Witczak Model ..................................... 116

Figure 74: g 2 Calibration Coefficient **for** the 1999 Witczak Model ..................................... 116

Figure 75: δ Calibration Coefficient **for** the 2006 Witczak Model ....................................... 119

Figure 76: α Calibration Coefficient **for** the 2006 Witczak Model ....................................... 120

Figure 77: b Calibration Coefficient **for** the 2006 Witczak Model ....................................... 120

Figure 78: g 1 Calibration Coefficient **for** the 2006 Witczak Model ..................................... 121

Figure 79: g 2 Calibration Coefficient **for** the 2006 Witczak Model ..................................... 121

Figure 80: p 0 Calibration Coefficient **for** the Hirsch Model ................................................. 123

Figure 81: p 1 Calibration Coefficient **for** the Hirsch Model ................................................. 123

Figure 82: p 2 Calibration Coefficient **for** the Hirsch Model ................................................. 124

vii

ACKNOLEDGEMENTS

I would like to express my gratitude to all those who helped me during the writing **of** this

thesis.

My deepest gratitude goes first and **for**emost to my advisor Dr. Chris Williams **for** his

support, guidance, and leadership throughout the course **of** my graduate studies and this

research.

I gratefully acknowledge the help **of** Dr. Stephenson, who has **of**fered me valuable

suggestions in statistical analysis.

I would also like to thank Dr. Schaefer **for** his assistance in my academic studies and

being part **of** my advisory committee.

I would additionally like to thank Debra Haugen and Andrew Cascione who provided

valuable in**for**mation to help me complete this research.

Last but not least, I would like to thank my family **for** their continuous support and

encouragement. I own much to my parents who provided great support and understanding

even though they were in a difficult time. This thesis would not have been possible without

their helps.

viii

ABSTRACT

Recycled asphalt shingles (RAS) have been used in road pavement construction **for** a

number **of** years primarily on low volume roads. The use **of** RAS represents economic and

environmental opportunities as it provides as good or better per**for**mance when processed and

proportioned appropriately than commonly used asphalt mixtures. The primary components

**of** RAS are asphalt, mineral filler, mineral granules, and felt. The effect **of** RAS fibers on an

asphalt mixture’s dynamic modulus, which is a key input in the Mechanistic-Empirical

Pavement Design Guide (MEPDG) and one **of** the critical properties **of** asphalt mixtures

affecting flexible pavement responses that are related to its per**for**mance, are still uncertain.

The National Pooled Fund Study #1208 conducted a series **of** researches to investigate

various issues related to RAS utilization. Thirteen mix designs with RAS contents ranging

from zero to six percent were developed and constructed in Indiana, Iowa, Minnesota, and

Missouri. Field produced mixtures were procured and sent to Iowa State University **Asphalt**

Lab **for** laboratory dynamic modulus tests. The testing results are used to evaluate two

commonly used dynamic modulus predictive models, the Witczak and Hirsch models. Two

versions **of** Witczak models, which were developed in 1999 and 2006, are evaluated in this

research. It was found that the Witczak models were not very effective in estimating the

modulus values **of** RAS mixtures and thus modifications were made to the models to account

**for** the effects **of** RAS. The study did determine out that the commonly used dosage **of** RAS

in asphalt mixtures does not affect the prediction accuracy **of** the Hirsch model, however

updates were made to improve the Witczak model’s accuracy.

ix

CHAPTER 1: INTRODUCTION

BACKGROUND

Environmental and economic concerns are important components in decision making

processes **of** infrastructure construction projects. With the fact that the global crude petroleum

price has increased rapidly in the past decade, liquid asphalt price has grown dramatically and is

more than $500/ton in 2010 [1]. As a product derived from petroleum distillation, asphalt is

becoming less available and more expensive because the crude petroleum is being used to

produce other products and restricted supply. Pavement engineers have been considering

substitutions **of** virgin asphalt **for** the past few years. Recycling **of** wasted materials such as

recycled asphalt pavement (RAP) and recycled asphalt shingles (RAS) provide possible solutions

to address this issue. These recycled materials can be used in roadway construction in order to

reduce the dependence on virgin asphalt binder.

RAS has been utilized in road paving practices **for** over 20 years. In the early 1990s, hot mix

asphalt (HMA) pavements containing RAS were experimentally used in the State **of**

Pennsylvania. A 0.93 mile four-lane highway was constructed with mix containing 5 percent

RAS in July, 1991 which is the first road paved with RAS [2]. In the same year, the Minnesota

Department **of** Transportation (Mn/DOT), the Minnesota Office **of** Environmental Assistance

(OEA), and the University **of** Minnesota started a research project to investigate the effectiveness

**of** pavements containing RAS and the influences **of** shingle products on mix properties. This

study recommended a maximum RAS content **of** 5 percent to be used. This recommendation was

legislated as a state specification in 1995[3]. Disney World in Orlando, Florida, built its parking

lots with a high RAS content **of** 10 percent in the early 1990s. This pavement has per**for**med very

well **for** the past 20 years [4]. RAS can be recycled from either manufacturer’s scrap or building

rero**of**ing process. Materials from manufacturer’s scrap are known as pre-consumer shingles or

manufacturer’s shingles. Materials from rero**of**ing projects are known as post-consumer or tear**of**f

shingles. It is estimated that approximately 1 million tons **of** pre-consumer shingles and 10

million tons **of** post-consumer shingles are generated in the United States every year [5]. Most **of**

them are deposited into landfills. Environmental issues related to this are considerable and

become one **of** the motivations **of** utilization **of** recycled shingles in pavement construction.

Some state agencies have allowed RAS to be used with certain maximum percentages in HMA.

10

Most states agencies limit the use **of** RAS to 5% by weight **of** the total aggregate. Figure 1 shows

the states that currently allow the utilization **of** RAS in HMA. In a 2011 supplemental

specification, the State **of** Ohio allows the use **of** either manufacturer’s RAS or tear-**of**f RAS

depending on the particular pavement courses [6]. It should be noticed that the Ohio only allows

the using **of** manufactured RAS in Figure 1.

Figure 1: States in the United States Allowing Using **of** RAS [7]

**Dynamic** complex modulus (E * ) is a measure **of** the stiffness **of** viscoelastic materials. It is

one **of** the most important HMA properties which are used to examine pavement responses such

as stress, strain, and deflection in the Mechanistic-Empirical Pavement Design Guide (MEPDG).

The MEPDG is a pavement design and per**for**mance predicting method developed by the

National Cooperative Highway Research Program (NCHRP) in 2002 to address shortcomings in

current pavement design methods [8]. The MEPDG uses mechanical principles to calculate

a**for**ementioned pavement responses. Empirical models are used to predict pavement

per**for**mance from the pavement responses. There are many E* predictive models developed by

various empirical and mechanical methods such as statistical regression, artificial neural

networks, ultrasonic direct test method, and so on. The Witczak and Hirsch models are the most

11

well-known procedures among them. The Witczak Model is an empirical model developed by

Matthew W. Witczak in 1972 [9]. Revisions were made to the model in 1995, 1999, and 2006.

The model is based on a sigmoidal function which is used to describe the relationship between

the dynamic modulus and loading rate. Aggregate gradation, volumetric properties **of** mixtures,

and binder rheological properties are addressed in the Witczak Model. The Hirsch Model was

developed by Y.J. Hirsch in the 1960s [10]. The Hirsch Model is a semi-empirical model based

on the law **of** mixture. There are several versions **of** the Hirsch Model. Christensen, Pellinen, and

Bonaquist conducted research in 2003 that evaluates various Hirsch models and recommends the

most effective model to be used.

PROBLEM STATEMENT

The MEPDG was adopted as a pavement design guide by the American Association **of** State

Highway and Transportation Officials (AASHTO) in April, 2011. With the promoted

implementation **of** the MEPDG design procedures, pavement engineers’ interest in a quick, easy,

and accurate method **of** obtaining dynamic modulus value are increasing. Laboratory dynamic

modulus testing is usually conducted to obtain the E* value directly from a subject mix.

However, the testing requires a series **of** expensive sampling and testing equipment, experienced

lab personnel, and a relative long waiting time be**for**e knowing the results. The E* predictive

models were developed as an alternative method **of** obtaining the dynamic modulus values. The

E* values can be easily calculated from other basic properties **of** aggregate, binder, and mixture

without a specifically designed E* experiment. The predictive models do not require any lab

equipment and the values can be estimated instantly. However, there are many factors that can

affect the dynamic modulus **of** mixes and are not addressed in the E* predictive models. When

these factors come into effect, the predicting accuracies **of** the models will decrease. RAS is one

**of** the factors that are not addressed by the Witczak and Hirsch Model. The research is motivated

by the needs **of** a reliable E* predictive method **for** mixes containing RAS.

OBJECTIVES

The demonstration projects **for** National Pooled Fund Study 1208 that were constructed in

the Summers **of** 2008, 2009, and 2010 are contained in this thesis. The objective **of** the pooled

fund study is investigating issues related to the use **of** RAS including effects on laboratory

testing properties and field per**for**mance in different scenarios as well as issues in processing,

12

transportation, and storage **of** RAS. Mix designs **for** each demonstration project were developed

individually **for** specific objectives. The Indiana demonstration project was developed to

investigate different effects **of** RAS on HMA and warm mix asphalt using foaming technology.

The demonstration project in Iowa was designed to study the influences **of** RAS content on

per**for**mance. The Minnesota demonstration project was constructed **for** the purpose **of**

comparing the effects **of** manufactured RAS and tear-**of**f RAS. The Missouri DOT constructed

the demonstration project to study the effects **of** RAS grind size. Various laboratory tests were

per**for**med to fulfill the objectives listed above. Some **of** the testing results are drawn to complete

the following objectives **for** this research:

Evaluate the predictive accuracies **of** the 1999 and 2006 Witczak **Models**, and the

Hirsch Model;

Identify factors that affect the predictive accuracies **of** the E* models;

Examine if the E* predictive models need to be calibrated to account **for** the effects **of**

RAS;

Develop modified E* predictive models as needed; and

Evaluate the effectiveness **of** the modified models.

METHODOLOGY

The mix designs were developed by SUPERPAVE design procedures. The testing materials

were produced in the field and sampled randomly. Laboratory tests were conducted by following

the corresponding ASTM and/or AASHTO standards. The dynamic modulus values were tested

in the laboratory. The input parameters in the E* predictive models were collected from QA/QC

reports, lab testing results, and mix designs. Statistical analyses including Analysis **of** Variance

(ANOVA) and Student’s t-test were per**for**med to identify significant factors affecting the model

accuracy and comparing multiple levels **of** significant factors. A non-linear regression approach

based on the least square method was used to develop the modified models. The effectiveness **of**

a model is evaluated by its goodness-**of**-fit and differences in master curves between the

predicted E* values and the lab results.

ORGANIZATION

This thesis is divided into five chapters including the introduction (Chapter 1), literature

review (Chapter 2), experimental plan (Chapter 3), evaluation and modification **of** the Witczak

13

and Hirsch **Models** (Chapter 4), and conclusions and recommendations (Chapter 5). Chapter 1

provides brief descriptions **of** the background, addressed issues, objectives, and methodology.

Chapter 2 discusses previous studies that have been conducted on recycled asphalt shingles,

dynamic modulus, and the Witczak and Hirsch E* predictive models. Chapter 3 outlines the

experimental plan and testing procedures. Chapter 4 summarizes the results **of** evaluations **for** the

original and modified E* predictive models as well as a detailed description **of** the modeling

process. Chapter 5 states the conclusions **of** the study and provides recommendations **for** future

research.

14

CHAPTER 2: LITERATURE REVIEW

ASPHALT SHINGLES

**Asphalt** shingles are the most widely used material **for** building ro**of**s. Compared to other

ro**of**ing materials, such as wood shakes, metal, concrete, or clay, asphalt shingles are less

expensive and easier to install and replace. **Asphalt** shingles are typically classified into two

types, organic and fiberglass, depending upon the materials used to produce the base felt. The

base felts **for** organic asphalt shingles are made from cellulosic fibers from woods or paper

wastes. The fiberglass shingles use fiberglass as the primary component **of** their base felts. The

manufacturing processes **for** both organic and fiberglass shingles are very similar. Firstly, felts

are saturated with liquid asphalt. Secondly, additional asphalt layers are attached to cover both

sides **of** the felts in order to make them waterpro**of**. Finally, shingles are surfaced with mineral

granules. Powdered limestone is usually added to asphalts as mineral stabilizer. Fibers can be

used as fibrous stabilizer in fiberglass asphalt shingles. The purposes **of** adding stabilizers to

shingles are to improve their fire resistance and weatherability. The procedures **for** producing

organic and fiberglass asphalt shingles are specified in ASTM D225 and ASTM D3462 [11].

**Asphalt**s used in producing shingles are stiffer and more viscous than the virgin asphalts that are

commonly used in road pavements. An “air-blown” process is applied to prepare the asphalts **for**

shingles. Air is injected into oxidizer with petroleum residue which was preheated to 400 °F (204

°C) at a constant rate **of** 0.008 to 0.026 m 3 /sec/Mg. Oxygen reacts with asphalt molecules

causing increase in the apparent molecular weight. The oxidization process increases the

asphalt’s s**of**tening point and viscosity while decreasing its penetration [12].

Shingles typically consist **of** asphalt binder, aggregate, and fibers. The proportion **of** each

component varies with shingle type and manufacturer. The most valuable component **of** shingles

is asphalt. In general, organic shingles have higher asphalt contents and lower fiber contents

compared to fiberglass shingles. Post-consumer shingles from rero**of**ing construction contain

more asphalt than pre-consumer shingles, due to weathering caused loss **of** surface granules. The

largest component **of** shingles is aggregate including the ceramic granules, headlap granules,

backsurfacer sand, and the stabilizer. Aggregates contained in shingles are very fine aggregates

that pass the No.12 (1.7mm) sieve [12]. The typical shingle compositions are summarized in

15

Table 1. The percentages in Table 1 are based on total weight **of** shingle products. The shingle

aggregate compositions and particle sizes are presented in Table 2.

Table 1: Typical Shingle Composition [11]

Material Organic Shingles Fiberglass Shingles

**Asphalt** Binder 30-35% 15-20%

Aggregate 30-50% 30-50%

Fibers/Mineral Fines 15-35% 20-35%

Table 2: Shingle Aggregate Compositions and Size [11]

Component

Typical Quantity

percent by weight **of**

sample

Typical Size

Ceramic Granules 10-20%

passing No.12

retained No.40

Headlap Granules 15-25% Same as above

Backsurfacer Sand 5-10%

passing No.40

retained No.140

Stabilizer 15-30%

90% passing No.100

70% passing No.200

Shingle Recycling

Ro**of**ing waste can contain 10 to 15% (by weight) extraneous matters other than asphalt

shingles, such as metal flashing, wood sheathing, paper, and nails [13]. Shingle wastes from

manufacturers are relatively pure, whereas, Tear-**of**f shingles must be cleaned be**for**e further

processing. Debris in tear-**of**f shingles can be cleaned by manual or mechanical separations [14].

Asbestos containing materials (ACM) are strictly controlled due to the hazard to worker health.

Federal law requires ACM in recycled materials do not exceed 1% by weight [15]. Both tear-**of**f

shingles and manufacturer’s scrap have to be reduced into finer particles. Finer processed

shingles are easier to transport and mix with asphalt mixtures. Georgia DOT requires all shingle

scraps to pass the 12.5mm (1/2”) sieve [16]. The Texas DOT requires 95% **of** shingle scraps to

pass 1/2” sieve. In most current practices, shingles are reduced to less than 1/2”. Processed

asphalt shingles are recommended to use in a short range **of** time due to the storage and handling

difficulties. Large clumps **of** asphalt can **for**m and cause transportation and mixing problems,

because shingle stockpiles can consolidate with time. Fine aggregate can be added to processed

16

shingles to alleviate the **for**mation **of** asphalt clumps. This could reduce the asphalt content **of**

processed shingles and has to be taken into account during mix design calculations [17].

Previous Researches and Practices **of** RAS Utilization

Early RAS research focused on studying pre-consumer asphalt shingles. Many state agencies

historically allowed only pre-consumer shingles to be used. In recent years, the research focus

has shifted to post-consumer asphalt shingles because **of** the increased pricing **of** asphalt. The

combination **of** RAS and RAP were studied in several recent research projects.

Minnesota’s Shingle Scrap Research [3]

A report prepared **for** the Minnesota Department **of** Transportation in October, 1996 studied

the properties and per**for**mance **of** asphalt containing RAS pavements. In early the 1990s, three

test sections were built on the Willard Munger recreational trail, Highway T.H.25 at south **of**

Mayer and Highway 17 at Scott County respectively. Only pre-consumer RAS were studied in

this research. Pavement conditions after 4 to 6 years from the completion **of** projects showed

RAS content up to 7% by aggregate weight would not adversely impact pavement per**for**mance.

Laboratory tests indicated the asphalt penetration at 77 °F **of** recovered binder containing RAS

were less than those **of** binder without RAS. However, the stiffness increase **of** the asphalt binder

due to RAS did not lead to significant low-temperature cracking problems. The Willard Munger

recreational trail also included a test section containing recycled rubbers. A severe raveling issue

was found **for** the rubber section.

Mn/DOT RAS/RAP Research [18]

A comprehensive research funded by the Minnesota Department **of** Transportation studied

the effects **of** RAP and RAS on mixture lab testing results and field per**for**mance. Shingles

studied in this research include both manufacturer’s scrap and tear-**of**f shingles. Mixture testing

samples were made from lab produced mixes. Three or five percent RAS were added with 0%,

15%, 25%, and 30% RAP to make the mixtures **for** lab testing. Mixtures that contained RAP

alone were also tested. Materials **for** binder testing were extracted from mixtures through a

solvent centrifuge process described in ASTM D5404. Six field projects were observed to

compare the pavement per**for**mance via resistance to different types **of** cracking and pavement

permanent de**for**mation. The following findings were found:

17

The binder grading results showed both high and low temperature per**for**mance

grades increased as the virgin to total binder ratio decreased. This correlation has R 2

value **of** 0.77 **for** the low temperature grade and 0.88 **for** the high temperature grade,

respectively. Binders extracted from mixtures that contained tear-**of**f shingles were

found to be stiffer than binders from mixtures that contain manufacturer’s scrap. The

stiffness difference between tear-**of**f shingles and manufacturer’s scrap is larger **for**

higher RAP contents.

For 5% RAS content, the | | values **for** samples containing tear-**of**f shingles are

higher than those **for** samples containing manufacturer’s scrap at the high frequency

end **of** master curves. At the low frequency end, the differences between the two

types **of** shingles are not obvious. For 3% RAS content, the difference between tear**of**f

shingles and manufacturer’s scrap is limited. **Dynamic** modulus test results also

showed the virgin to total asphalt content–stiffness correlation was valid at a high

temperature (100 °F).

**Asphalt** Pavement Analyzer (APA) results indicated that pavement with recycled

materials tended to have less rutting,

Moisture sensitivity test (Lottman) results indicated that RAS and RAP increased

pavement moisture sensitivity which could potentially increase the risk **of** moisture

damage cracking.

Comparisons between laboratory and field produced mixtures showed that asphalt

mixtures prepared in the lab exhibited a higher stiffness than those prepared in the

field.

Pavement condition survey results indicated that the pavement per**for**mance **of** mixes

containing tear-**of**f shingles and manufacturer’s scrap contained pavement are very

similar.

Laboratory Evaluation **of** Post-consumer RAS Contained HMA Mixture [19]

A conference paper prepared **for** the Association **of** **Asphalt** Paving Technologists (AAPT)

2011 annual meeting evaluated the influences **of** post-consumer RAS on various lab tests results.

The binder and mixture materials were from an Illinois Tollway project on I-90 west **of** Chicago.

The evaluated lab tests include DSR and bending beam rheometer (BBR) test **for** asphalt binders;

as well as dynamic modulus, beam fatigue, and disc shaped compact tension (DCT) testing **for**

18

asphalt mixtures. In this project, RAS was used in combination with fractionated recycled

asphalt pavement (FRAP). Eight mix designs with total recycled material content from 25% to

50% were developed. Mixes with 5% RAS were compared to the mixes with the same amount **of**

recycled material but containing 0% RAS. Lab results indicated the RAS increases asphalt binder

stiffness. The stiffening effect was significant when lower FRAP contents were used. Binder

high temperature per**for**mance grades were increased by adding 5% RAS to mixtures with total

recycled materials less than 40%.For recycled materials more than 40%, the stiffening effect **of**

RAS is not obvious. **Dynamic** modulus test results showed the mixture high temperature | |

values increased as additional FRAP was added. No significant improvements **of** | | values

were observed **for** recycled material percentages higher than 40%.The paper also indicated that

the utilization **of** RAS and FRAP in asphalt pavement did not caused more fatigue damage.

Oregon State University RAP/RAS Study [20]

Oregon State University conducted a research project to investigate the effects **of** various

proportions **of** RAP and tear-**of**f shingles on binder high and low temperature grades. The report

was published in February, 2010. Seven mix designs were studied with 0% or 5% RAS and RAP

percentages ranging from 0% to 50% by the weight **of** total mixture. The study determined that

5% RAS alone increased the recovered binder high and low temperature per**for**mance grades.

Adding 10 to 30 percent RAP to mixes with 5% RAS could increase binder grades at both high

and low temperatures. However, additional RAP above 30% did not cause further improvements

**of** binder per**for**mance grades. The results agreed with the Cascione et al. study.

DYNAMIC MODULUS

**Dynamic** modulus, E*, is the absolute value **of** the complex dynamic modulus, which is the

stress-to-strain ratio **of** linear viscoelastic materials under a continuous sinusoidal loading. It can

be computed as the amplitude **of** the sinusoidal stress divided by the maximum recoverable

strain:

| |

Equation 1

where | |

dynamic modulus,

19

maximum stress, and

maximum strain

When the strain is at a small level which is less than 100 micro-strain (με), the asphalt stressstrain

relationship is considered linear viscoelastic [21]. For linear viscoelastic materials,

material responses are time dependent. The corresponding strain occurs a period **of** time after a

load is applied. The time lag is defined as the phase angle (Φ). For perfectly elastic materials, Φ

equals to 0; and **for** perfect viscous materials, Φ equals to 1. The phase angle can be calculated

by Equation 2 [22]:

Equation 2

where

phase angle,

lag time between stress and strain cycles, and

time **of** one strain cycle.

Figure 2 demonstrates this process. The term “perfectly elastic” means material strain reacts

to stress instantaneously. In other words, the material achieves its maximum strain at exactly the

same time that the maximum stress is applied. The term “perfectly viscous” means the maximum

strain occurs at the same time the minimum stress is applied. For any given time, the material

stress to strain ratio is the complex dynamic modulus. The complex dynamic modulus can be

mathematically expressed by Equation 3 [23]:

where the parameters are defined previously.

Equation 3

20

Figure 2: Stress and Strain **of** Typical Viscoelastic Material under Sinusoidal Loading

The dynamic modulus is a measure **of** relative stiffness **for** viscoelastic materials. **Asphalt**

mixtures that have higher dynamic moduli tend to de**for**m less under a traffic loading than

mixtures with lower dynamic modulus. At high temperatures, less de**for**mation is related to better

resistance to rutting. At low temperatures, high dynamic modulus pavements achieve high

internal stresses which could result in greater susceptibility to low-temperature cracking.

**Dynamic** **Modulus** Testing

C**of**fman and Pagen at Ohio State University developed the first dynamic modulus protocol

in the 1960’s [22]. It was accepted as an ASTM standard in 1979. The designation is D3496 in

ASTM standards and TP62 in AASHTO specifications. The protocol came up with the idea **of**

testing the dynamic modulus **of** viscoelastic materials from a triaxial test under a uniaxial

sinusoidal stress. The stress could be either compressive or tensile; most dynamic tests were

conducted with compressive stresses. Shear stress can also be used to determine the dynamic

complex modulus **for** asphalt binders with a dynamic shear rheometer. The binder dynamic shear

complex modulus is denoted as G * ; the testing procedures are specified in AASHTO D7175,

standard test method **for** determining the rheological properties **of** asphalt binder using a

dynamic shear rheometer [24]. The binder dynamic modulus is assumed to be 3 times **of** the G *

based on experiences [10]. For mixture dynamic modulus testing, AASHTO specification

requires a servo-hydraulic testing machine to apply the sinusoidal loading. A Superpave

21

Gyratory Compactor (SGC) is used to compact

(height by diameter) asphalt

cylinder with air void content not exceeding from the specified target air void content. A

Testing specimen is cored and cut to

from the compacted asphalt specimen.

Sample axial de**for**mation is measured with linear variable differential trans**for**mers (LVDT).

Samples are **of**ten tested at several temperatures. At each temperature, dynamic moduli are taken

**for** multiple loading frequencies typically varying from 0.1Hz to 25Hz, in a strain controlled

mode **of** loading. Loading is adjusted to obtain 50 to 150με.The permanent de**for**mation **of**

specimen is **of**ten controlled to less than 1500με [25]. The testing results are generally presented

as master curves.

**Dynamic** **Modulus** Master Curve

**Asphalt** mixture dynamic modulus varies with temperature and loading frequency. The

comparisons **of** testing results are complicated, especially when the testing temperatures are

different. The dynamic modulus master curve provides a direct visual expression **of** dynamic

modulus results. Comparisons between two sets **of** dynamic modulus results can be possible

[26].The standard dynamic testing procedure elaborated by ASTM D3497 recommends using

three temperatures (5, 25, and 40ºC). At each temperature, | | values are tested at three

frequencies (1, 4, 16Hz). In order to develop more precise master curve, five temperatures (-9,

4.4, 21.1, 37.8, and 54.4ºC) with six frequencies (25, 10, 5, 1, 0.5, and 0.1Hz) at each

temperature are usually used **for** dynamic modulus testing. According to the research conducted

by Li and Williams [36], testing | | values at three temperatures (4.4, 21.1, and 37.8ºC) did not

change the shape **of** master curves constructed by data from the nine temperatures. In practice,

engineers are interested in pavement properties in the worst scenarios. The lowest temperatures

at most places **of** U.S. are far below the lab low temperature test. Master curve also provides

estimations **of** dynamic moduli out **of** the lab testing range. The 2002 NCHRP pavement design

guide uses asphalt dynamic moduli determined from master curves [27].

The| | master curve can be constructed at a reference temperature or frequency based on the

time-temperature superposition principle. **Asphalt** exhibits higher E* values at low temperatures

or high loading frequencies. There**for**e, an E* value tested at a lower temperature could equal to

an E* value tested at a higher temperature but at a lower frequency. There**for**e, E* values tested

at different temperatures and frequencies can be transferred to a single reference temperature or

22

frequency. Often times, dynamic modulus testing can be easily done at multiple frequencies.

Changing the test temperature is usually time consuming and thus costly. As a result, researchers

usually test dynamic modulus at few temperatures but many different frequencies. The transition

from frequency to temperature is much easier than from temperature to frequency. A number that

is used to equalize frequencies at different temperatures is called a shift factor, a(T). Equation 4

shows the mathematical definition **of** this shift factor:

where f r = reduced frequency (loading frequency at the reference temperature),

f = loading frequency, and

a(T) = shift factor.

Equation 4

The Shift factor is 1 at the reference temperature; and the log(a(T)) is there**for**e 0.The “2002

Guide **for** the Design **of** New and Rehabilitated Pavement Structures” uses a sigmoidal function

shown below to construct a master curve fitting line [27]:

| |

where | | dynamic modulus,

time **for** loading at the reference temperature (reduced time),

minimum modulus value,

maximum modulus value, and

parameters describing the shape **of** the sigmoidal function.

Equation 5

The parameters that are used to represent the master curve including

can be

solved by using Excel Solver Function to match the calculated E* values from the sigmoidal

function with the lab tested E* values. Figure 3 illustrates the shifting **of** E* values and

construction **of** master curve.

23

Figure 3: Master Curve Construction

Witczak E* **Predictive** Model

The early Witczak’s dynamic modulus predictive model was developed in 1972. The model

was based on non-linear polynomial regression **of** laboratory E* values. The early model was

established from 29 mixtures with 87 total data points. Several revisions were made ensuring

twenty years. The current MEPDG pavement design program uses the Witczak model developed

in 1999 **for** E* estimation. The 1999 Witczak model is developed from 205 laboratory mixtures

including 171 unmodified asphalt binders and 34 modified binders that produced 2750 data

points. The newest Witczak model was published in 2006 including 7400 data points from 346

HMA mixtures [9].

The 1999 Witczak model is the most widely used version **of** Witczak model because **of** the

application **of** the MEPDG program in pavement design. This model predicts E* values **of** HMA

mixtures from 8 input parameters that characterize aggregate gradation, asphalt binder behavior,

binder–aggregate interaction, and loading condition. An R 2 **of** 0.96 and Se/Sy **of** 0.24 were

observed **for** this model on a logarithm scale. The model is shown in Equation 6 [23]:

24

| |

( )

where | | dynamic modulus (psi),

bitumen viscosity (10 6 Poise),

loading frequency (Hz),

air void content (%),

effective bitumen content(% by volume),

cumulative % retained on the 19-mm (3/4inch) sieve,

cumulative % retained on the 9.5-mm (3/8inch) sieve,

cumulative % retained on the 4.75-mm (No.4) sieve, and

% passing the 0.075-mm (No.200) sieve.

Equation 6

Laboratory viscosity tests can only be done at high temperatures that allow asphalt binders to

flow. **Asphalt** binders at low temperatures are difficult to test directly. The viscosity-temperaturesusceptibility

(VTS) method allows estimation **of** asphalt’s viscosity at any temperature from lab

tested viscosities at several temperatures from laboratory testing can be easily done. It should be

noticed that this log-log to log linearity is only applicable **for** conventional type “S” asphalt

cement. There are several ways to obtain the laboratory viscosities. Viscosities can be tested

directly with the rotational viscometer by following ASTM D2983. The viscosities can be also

estimated from binder penetration test results and dynamic shear rehometor (DSR) test results.

The penetration–viscosity relation is expressed in Equation 7 [28]:

where

viscosity (Poise), and

penetration **for** 100 g, 5 seconds loading (0.1 mm).

25

Equation 7

The penetration viscosities were used prior to the DSR testing being available. This empirical

equation is developed from regression **of** 17 test sections with 766 data points. The R 2 value is

0.377 in normal scale and 0.927 in logarithm scale [23]. The Equation 8 is commonly used now

[9]:

| |

Equation 8

where viscosity (Poise),

| | asphalt binder shear modulus (Pa), and

asphalt binder phase angle.

One problem that is brought up regarding the 1999 Witczak model is that the binder stiffness

is characterized by viscosity which does not take into consideration **of** the effects **of** loading

frequency. Frequency is treated as another independent input variable in the predictive equation.

However, binder viscosity is frequency dependent. Changes in loading frequencies also induce

viscosity changes **of** the binder. The scenario intimated by the 1999 Witczak model that binder

viscosity can remain the same while loading frequency varies may never happen in reality. This

contradiction was addressed and modified by the 2006 Witczak model which uses the dynamic

shear complex modulus (| |), and phase angle ( ), from DSR tests instead **of** viscosity to

characterize binder stiffness. The G* values at each temperature and loading frequency and the

corresponding values can be estimated by constructing a master curve based on asphalt binder

DSR results. The 2006 Witczak predictive equation is expressed in Equation 9 [9]:

(| | )

(

( ))

( )

| |

Equation 9

26

where dynamic modulus (psi),

aggregates (by weight **of** the total aggregates) passing through no. 200 sieve (%),

cumulative aggregates (by aggregates weight) retained on no. 4 sieve (%),

cumulative aggregates (by aggregates weight) retained on the 3/8” sieve (%),

cumulative aggregates (by aggregates weight) retained on the 3/4” sieve (%),

air voids (by volume **of** the mix) (%),

effective binder content (by volume **of** the mix) (%),

| | dynamic shear modulus **of** binder (psi), and

phase angle **of** binder associated with | | (degree).

Hirsch E* **Predictive** Model

The Hirsch dynamic modulus predictive model is a semi-empirical method based on various

modified law **of** mixtures developed by Y.J. Hirsch in the 1960s. There are two versions **of** the

law **of** mixtures presented in Equations 10 and 11 [10]:

⁄ ⁄ ⁄

Equation 10

Equation 11

Where E c is the composite material property, v 1 and v 2 are the volume fractions **of** component

phase 1 and 2 **of** the composite material, respectively, and E 1 and E 2 are the material properties **of**

component phase 1 and 2, respectively. The principle **of** the law is that a composite material

property can be treated as a combination **of** the properties **of** its components. The influence **of**

each component is proportional to its volume fraction. Phases **of** composite material can be

arranged either in parallel, or series, or even a combination **of** both. The Hirsch model uses the

combined arrangement **of** phases. The schematic expression **of** Hirsch model is shown in Figure

4 (a). Figure 4 also shows some important the variations **of** the Hirsch model.

27

V 1S

V 2S

Va ’

Vc Vv V

m

V 1P V 2P

(b) Series Version

(a) Hirsch model

Va ’

Vc

Vv

Vm

Vc Vv Va’,V

m

(c) Parallel Version

(d) Dispersed Version

Va’s

Va’p Vmp Vvp

Vms

Vvs

(e) Alternate Version

Figure 4: Schematic Representation **of** Hirsch Model and Four Modified Versions [10]

In Figure 4, Va’ is the volume fraction **of** aggregate excluding the contact volume and

mineral filler, Vc is the aggregate contact volume, Vv is the volume fraction **of** air voids, and

Vm is the mastic volume. The subscripts “p” and “s” refer to the arrangement type “parallel” and

“series”, respectively. Christensen, Pellinen, and Bonaquist did evaluations on various versions

**of** Hirsch model and found out the alternate version in Figure 4(e) was the most accurate model.

The alternate version **of** Hirsch model can be mathematically represented as Equation 12 [10]:

Equation 12

where Ec = modulus **of** asphalt mixture,

Ea = aggregate modulus,

Em = mastic modulus, and

28

Pc = aggregate contact volume fraction.

Other parameters are as defined be**for**e. The aggregate contact volume can be calculated by

Equation 13 [10]:

where VMA’= voids in the mineral aggregate,

VFM = voids filled with mastic, and

P 0 , P 1 , and P 2 = empirically determined constants

Equation 13

Several Hirsch model equations were constructed and evaluated by Christensen and his

colleagues. The final model **for** predicting mixture dynamic modulus is presented by the

following functions [10]:

| | [ ( ) | | ( )]

| |

| |

Equation 14

| |

where

parameters are defined previously.

Equation 15

In Equation 14, the term VFA which is the volume **of** voids filled by asphalt is equivalent to

VFM in Equation 15. The dynamic modulus **of** the asphalt binder is considered 3 times binder

shear modulus (| | ). The aggregate modulus is estimated as 4,200,000 psi with standard

error **of** 6.5%. The unit **of** predicted mixture dynamic modulus (| | ) is pounds per square

inch.

29

Previous Evaluation **of** the Witczak and Hirsch E * **Predictive** **Models**

This section contains the main findings **of** several studies on accuracies **of** the Witczak and

Hirsch dynamic modulus predictive models. Many researchers have compared the efficiencies **of**

Witczak and Hirsch models. Pavement projects studied cover the majority **of** the United States

climate regions. An overseas project from Argentina is also included.

University **of** Minnesota Study [29]

Clyne, Li, Marasteanu, and Skok from the University **of** Minnesota tested the dynamic

complex modulus and phase angle **of** asphalt mixtures from Mn/ROAD test cells. Mixtures from

cells 33, 34, and 35 at Mn/ROAD used the same mix design with different types **of** asphalt.

Sample cylinders **for** cells 33, 34, and 35 were made by field produced loose mixes. Cores were

taken at cell 21 which was paved 6 years be**for**e the other cells and there**for**e loose mix was not

available. This project also included two polymer modified asphalts. Table 3 summarizes the

source material properties and Table 4 summarizes the mixture gradations.

Table 3: Material Properties [29]

Cell 21 33 34 35

Binder 120/150 PG 58-28 PG 58-34 PG 58-40

Type

Polymer No No Yes Yes

Modified?

Sample Core Loose Mix Loose Mix Loose Mix

Type

Paving Date 07-1993 08-1999 08-1999 08-1999

30

Sieve Size,

mm

Table 4: Mixture Gradation [29]

Percent Passing

Cell 21 Cell 33 Cell 34 Cell 35

Sieve Size,

in.

19 3/4 100 100 100 100

16 5/8 99

12.5 1/2 96 94 94 94

9.0 3/8 88 86 86 86

4.75 #4 70 66 66 66

2.36 #8 54 54 54

2.0 #10 58

1.0 #20 44

0.45 #40 26

0.25 #80 9

0.0075 #200 4.3 4.7 4.7 4.7

Figure 5 through Figure 8 show master curves constructed based on the laboratory dynamic

modulus results and the 1995 and 2000 Witczak’s predictive models.

Figure 5: Master Curve Comparison **for** Cell 21 [29]

31

Figure 6: Master Curve Comparison **for** Cell 33 [29]

Figure 7: Master Curve Comparison **for** Cell 34 [29]

32

Figure 8: Master Curve Comparison **for** Cell 35 [29]

The master curve comparisons show that the Witczak model made relatively accurate

predictions at intermediate and low temperatures **for** cells 21 and 35. At the high temperature

range, the Witczak model did not fit the lab data. For mixtures from cells 33 and 34, the Witczak

predictive model is poor to fit the lab results. The 2000 Witczak model tends to predict lower

dynamic modulus values at high temperatures than those tested.

North Carolina State University Study [30]

This research per**for**med by Y. Richard Kim et al. [30] studied dynamic complex modulus **of**

mixtures made from materials that were commonly used in North Carolina. The study includes

42 different mix designs with two types **of** asphalt binder. The laboratory results were compared

with the 2000 Witczak predictions as well as the Hirsch predictions. In the final report, accuracy

**of** the predictive model is quantified by the percent **of** error which is the difference between lab

result and model prediction divided by the lab result. Figure 9 and Figure 10 show the results **of**

comparisons.

33

Figure 9: Summary **of** Percent Error in **Dynamic** Moduli **for** Witczak’s Prediction [30]

Figure 10: Summary **of** Percent Error in **Dynamic** Moduli **for** Hirsch’s Prediction [30]

The results indicate that the Witczak model fits lab observations better at lower temperatures

than high temperatures. Similar model efficiencies were found at 35°C and 54.4°C. However, the

Hirsch model showed very low accuracy **of** prediction at 10°C. The authors explained this as a

result **of** extrapolating binder viscosities at 10°C instead **of** testing directly.

Christensen, Pellinen and Bonaquist [10]

This study evaluated three different versions **of** the Hirsch model using 206 data points

collected from the Federal Highway Administration’s Accelerated Loading Facility (ALF)

project, the Mn/Road project, and the WesTrack project. The three Hirsch models included the

“simple version”, the “mastic version” which accounts **for** the mineral filler’s effects on mixture

34

stiffness, and the “transition zone version” which is modified **for** the effects **of** film thickness.

The authors found out that a R-square value **of** 0.968 were observed **for** all three **of** the models.

Taking into account **for** the effects **of** mineral filler and film thickness did not improve the model

efficiency. In addition, a comparison between the Hirsch model and Witczak models were also

made. The comparison result is shown in Figure 11.

Figure 11: Predicted and Measured E* Values [10]

Figure 11 indicates the accuracies **of** Witczak and Hirsch models are on similar scales. At

low temperatures, the Hirsch model tends to be more effective.

University **of** Florida Study [31]

The study is focusing on the efficiency **of** Witczak model (1999) on predicting the dynamic

modulus **of** Florida mixtures. Twenty eight commonly used mixtures in the state **of** Florida were

studied. Three methods were used to obtain binder viscosities including: 1. directly test asphalt

viscosities with Brookfield viscometer; 2. calculate viscosities by shear modulus and phase angle

values from DSR test; 3. use empirical A and VTS parameters recommended by Witczak and

Fonseca **for** mix/laydown condition. The results are shown in Figure 12 through Figure 14

respectively.

35

Figure 12: Measured Values vs. Predicted Values **of** **Dynamic** **Modulus** on log-log Scale

(RTFO Condition, Viscosity from Brookfield Test) [31]

Figure 13: Measured Values vs. Predicted Values **of** **Dynamic** **Modulus** on log-log Scale

(RTFO Condition, Viscosity from DSR Test) [31]

36

Figure 14: Measured Values vs. Predicted Values **of** **Dynamic** **Modulus** on log-log Scale

(Mix/Laydown condition) [31]

The results indicate the Witczak model well simulates the trend **of** dynamic modulus values.

The best fitting lines parallelly deviate from the lines **of** equality. By applying a multiplier or

shift factor **for** each method, the Witczak model showed high accuracy on predicting dynamic

modulus values **for** Florida mixtures. It should be noticed that using DSR test results to estimate

a binder’s viscosity results in lower predicted dynamic modulus values.

Argentina Study [32]

Materials studied in this research contain both lab produced mixtures and field cores. Field

cores were taken from 17 sections around Rosario in the Littoral region **of** Argentina containing

42 types **of** mixtures. Eight laboratory mixtures were designed and compacted to sample

cylinders using Marshall Procedures. Lab data were used to evaluate the 2000 Witczak model,

the Hirsch clarify model, and the Heukelomp and Klomp equation developed in 1964. Figure 15

through Figure 18 show the dynamic modulus values predicted by the Witczak and Hirsch

models versus laboratory results on log-log scale **for** lab produced mixtures and field mixes,

respectively.

37

Figure 15: Comparison **of** Values Using the Witczak **Predictive** Equation [32]

Figure 16: Comparison **of** Values Using the Hirsch Model [32]

38

Figure 17: Comparison **of** Values Using the Witczak **Predictive** Equation [32]

Figure 18: Comparison **of** Values Using the Hirsch Model [32]

The results indicate that the Witczak and Hirsch models have the similar accuracy predicting

dynamic moduli **of** Argentina mixtures. Both **of** the models have good prediction at lower

temperatures. At high temperatures, the predicted E* values tend to be larger than the measured

values.

39

Effects **of** Fibers on **Asphalt** Concrete Mixture **Dynamic** **Modulus**

This section summarizes the findings **of** two research projects: Serfass and Samanos’ study

[33], and a Wuhan University **of** Technology study [34]. Four types **of** manufactured fibers were

studied by Serfass and Samanos, and three types **of** manufactured fibers were studied by the

Wuhan University **of** Technology. The conclusions **of** two studies are agreed showing that

different fibers have notable strengthening effects on mixture dynamic modulus values.

Serfass and Samanos Study [33]

The comprehensive study per**for**med various laboratory tests on mastics, mortars, and asphalt

concretes. Two types **of** mixtures were tested: thin course mixes, and porous mixes. Static and

dynamic moduli tests were per**for**med only **for** the thin course mixes. Pavement conditions

surveys were also conducted. Pavement skid resistance, sand patch depth, and cracking

in**for**mation were collected over more than ten years. The fibers studied included chrysotile, rock

wool, glass wool, and cellulose. Some **of** the research conclusions were:

Fibers could reduce the loss **of** binder in coating mastic, thus increasing a pavement’s

resistance to moisture, aging, and fatigue damage;

Attention needs to be paid on rutting resistance **for** thin wearing courses; and

The static and dynamic modulus values **of** fiber-modified asphalt mixtures are

distinctly higher than mixtures that use the same binders but without fibers.

Wuhan University **of** Technology Study [34]

The three types **of** fibers used in this study were cellulose, polyester and mineral fibers.

Unconfined dynamic modulus tests were per**for**med at five temperatures from -10°C to 54.4°C,

and nine frequencies ranging from 0.1 Hz to 25 Hz. The results indicate adding fibers to asphalt

mixtures can increase HMA dynamic modulus values. Lower phase angles at lower temperatures

and higher phase angles at higher temperatures were observed **for** fiber-modified asphalt

mixtures. **Asphalt** mixtures containing fibers tend to have lower loss modulus values at medium

temperatures.

40

CHAPTER 3: EXPERIMENTAL PLAN AND TESTING METHODS

EXPERIMENTAL PLAN AND TESTING MATERIALS

Experimental materials were procured from the national pooled fund study #1208 testing

sections. The national pooled fund study #1208 conducted a comprehensive research on

application **of** RAS in asphalt pavement including the study **of** mixture and binder properties,

issues in RAS processing and storage, and pavement field per**for**mance. Missouri is the lead state

**of** the pooled fund study. Participating states include Cali**for**nia, Colorado, Indiana, Iowa, Illinois,

Minnesota, and Missouri. This research studied the materials produced **for** the Indiana, Iowa,

Minnesota, and Missouri projects. For each state project, a control section that does not contain

any shingles was constructed. Mixtures containing different types and percentages **of** RAS were

produced as experimental sections. RAP was used with RAS in the Minnesota, Indiana, and

Missouri sections. Iowa mixtures used RAS alone as the virgin asphalt replacement material.

Minnesota testing sections used both tear-**of**f and manufactured RAS. RAS used in other states

are all tear-**of**f RAS. The gradations **of** RAS in Missouri mixes are different; one is ground finer

than the other. Only one type **of** RAS was used in Iowa and Indiana projects. Warm mix asphalt

(foaming method) was studied in the Indiana project. Detailed material in**for**mation **for** each state

project is covered in this chapter.

Field produced loose mixtures and extracted binders were provided to the Iowa State

University (ISU) **Asphalt** Lab in Ames by the state agencies. Sample cylinders were compacted

with Superpave procedures to test dynamic moduli. Five replications were prepared **for** each mix.

Three replications were prepared **for** each extracted binder to test shear moduli and phase angles.

One frequency sweep test was also conducted **for** each type **of** binder. A table **of** experimental

plan is presented below in Table 5. Due to not enough material, three samples were made **for** the

mix #11 instead **of** five samples which were prepared **for** other mixes.

41

Project

Mix

Number

Table 5: Experimental Plan

Mix Description

**Dynamic**

**Modulus**

DSR

DSR

frequency

sweep

1 5% Mfr. RAS 1 xxxxx 2 xxx x

Minnesota 2

5% Tear-**of**f

RAS

xxxxx xxx x

3 Control Mix xxxxx xxx x

4 Control Mix xxxxx xxx x

Iowa

5 4% RAS xxxxx xxx x

6 5% RAS xxxxx xxx x

7 6% RAS xxxxx xxx x

8 Control Mix xxxxx xxx x

Missouri 9 5% Fine RAS xxxxx xxx x

10 5% Coarse RAS xxxxx xxx x

11 Control Mix xxx xxx x

Indiana

12

3% RAS &

HMA

xxxxx xxx x

13

3% RAS &

WMA

xxxxx xxx x

1: manufactured Recycled **Asphalt** Shingle

2: each “x” states **for** one experiment replication

Minnesota DOT Demonstration Project

The Minnesota demonstration project is located at the Mn/Road Cold Weather Road

Research Facility in Albertville, Minnesota. The project is 3.5 miles long with 18 test sections on

the passing and driving shoulders **of** westbound I-94 mainline. A plan view **of** test cells is shown

in Figure 19. Mix laid down in Cell 20 contains 30% RAP and serves as the control section.

Mixes **of** Cells 5, 6, 13, and 14 contain 5% manufactured RAS. Mixes **of** Cells 15 to 23 contain 5%

tear-**of**f RAS. Each cell is 500 feet long including a 50 feet transition area. All cells are 3 inches

thick with a granular base, except **for** Cell 5 is paved on top **of** a HMA base. Construction **of** test

sections was completed in September, 2008 [35].

The Minnesota demonstration project used a 12.5mm (1/2 inch) NMAS (nominal maximum

aggregate size) aggregate gradation **for** all test mixes. The aggregate gradations are shown in

Table 6 and Figure 20. The gradations **of** mixes containing 5% RAS are similar to each other.

The control mix gradation contains more coarse aggregates than the mixes containing RAS. All

42

mixes used the same per**for**mance grade (PG) 58-22 virgin binder. The asphalt content is 17.1%

**for** the manufactured RAS and 23% **for** the tear-**of**f RAS. The RAP used in control section has an

asphalt content **of** 6%. The total asphalt content **for** all mixes is 5%. The loose mixes received by

ISU **Asphalt** Lab are from randomly chosen from Cells 5, 6, 15, 18, 19, and 22. Control mix

from Cell 20 was also received and tested by the ISU **Asphalt** Lab.

43

500'

500'

500'

500'

500'

500'

500'

500'

500' 500' 500' 500' 500' 500'

500' 500' 500'

500'

Traffic Lanes

To Monticello

Cell 50 Cell 50

Cell 51 Cell 51

Cell 5

(b) (3'

wide)

Cell 6 (b)

(4' Wide)

Cell 5 (a)

(8' wide)

Cell 7 Cell 7

Cell 8 Cell 8

Cell 9 Cell 9

Cell 60 Cell 60

Cell 61 Cell 61

Cell 62 Cell 62

Cell 63 Cell 63

Cell 96 Cell 96

Cell 97 Cell 97

Cell 92 Cell 92

Cell 10 I

Cell 10

Cell 11 Cell 11

9

Cell 12 Cell 12

Cell 13 (b)

(4' wide)

Cell 14 (b)

(4' wide)

MnRoads I94 Mainline Test Section

Passing Shoulder

West Transition

4

W

e

s

t

Driving Shoulder

Cell 6 (a)

Cell 13 (a)

Cell 14 (a)

Cell 15

Cell 16

Cell 17

Cell 18

Cell 19

Cell 20 (b)

Cell 20 (a)

Cell 21

Cell 22

← 10' →

Albertville

East Transition

Cell 23

← 10' →

Figure 19: Plan View **of** MnROAD Test Cells [35]

44

Percent Passing, %

Table 6: Minnesota Demonstration Project Sieve Analysis Results

%PASS

SIEVE Control

Mix

Mfr. RAS

Mix

Tear-**of**f

RAS Mix

1" 100 100 100

3/4" 100 100 100

1/2" 95 91 86

3/8" 89 84 73

#4 66 58 39

#8 52 45 28

#10 48 43 26

#16 36 34 21

#30 23 22 14

#40 17 16 10

#50 12 10 7

#100 4 4 2

#200 1 1.3 1

100.0

90.0

80.0

70.0

Mfr. RAS Mix

60.0

Tear-**of**f RAS Mix

50.0

Control Mix

40.0

30.0

Control Points

20.0

Restricted Zone

10.0

Maximum Density Line

0.0

0.000 1.000 2.000 3.000 4.000 5.000

Sieve Size^0.45 Power, mm

Figure 20: Aggregate Gradation 0.45 Power Chart **for** Minnesota Demonstration Project

Gradations

45

Iowa DOT Demonstration Project

The Iowa DOT demonstration project is located on Highway 10 west **of** Pavlina, Iowa. The

project was constructed in June and July, 2010. The total project is 32.5 lane miles including four

test sections. Every test section has a 2 inch thick surface course underlying by a granular base.

Figure 22 shows a plan view **of** the demonstration project sections. Four types **of** mixes were

randomly assigned to the four test sections as shown in Figure 22.The mixes were designed with

the same aggregate gradations and virgin binders, but different RAS contents ranging from 0% to

6%. The Iowa demonstration project used a 12.5mm NMAS **for** mix design and a PG64-22

binder **for** the virgin asphalt. The aggregate gradation is summarized in Table 7 and

schematically presented in Figure 23. The total asphalt content is 5.5%, and the virgin binder

content is varying with the amount **of** shingle in each mix. Figure 21 shows how much virgin

binder is replaced by the asphalt in the recycled shingles. The figure indicates that adding 4% to

6% RAS to asphalt mix can reduce the use **of** virgin asphalt by 15% to 20%.

20%

7%

6%

15%

5%

Virgin Binder

Replacement

10%

5%

4%

3%

2%

1%

RAS Content

Virgin Binder

Replacement

RAS%

0%

Section 4 Section 2 Section 1 Section 3

0%

Figure 21: RAS Content and Virgin Binder Replacement **for** Iowa Demonstration Project

Test Sections

46

← 3.4 mi → ← 3.6 mi → ← 6.3 mi →

← 3.75 mi →

← 5.35 mi → ← 3.0 mi → ← 4.1 mi → ← 3.8 mi →

Iowa Highway 10

Eastbound Lane

↓Paullina

Westbound Lane

↑Alton

Control Section 4

(b)

0% RAS

Control Section 4

(a)

0% RAS

Test Section 3

(b)

6% RAS

Test Section 3

(a)

6% RAS

Test Section 2

(b)

4% RAS

Test Section 2

(a)

4% RAS

Test Section 1

(b)

Test Section 1

(a)

5% RAS 5% RAS

← 12' → ← 12' →

Figure 22: Plan View **of** Iowa Demonstration Project Test Sections [35]

47

Percent Passing, %

Table 7: Iowa Demonstration Project Sieve Analysis Results

SIEVE

%PASS

0%RAS 4%RAS 5%RAS 6%RAS

1" 100 100 100 100

3/4" 100 100 100 100

1/2" 94 95 94 93

3/8" 84 85 87 84

#4 66 67 71 66

#8 46 45 48 44

#10 43 41 44 40

#16 34 31 33 30

#30 23 20 22 20

#40 17 15 16 14

#50 11 9 9 9

#100 3 3 3 3

#200 0.6 0 1 0.6

100.0

90.0

80.0

70.0

60.0

50.0

40.0

30.0

20.0

10.0

0.0

0.000 1.000 2.000 3.000 4.000 5.000

Sieve Size^0.45 Power, mm

Control Points

Restricted Zone

Maximum Density

Line

Figure 23: Aggregate Gradation 0.45 Power Chart **for** Iowa Demonstration Project

Missouri DOT Demonstration Project

The Missouri DOT constructed the demonstration project **for** the pooled fund study in May

and June, 2010. The 8.8 mile project is located on US Route 65 south **of** Springfield, Missouri.

The total project is 17.6 lane miles with a 3.75 inches surface layer underlying by a concrete

pavement. This demonstration project was developed to study the influences **of** RAS grind size

48

on pavement per**for**mance and the economic feasibility **of** incorporating ground tire rubber (GTR)

and asphalt mixes containing RAS and RAP. Three test sections were paved as shown in Figure

24. A PG 64-22 asphalt was selected as the virgin binder. The virgin binder was modified with

GTR and a vestenamer polymer to achieve a 70-22 per**for**mance grade. The control section

contains 15% RAP and 0% RAS. Test section 2 contains 5% fine ground RAS which 100% **of**

RAS particles pass the 3/4 inch sieve and 95% particles pass the #4 sieve. Test section 3 contains

5% coarse ground RAS which 100% RAS particles pass 1/2 inch sieve. Both test sections 2 and

3 contain 10% RAP so that all mixes have 15% recycled materials. The same aggregate

gradations were designed **for** the three test sections. Figure 25 shows the designed aggregate

gradation. The sieve analysis results are summarized in Table 8. The design asphalt content was

5.3%. Test sections containing 5% RAS used 3.7 virgin binders content to achieve the design

binder content.

Figure 24: Plan View **of** Missouri Demonstration Project Test Sections [35]

49

Percent Passing, %

100.0

90.0

80.0

70.0

60.0

50.0

Control Points

40.0

Restricted Zone

30.0

Maximum Density Line

20.0

10.0

0.0

0.000 1.000 2.000 3.000 4.000 5.000

Sieve Size^0.45 Power, mm

Figure 25: Aggregate Gradation 0.45 Power Chart **for** Missouri Demonstration Project

Table 8: Missouri Demonstration Project Sieve Analysis Results

%PASS

SIEVE Control

Mix

5% Fine

RAS

5% Coarse

RAS

1" 100.0 100.0 100.0

3/4" 100.0 99.2 100.0

1/2" 92.8 94.1 94.2

3/8" 85.0 85.7 85.6

#4 52.7 49.1 51.4

#8 27.3 26.0 26.7

#10 24.0 23.3 23.6

#16 16.8 17.0 16.4

#30 11.0 11.6 10.8

#40 8.9 9.5 8.9

#50 7.2 7.8 7.3

#100 4.2 4.5 4.4

#200 1.5 1.3 1.3

Indiana DOT Demonstration Project

The Indiana DOT demonstration project was completed in July, 2009. The project is located on

U.S. Route 6 east **of** Nappance, Indiana. The overall construction is 13.6 lane miles. A 1.5 inch

surface layer was placed on top **of** a previously existing asphalt surface with an underlying

50

← 6.8 mi →

←1.0 mi→

← 4.7 mi →

concrete pavement. The demonstration project was developed to evaluate the per**for**mance **of**

incorporation **of** RAS and warm mix asphalt in asphalt concrete pavements. Three test sections

were constructed as shown in Figure 26. The control section used a hot mix asphalt containing

15% fractionated recycled asphalt pavement (FRAP). Test section 2 used the same hot mix

asphalt with 3% RAS. A foaming method was applied to produce warm mix asphalt which is laid

down in test section 3. The test section 3 also contains 3% RAS. The same aggregate gradation

was designed **for** different test sections as shown in Figure 27. The sieve analysis results are

summarized in Table 9. A PG 70-22 asphalt was selected as the virgin binder. The design binder

content was 6.2%. Test sections containing 3% RAS used 5.4% virgin binder content to achieve

the design total binder content.

Indiana US Route 6

Eastbound Lane

↓Ligonier

Westbound Lane

↑Nappanee

Test Section 3

WMA

Test Section 2

HMA

←1.1 mi→

Control Section 1(b)

HMA

Control Section 1(a)

HMA

← 12' → ← 12' →

Figure 26: Plan View **of** Indiana Demonstration Project Test Sections [35]

51

Percent Passing, %

Table 9: Indiana Demonstration Project Sieve Analysis Results

%PASS

SIEVE Control

Mix

3% RAS

HMA

3% RAS

WMA

1" 100.0 100.0 100.0

3/4" 100.0 100.0 100.0

1/2" 100.0 99.9 100.0

3/8" 96.6 94.6 96.0

#4 75.7 72.1 73.5

#8 53.7 50.1 51.5

#10 49.5 46.3 47.7

#16 35.8 33.6 34.3

#30 22.2 21.2 21.2

#40 16.1 15.9 15.7

#50 10.5 10.9 10.7

#100 3.8 4.4 4.2

#200 0.5 0.6 0.6

100.0

90.0

80.0

70.0

60.0

50.0

Control Points

40.0

Restricted Zone

30.0

Maximum Density Line

20.0

10.0

0.0

0.000 1.000 2.000 3.000 4.000 5.000

Sieve Size^0.45 Power, mm

Figure 27: Aggregate Gradation 0.45 Power Chart **for** Indiana Demonstration Project

52

LABORATORY TESTING DESIGN

**Dynamic** **Modulus** Test

The dynamic modulus tests were per**for**med with a universal testing machine (UTM) in a

environmental chamber shown in Figure 28. The UTM has a hydraulically driven load frame

which can provide a maximum load **of** 25kN (5620lbs) at various frequencies. The magnitude

and frequency **of** applied load can be precisely controlled. The applied sinusoidal load was

carefully selected to maintain a sample strain level **of** 85 to 110με to ensure a measurable strain

and prevent excessive damage to sample. Excessive unrecoverable de**for**mation can be achieved

if the strain is too high. The testing was conducted following ASTM D3496. The standards

requires

(height by diameter) asphalt cylinder cored from a

cylinder compacted by the Superpave Gyratory Compactor (SGC). Extra time and costs

are needed to core an asphalt cylinder. According to Robinette and Williams’ study (2006), the

dynamic modulus test results **of** cored and directly compacted samples are not significantly

different. More than 70 samples were made **for** this research including trial samples to determine

the required mass **for** target air void and samples **for** testing dynamic modulus. In order to lower

the cost and make the laboratory work more practical, the 150mm by 100mm cylinders in this

research were compacted by the SGC with a special mold designed specifically **for** samples in

this size. The sample strain was tested with three evenly spaced LVDTs attached on the side **of**

the sample.

The statistical design **of** dynamic modulus experiment is split plot. **Dynamic** moduli were

tested at 4°C , 21°C , and 37°C and nine frequencies (0.1, 0.2, 0.5, 1, 2, 5, 10, 20, and 25Hz) at

each temperature **for** each sample. There**for**e, each sample was tested with 27 treatment

combinations. The 13 types **of** mixtures **for**m the whole plots. Mixture type is the whole plot

factor. Five samples were made from each mixture to **for**m the sub plots. The sub plot factor is

the individual cylinder. Thus, the variability caused by mixture type and treatments can be

determined. The variability between the five replications **for** each mixture can be also calculated

and separated from the total error, increasing the chance to identify the significant differences

between different types **of** mixtures.

53

Figure 28: Universal Testing Machine and Environmental Chamber

Direct Shear Rehometer (DSR) Test

The DSR tests were conducted to model the asphalt rheological properties. Testing materials

were extracted from field mixes **of** the pooled fund study demonstration projects by following

AASHTO Designation TP2-94, Standard Test Method **for** the Quantitative Extraction and

Recovery **of** **Asphalt** Binder from Hot Mix **Asphalt** (HMA). The extraction method uses asphalt

solvents blended with ethanol to separate the asphalt binder from aggregates. The commonly

used asphalt solvents are n-Propyl Bromide, Trichloroethylene, and Toluene. **Asphalt** binder is

recovered through a centrifuge. The extractions were per**for**med by the Minnesota DOT. The

referenced standard **for** DSR testing is ASTM D7175, Standard Test Method **for** Determining the

Rheological Properties **of** **Asphalt** Binder using a **Dynamic** Shear Rheometer. Two DSR

experiments were designed **for** different research interests elaborated in following paragraphs.

Binder High Temperature Grading

DSR tests were per**for**med to determine asphalt binder high temperature grade by following

the Superpave test specifications. Because the asphalt binders were extracted from field

produced mixtures which were short-term aged, the grading procedures followed the Superpave

grading method **for** rolling thin film oven (RTFO) aged asphalt material. DSR tests were

54

conducted with a dynamic shear rheometer shown in Figure 29. At least three temperatures were

tested **for** each sample in order to grade the asphalt.

Figure 29: AR1500 **Dynamic** Shear Rheometer

Frequency Sweep

DSR frequency sweep tests were designed to construct master curves **of** binder complex

shear modulus (G*) and phase angle (Φ). The master curves characterize binder rheological

properties over a wide range **of** temperature or frequency. The master curves can be used to

estimate binder G* and Φ values at any interested temperature and frequency. The G* and Φ **for**

each binder were tested at seven temperatures and 15 frequencies 1 ranging from 0.1Hz to 50Hz

**for** each temperature. The seven testing temperatures are 13, 21, 29, 37, 46, 58, and 70°C .

Because the binders were tested over a large temperature range, different sample sizes were

selected. The 25mm diameter samples were tested at 46, 58 and 70°C . The required stress to

maintain a measurable strain level **of** a 25mm sample at low temperature exceeds the machine

capacity. There**for**e, the 8mm diameter sample size was selected to test the G* and Φ values at

13, 21, 29, and 37°C . The dynamic rheological properties were tested by measuring the required

50Hz.

1 15 frequencies: 0.1, 0.158, 0.251, 0.398, 0.631, 1, 1.585, 2.512, 3.981,6.31, 10, 15.849, 25.121, 39.809, and

55

shear stress to achieve a preset strain level. The strain level should be large enough so that it is

measurable and also small enough so that the required stress does not exceed the capacity **of** the

testing device or damage the sample. The controlled strain level **for** the 8mm sample is 0.1% and

**for** the 25mm sample is 10%.

56

CHAPTER 4: EVALUATION AND MODIFICATION OF WITCZAK AND HIRSCH

MODELS

Many previous studies, such as studies conducted by University **of** Minnesota [29],

Christensen, Pellinen, and Bonaquist [10], North Carolina State University [30], University **of**

Florida [31], and Marinez and Angelone [32] have shown that the Witczak and Hirsch models

have reasonable accuracy to predict the dynamic modulus **of** HMA mixtures. The Witczak model

uses four input parameters ( , , 2 , and 3 ) to characterize aggregate gradation, two

parameters (V 4 a and V 5 beff ) to describe mixture volumetric property, and two parameters

(frequency and viscosity, or shear modulus and phase angle 6 ) to include the binder rheological

behavior. In the Hirsch model, three input parameters including voids in mineral aggregate

(VMA), voids filled by asphalt (VFA), and binder shear modulus are considered as the factors

that are used to estimate a mixture dynamic modulus. The primary components **of** RAS include

asphalt, granules (passing #12 screen), dust (passing #200 screen), and fibers. The asphalt in

RAS is manufactured through an “air-blown” process and exposed to long-term weathering.

There**for**e, the asphalt usually has a higher stiffness than typical asphalt used in asphalt mixtures.

The effects **of** shingles in HMA include a change in aggregate gradation and volumetric

properties, an increase in binder viscosity and shear modulus, a decrease in binder’s phase angle,

and a stiffening effect introduced by fibers. The changes in gradation, volumetrics, and binder

rheology can be explained by the original Witczak and Hirsch models. However, both models do

not include the effects **of** fibers. In this chapter, two versions **of** the Witczak model (1999 and

2006 versions) and the latest Hirsch model are evaluated to determine the accuracy **of** predicting

mixture dynamic modulus caused by the fibers in shingles. **Modification**s were made to account

**for** this effect using the results **of** a**for**ementioned tests in Chapter 3.

2

, , : cumulative percent **of** aggregate mass retaining on 3/8”, 3/4”, and U.S. #4 (4.75mm) sieves

3

: percent **of** aggregate mass passing U.S. #200 (0.075mm) sieve

4 V a is the air content **of** compacted mixture

5 V beff is the effective bitumen content by volume

6 Frequency and viscosity are used in the 1999 Witczak Model, shear modulus and phase angle are used in the

1999 Witczak Model

57

ORIGINAL MODEL EVALUATION

A total number **of** 1701 dynamic modulus values were observed from 13 mixes to evaluate

the 1999 Witczak Model. The comparisons between predicted and tested E* values on both

normal and logarithm scales are plotted in Figure 30 and Figure 31, respectively. The plotted

points lined up along the line **of** equality, except **for** the data **of** the Iowa mixes are above the line

**of** equality. This indicates the 1999 Witczak Model tends to overestimate the E* **of** Iowa mixes.

The overall linear trend line matches the line **of** equality showing a high prediction accuracy **of**

the 1999 Witczak Model. On a normal scale, the overall variability becomes larger when the

model is used to predict larger E* values which is referring to the scenario that the pavement is

subjected to a lower temperature or higher loading rate. The model tends to overestimate the E*

values **of** Iowa mixes and underestimate the Minnesota mixes. Each project has a distinct linear

trend line. On the logarithm scale, the overall variability becomes smaller when the predicted E*

values are larger. Compared to the overall variability, the variability within each project is small.

The overall variability includes the variability between projects and the variability within each

project. Variability in accuracies **of** predictions arises from differences in materials, asphalt plant

operations, RAS contents, and sampling and testing errors. The effects **of** different RAS contents

do not result in the variability between projects. The coefficient **of** determination, R 2 , is 0.86 on

a normal scale, and 0.87 on a logarithm scale. The standard error ratio, Se/Sy, is 0.37 **for** a

normal and 0.36 **for** a logarithm scale. A commonly used criterion **of** measuring a model’s

goodness-**of**-fit is given in Table 10. According to the subjective criteria, the goodness-**of**-fit **for**

the1999 Witczak Model is good.

Table 10: Subjective Classification **of** the Goodness-**of**-Fit Statistical Parameters [37]

Criteria R2 Se/Sy

Excellent >0.90

Witczak 1999 Model Predicted **Dynamic**

**Modulus**, psi

Witczak 1999 Model Predicted **Dynamic**

**Modulus**, log(psi)

3500000

3000000

2500000

2000000

1500000

1000000

500000

0

0 1000000 2000000 3000000 4000000

**Dynamic** **Modulus** Lab Results, psi

Figure 30: Lab Tested vs. Witczak Model (1999) Predicted E* Values on Normal Scale

7.5

7

6.5

6

5.5

5

4.5

4

Minnesota 0% RAS

Minnesota 5% RAS

Iowa 0% RAS

Iowa 4% RAS

Iowa 5% RAS

Iowa 6% RAS

Missouri 0% RAS

Missouri 5% RAS

Indiana 15% FRAP HMA

Indiana 3% RAS

Line **of** Equality

Linear Trend Line

4 5 6 7 8

**Dynamic** **Modulus** Lab Results, log(psi)

Figure 31: Lab Tested vs. Witczak Model (1999) Predicted E* Values on Logarithm Scale

Because **of** material shortages **of** the recovered asphalt binders from Minnesota tear-**of**f RAS

mix and Iowa 5% RAS mix, the G* values and phase angles were not able to be tested **for** Mixes

59

Witczak 2006 Model Predicted **Dynamic** **Modulus**, psi

#2 and #6. There**for**e, 1431 dynamic modulus values from lab tests were observed to evaluate the

2006 Witczak Model. The comparisons between predicted and tested E* values on both the

normal and logarithm scales are plotted in Figure 32 and Figure 33, respectively. The linear trend

lines in both Figure 32 and Figure 33 are above the line **of** equality. This indicates the 2006

Witczak Model tends to overestimate the E* values in general. Compared to the 1999 Witczak

Model, the trend **for** each project is not that obvious. However, the linear trend line **for** each

project is still distinct. This indicates a large portion **of** overall variability is caused by the

differences between projects. On the normal scale, the overall variability becomes larger when

the model is trying to predict larger E* values. However, on the logarithm scale, the overall

variability becomes smaller when the predicted E* values are larger. The variability within each

project is smaller than the overall variability. The 2006 Model has a R 2 value **of** 0.44 and Se/Sy

**of** 0.75 on logarithm scale. The prediction accuracy **of** the 2006 Witczak Model is fair.

7000000

6000000

5000000

4000000

3000000

2000000

1000000

0

0 1000000 2000000 3000000 4000000

**Dynamic** **Modulus** Lab Results, psi

Figure 32: Lab Tested vs. Witczak Model (2006) Predicted E* Values on Normal Scale

60

Witczak 2006 Model Predicted **Dynamic** **Modulus**,

log(psi)

7.5

7

Minnesota 0% RAS

Minnesota 5% Mfr. RAS

6.5

6

5.5

5

4.5

4

Iowa 0% RAS

Iowa 4% RAS

Iowa 6% RAS

Missouri 0% RAS

Missouri 5% RAS

Indiana 15% FRAP HMA

Indiana 3% RAS

Line **of** Equality

Linear Trend Line

4 4.5 5 5.5 6 6.5 7 7.5

**Dynamic** **Modulus** Lab Results, log(psi)

Figure 33: Lab Tested vs. Witczak Model (2006) Predicted E* Values on Logarithm Scale

The evaluation **of** the Hirsch model includes 1431 dynamic modulus values. The comparison

between predicted and tested E* values are plotted in Figure 34 and Figure 35 on normal and

logarithm scales, respectively. On both figures, the linear trend line is very close to the line **of**

equality indicating the Hirsch model has a high level **of** accuracy **for** dynamic moduli **of** asphalt

mixtures. There is not distinct trend **for** each project. Different projects have similar variability.

Figure 34 shows the Hirsch model tends to overestimate the E* values **for** Iowa mixes, and

underestimate the Minnesota mixes. However, the differences between prediction accuracies **of**

different projects are very small. This indicates that the differences between projects do not

contribute too much variability to the total error. The R 2 values **of** the Hirsch model on normal

and logarithm scales are 0.90 and 0.83, respectively. The corresponding Se/Sy values **for** the

normal and logarithm scales are 0.31 and 0.41 respectively. There**for**e, according to Table 10, the

goodness-**of**-fit **of** Hirsch model is excellent on a normal scale, and good on a logarithm scale.

61

Hirsch Model Predicted **Dynamic** **Modulus**,

log(psi)

Hirsch Model Predicted **Dynamic** **Modulus**,

psi

3000000

2500000

2000000

1500000

1000000

500000

0

Minnesota 0% RAS

Minnesota 5% RAS

Iowa 0% RAS

Iowa 4% RAS

Iowa 6% RAS

Missouri 0% RAS

Missouri 5% RAS

Indiana 15% FRAP HMA

Indiana 3% RAS

Line **of** Equality

linear trend line

0 1000000 2000000 3000000

**Dynamic** **Modulus** Lab Results, psi

Figure 34: Lab Tested vs. Hirsch Model Predicted E* Values on Normal Scale

6.5

6

5.5

5

4.5

Minnesota 0% RAS

Minnesota 5% Mfr. RAS

Iowa 0% RAS

Iowa 4% RAS

Iowa 6% RAS

Missouri 0% RAS

Missouri 5% RAS

Indiana 15% FRAP HMA

Indiana 3% RAS

Line **of** Equality

Linear Trend Line

4

4 4.5 5 5.5 6 6.5

**Dynamic** **Modulus** Lab Results, log(psi)

Figure 35: Lab Tested vs. Hirsch Model Predicted E* Values on Logarithm Scale

Evaluations **of** the three E* predictive models show that the 1999 Witczak Model has the

highest prediction accuracy, and the prediction accuracy **of** the 2006 Witczak Model is the

62

lowest. The three models tend to overestimate mixture dynamic moduli in general. The

accuracies **of** both Witczak models are dependent upon different projects. The differences

between projects do not have significant impact on prediction accuracies **of** the Hirsch model.

On the tested vs. predicted E* figures (Figure 30 through Figure 35), the mixes containing 0%,

3%, 4%, 5%, and 6% RAS are denoted by rhombus, cross, circle, triangle, and rectangle symbols,

respectively. For each project, the plotted points with the same denotation are concentrated with

a distinct trend line. This indicates the differences between RAS contents have impacts on the

prediction accuracies **of** the three models. Analysis **of** Variance (ANOVA) tables with the ratio

**of** model predicted E* to lab tested E* as the response are given in Table 11 through Table 13**for**

the 1999 Witczak, 2006 Witczak, and Hirsch models, respectively. Three main factors are RAS

content, treatment type, and project. The results show that RAS content in each model has a p-

value less than 0.0001. It indicates the RAS content is a significant factor that can affect the

value **of** model predicted E* divided by the lab tested E* values which is referring to the

prediction accuracy **of** a predictive model. A prediction accuracy value **of** 1 indicates the

predicted value is exactly the same as the actual value. The prediction accuracy decreases as this

number deviates from 1.

Table 11: ANOVA Table **for** Witczak 1999 Model with Predicted E*/Lab E* as the

Response

Source

Degree **of** Sum **of**

Freedom Squares

F Ratio Prob>F

RAS% 4 119 393

Table 13: ANOVA Table **for** Hirsch Model with Predicted E*/Lab E* as the Response

Source

Degree **of** Sum **of**

Freedom Squares

F Ratio Prob>F

Project 3 37.12814 6.0789 0.0004

Treatment 29 165.25453 2.7990

Table 14: Mean **of** Model Prediction Accuracy

Model Level Mean

1999

Witczak

2006

Witczak

Hirsch

0% 1.21216

3% 1.14153

4% 1.43447

5% 1.27868

6% 2.15744

0% 3.36279

3% 2.45701

4% 4.5773

5% 3.38944

6% 5.2273

0% 1.31907

3% 1.685497

4% 1.31907

5% 1.223297

6% 1.525975

Table 15: Student-t Test Results **for** Model Prediction Accuracy

Model

Project Comparison

RAS% Comparison

Comparison Significant Difference Comparison Significant Difference

MN vs. IA Yes 0% vs. 3% Yes

MN vs. MO Yes 0% vs. 4% Yes

Witczak MN vs. IN Yes 0% vs. 5% Yes

1999 IA vs. MO Yes 0% vs. 6% Yes

IA vs. IN Yes 3% vs. 4% Yes

MO vs. IN No 3% vs. 5% Yes

3% vs. 6% Yes

4% vs. 5% Yes

4% vs. 6% Yes

5% vs. 6% Yes

MN vs. IA Yes 0% vs. 3% Yes

MN vs. MO Yes 0% vs. 4% No

Witczak MN vs. IN Yes 0% vs. 5% No

2006 IA vs. MO Yes 0% vs. 6% Yes

IA vs. IN Yes 3% vs. 4% Yes

MO vs. IN Yes 3% vs. 5% Yes

3% vs. 6% No

4% vs. 5% Yes

4% vs. 6% Yes

5% vs. 6% No

Hirsch MN vs. IA No 0% vs. 3% Yes

65

MN vs. MO Yes 0% vs. 4% Yes

MN vs. IN Yes 0% vs. 5% No

IA vs. MO Yes 0% vs. 6% No

IA vs. IN Yes 3% vs. 4% No

MO vs. IN No 3% vs. 5% Yes

3% vs. 6% No

4% vs. 5% Yes

4% vs. 6% No

5% vs. 6% No

MODELING METHDOLOGY

The philosophy **of** modifying the E* predictive models **for** shingle effects is identifying the

prediction accuracy variability caused by differences **of** RAS contents. The prediction accuracy

**for** each pair **of** predicted and tested E* values can be measured by their difference (e.g.

predicted E* - tested E*) or ratio (e.g. predicted E*/ tested E*). The prediction accuracies are

affected by errors in measuring the true dynamic moduli **of** HMA mixtures, and inaccuracies **of**

the predicted E* values. The E* measurement errors can be caused by systematic errors which

are due to the inaccuracies **of** testing apparatuses, and variability in sampling and testing

procedures. The inaccuracies **of** the predicted E* result from incorrect values **of** input parameters

and the inaccuracies **of** the models themselves. The three E* predictive models have 12 different

input parameters characterizing aggregate gradation, binder rheology, and mixture volumetric

properties. The parameters **for** aggregate gradation and mixture volumetrics were calculated or

directly observed from testing results. The parameters to describe binder rheology were obtained

from asphalt rheological models. Errors in lab testing and models can result in inaccurate input

parameter values, too. The models themselves can be inaccurate because **of** incorrect

assumptions that are made to construct the model, missing factors that have effects on the

prediction results, and limitations **of** databases that were used to develop the models. The

Witczak models assume the relation between E* and loading frequency is depicted by a sigmoid

function. The Hirsch Model is based on the assumption that the law **of** mixture can be applied to

HMA. In the Hirsch Model, the dynamic modulus **of** an asphalt binder is assumed to be three

times the binder shear modulus. Although these assumptions provide high accuracy **for**

simulations, errors **of** the simulations still exist. Missing effective factors include RAS content,

aggregate stiffness, and other factors that have effects on the E* values. The coefficients **of** a

66

model are determined by regression **of** lab tested E* values. The size and diversity **of** a database

can affect a model’s applicability. The objective **of** this chapter is to determine the effects **of**

different RAS contents on the model prediction accuracies. Three steps were taken to approach

this objective: firstly, determine the input parameters; secondly, calibrate the predictive models

using E* **of** the control mixes to eliminate the project variability in prediction accuracies; and

thirdly, modify the predictive models with RAS content as a factor if possible.

Model Input Parameters

At the beginning **of** this Chapter, the 12 input parameters related to aggregate gradation,

volumetrics, and binder rheology are introduced. The 12 input parameters include cumulative

aggregate percentage retained on #4 (ρ 4 ), 3/8” (ρ 38 ), and 3/4” (ρ 34 ) sieves, fine content (ρ 200 ),

voids in mineral aggregate (VMA), voids filled by asphalt (VFA), effective binder volume

content (V beff ), air voids (V a ), dynamic shear modulus **of** binder (G*), phase angle **of** binder (δ),

loading frequency (f), and binder viscosity (η). The aggregate gradation parameters, ρ 4 , ρ 38 , ρ 34 ,

and ρ 200 , are obtained from the sieve analysis tests **for** quality assurance and quality control

(QA/QC). The results **of** the sieve analysis tests are provided in the experimental plan in Chapter

2. The mixture volumetric parameters, VMA, VFA, V a , and V beff , are calculated from the

specific gravities **of** aggregate (G sb ), asphalt binder (G b ), mixture (G mm ), and compacted sample

cylinder (G mb ). The G sb and G mm values **for** each type **of** mix are procured from the mix design **of**

each project. The specific gravity **of** asphalt binder is estimated from the pooled fund study

literature to be 1.038 **for** all types **of** binder in this research. Cylinder bulk specific gravity values

were observed from lab tests following the standard test procedures specified in AASHTO T166.

The volumetric properties are summarized in Table 16. The binder rheological properties are

predicted by the viscosity-temperature susceptibility (A-VTS) method and the master curves **for**

binder shear modulus and phase angle.

67

Table 16: Volumetric Properties **of** Compacted Sample Cylinder

Sample

Number

Project Mix Description Gsb Gmb Gmm Va VMA VFA Vbeff

1 MN 5% Mfr. RAS 2.697 2.348 2.527 7.1 17.2 58.8 10.1

2 MN 5% Mfr. RAS 2.697 2.342 2.527 7.3 17.4 58.1 10.1

3 MN 5% Mfr. RAS 2.697 2.346 2.527 7.2 17.3 58.3 10.1

4 MN 5% Mfr. RAS 2.697 2.348 2.527 7.1 17.2 58.7 10.1

5 MN 5% Mfr. RAS 2.697 2.345 2.527 7.2 17.3 58.4 10.1

6 MN 5% Tear-**of**f RAS 2.697 2.378 2.547 6.7 16.3 59.0 9.6

7 MN 5% Tear-**of**f RAS 2.697 2.379 2.547 6.6 16.3 59.4 9.7

8 MN 5% Tear-**of**f RAS 2.697 2.369 2.547 7.0 16.6 57.9 9.6

9 MN 5% Tear-**of**f RAS 2.697 2.374 2.547 6.8 16.5 58.7 9.7

10 MN 5% Tear-**of**f RAS 2.697 2.366 2.547 7.1 16.7 57.6 9.6

11 MN 30% RAP 2.697 2.355 2.527 6.8 17.1 60.3 10.3

12 MN 30% RAP 2.697 2.359 2.527 6.6 17.0 61.1 10.4

13 MN 30% RAP 2.697 2.352 2.527 6.9 17.2 60.0 10.3

14 MN 30% RAP 2.697 2.350 2.527 7.0 17.3 59.6 10.3

15 MN 30% RAP 2.697 2.349 2.527 7.1 17.4 59.1 10.3

16 IA 0% RAS 2.617 2.275 2.443 6.9 17.8 61.3 10.9

17 IA 0% RAS 2.617 2.270 2.443 7.1 18.0 60.7 10.9

18 IA 0% RAS 2.617 2.279 2.443 6.7 17.7 62.2 11.0

19 IA 0% RAS 2.617 2.273 2.443 7.0 17.9 60.9 10.9

20 IA 0% RAS 2.617 2.271 2.443 7.0 18.0 61.1 11.0

21 IA 4% RAS 2.617 2.298 2.464 6.7 17.0 60.6 10.3

22 IA 4% RAS 2.617 2.289 2.464 7.1 17.3 59.1 10.2

23 IA 4% RAS 2.617 2.298 2.464 6.7 17.0 60.6 10.3

24 IA 4% RAS 2.617 2.288 2.464 7.1 17.4 59.2 10.3

25 IA 4% RAS 2.617 2.291 2.464 7.0 17.3 59.5 10.3

26 IA 5% RAS 2.617 2.293 2.460 6.8 17.2 60.5 10.4

27 IA 5% RAS 2.617 2.283 2.460 7.2 17.6 59.0 10.4

28 IA 5% RAS 2.617 2.280 2.460 7.3 17.7 58.7 10.4

29 IA 5% RAS 2.617 2.299 2.460 6.6 17.0 61.2 10.4

30 IA 5% RAS 2.617 2.290 2.460 6.9 17.3 60.2 10.4

31 IA 6% RAS 2.617 2.277 2.451 7.1 17.6 59.7 10.5

32 IA 6% RAS 2.617 2.272 2.451 7.3 17.8 58.9 10.5

33 IA 6% RAS 2.617 2.273 2.451 7.3 17.7 58.8 10.4

34 IA 6% RAS 2.617 2.287 2.451 6.7 17.2 61.1 10.5

35 IA 6% RAS 2.617 2.277 2.451 7.1 17.6 59.7 10.5

36 MO 15% RAP 2.630 2.295 2.471 7.1 17.0 58.2 9.9

37 MO 15% RAP 2.630 2.293 2.471 7.2 17.1 57.9 9.9

38 MO 15% RAP 2.630 2.301 2.471 6.9 16.8 59.1 9.9

68

39 MO 15% RAP 2.630 2.295 2.471 7.1 17.0 58.2 9.9

40 MO 15% RAP 2.630 2.298 2.471 7.0 16.9 58.6 9.9

41 MO 5% Fine RAS 2.632 2.295 2.547 6.8 17.3 60.6 10.5

42 MO 5% Fine RAS 2.632 2.298 2.547 6.7 17.1 61.2 10.5

43 MO 5% Fine RAS 2.632 2.294 2.547 6.8 17.3 60.6 10.5

44 MO 5% Fine RAS 2.632 2.293 2.547 6.8 17.3 60.4 10.5

45 MO 5% Fine RAS 2.632 2.293 2.547 6.8 17.3 60.4 10.5

46 MO 5% Coarse RAS 2.632 2.293 2.527 6.5 17.3 62.8 10.9

47 MO 5% Coarse RAS 2.632 2.287 2.527 6.7 17.5 61.8 10.8

48 MO 5% Coarse RAS 2.632 2.281 2.527 7.0 17.8 60.9 10.8

49 MO 5% Coarse RAS 2.632 2.284 2.527 6.8 17.6 61.4 10.8

50 MO 5% Coarse RAS 2.632 2.274 2.527 7.2 18.0 59.8 10.8

51 IN 15% RAP 2.647 2.301 2.468 6.8 18.3 63.0 11.5

52 IN 15% RAP 2.647 2.292 2.468 7.1 18.6 61.6 11.5

53 IN 15% RAP 2.647 2.299 2.468 6.8 18.4 62.7 11.5

54 IN 3% RAS&HMA 2.618 2.279 2.448 6.9 18.3 62.4 11.4

55 IN 3% RAS&HMA 2.618 2.277 2.448 7.0 18.4 62.1 11.4

56 IN 3% RAS&HMA 2.618 2.285 2.448 6.7 18.1 63.3 11.5

57 IN 3% RAS&HMA 2.618 2.275 2.448 7.1 18.5 61.7 11.4

58 IN 3% RAS&HMA 2.618 2.276 2.448 7.0 18.5 61.9 11.4

59 IN 3% RAS&WMA 2.618 2.299 2.463 6.6 17.6 62.3 11.0

60 IN 3% RAS&WMA 2.618 2.293 2.463 6.9 17.8 61.4 10.9

61 IN 3% RAS&WMA 2.618 2.294 2.463 6.9 17.8 61.4 10.9

62 IN 3% RAS&WMA 2.618 2.294 2.463 6.9 17.8 61.4 10.9

63 IN 3% RAS&WMA 2.618 2.296 2.463 6.8 17.8 61.7 11.0

Viscosity (η)

Binder viscosities are calculated from DSR tests results through Equation 16 The procedures

to test high temperature per**for**mance grade **of** RTFO aged binder were applied. Binder shear

modulus and phase angle values were observed at temperatures ranging from 58°C to 82°C with

increments **of** 6°C . Three or four viscosity values were tested **for** each type **of** binder. The A-

VTS method is used to predict the binder viscosities at the interested temperatures which are the

temperatures that the dynamic moduli **of** compacted samples were tested. The A-VTS method

assumes that the binder viscosity is linearly related to temperature on a log-log to log scale. The

expression **of** the method is presented in Equation 17. The VTS coefficients, A and VTS, are

summarized in Table 17 and graphically presented in Figure 36.

69

| |

where η = viscosity (Poise),

| |= binder complex shear modulus (Pa), and

δ = phase angle.

Equation 16

where A, VTS = VTS coefficients,

t r = temperature (°Rankin), and

η = viscosity (centipoises).

Equation 17

Table 17: VTS Coefficients **of** Recovered **Asphalt** Binder

Mix Number Project Description A VTS

BC-21

5% Mfr. RAS 10.53205 -3.50984

BC-22 MN 5% Tear-**of**f RAS 10.88701 -3.63714

BC-23 30% RAP 11.05463 -3.70279

BC-24

0% RAS 11.05398 -3.69434

BC-25 4% RAS 10.5888 -3.52328

IA

BC-26 5% RAS 10.35324 -3.43054

BC-27 6% RAS 9.783821 -3.22009

BC-28

15% RAP 10.92817 -3.64293

BC-29 MO 5% Fine RAS 9.692357 -3.18057

BC-30 5% Coarse RAS 9.842163 -3.23768

BC-31

15% FRAP 10.96405 -3.65855

BC-32 IN 3% RAS&HMA 10.77171 -3.58458

BC-33 3% RAS&WMA 10.83753 -3.60935

70

Log(log(η))

0.86

0.84

0.82

0.80

0.78

0.76

0.74

0.72

0.70

2.77 2.78 2.79 2.80 2.81

Log(Tr)

MN-5%Mfr.RAS

MN-5%Tear-**of**f RAS

MN-30%RAP

IA-0%RAS

IA-4%RAS

IA-5%RAS

IA-6%RAS

MO-15%RAP

MO-5%Fine RAS

MO-5%Coarse RAS

IN-15%RAP

IN-3%RAS&HMA

IN-3%RAS&WMA

Figure 36: VTS Curves **of** Recovered **Asphalt** Binder

Complex Shear **Modulus** (G*)

DSR frequency sweep tests were per**for**med at multiple temperatures and frequencies. Binder

complex shear modulus master curves are developed by shifting G* values at different

temperatures to a reference temperature using shift factors (a(T)). The selected reference

temperatures are the interested temperatures, 4°C , 21°C , and 37°C . Figure 37 shows the actual

observed G* values **for** binder extracted from Iowa 0% RAS mix. The G* curves are horizontally

moved by factoring the actual testing frequencies with a(T) to achieve a smooth curve as shown

in Figure 38. Figure 37 and Figure 38 provide an example **of** the master curve construction

process. Master curves **for** other recovered binders were constructed and included in the

Appendix. The a(T) values at 37°C are summarized in Table 18. At reference temperature, the

corresponding frequencies **of** G* values are the actual testing frequencies. It is not necessary to

factor the frequencies at the reference temperature. There**for**e, the shift factor at the reference

temperature is equal to 1. To calculate the shift factors **for** 4°C or 21°C reference temperatures,

simply divide each shift factor **for** the 37°C reference temperature by the shift factor at 4°C or

21°C **for** the 37°C reference temperature. Lab G* tests were not per**for**med at 4°C because it

takes significantly longer time to lower the water bath temperature to 4°C than other

71

G*, Pa

G*, Pa

temperatures. As shown in Figure 39, the log shift factor values are linearly correlated to

temperature. The shift factor at 4°C is estimated **for** each recovered binder. The G* used **for** E*

predictive models is the corresponding G* **of** a particular frequency and temperature on the

master curve.

1.00E+09

1.00E+08

1.00E+07

1.00E+06

1.00E+05

1.00E+04

0.01 0.1 1 10 100

Frequency, Hz

9C

13C

21C

29C

37C

Figure 37: Lab Tested G* Values **of** **Asphalt** Binder Recovered from Iowa 0% RAS Mix

1E+09

100000000

10000000

1000000

100000

9C

13C

21C

29C

37C

10000

0.01 0.1 1 10 100 1000 10000 100000

Frequency, Hz

Figure 38: G* Master Curve **for** **Asphalt** Binder Recovered from Iowa 0% RAS Mix

(Reference Temperature is 37ºC )

72

Log(a(T))

3.5

3

2.5

2

1.5

1

0.5

0

0 10 20 30 40

Temperature, °C

Figure 39: Shift Factors **for** Mix BC-25

Table 18: G* Shift Factors **for** Recovered Binders at Reference Temperature **of** 37 ºC

Mix Number A(4ºC) A(9ºC) A(13ºC) A(21ºC) A(29ºC) A(37ºC)

BC-21 2243 736 550 56 6.7 1

BC-23 3172 1700 550 55 7.0 1

BC-24 4804 1400 480 50 6.5 1

BC-25 5666 1600 550 52 6.0 1

BC-27 2972 908 550 55 7.0 1

BC-28 6638 3000 1000 80 8.5 1

BC-29 12066 3000 900 90 8.0 1

BC-30 4804 3500 1200 95 8.0 1

BC-31 7278 2000 650 60 7.0 1

BC-32 8674 2500 700 60 7.5 1

BC-33 7667 2000 700 65 7.5 1

Phase Angle (δ)

**Models** to estimate the value **of** phase angle are developed using the same method as the

a**for**ementioned method to estimate G*. Figure 40 shows an example **of** the phase angle master

curves at reference temperature equal to 4ºC , 21ºC , and 37ºC . The determined phase angle shift

factors are summarized in Table 19.

73

Phase Angle

75

65

55

45

35

25

15

37C

4C

21C

-7 -5 -3 -1 1 3 5 7

Frequency, Hz

Figure 40: Phase Angle Master Curves **for** **Asphalt** Binder Recovered from Iowa 0% RAS

Mix

Table 19: Phase Angle Shifting Factors **for** Recovered Binders at Reference Temperature

**of** 37 ºC

Mix Number A(9ºC) A(13ºC) A(21ºC) A(29ºC) A(37ºC) A(4ºC)

BC-21 11162 5500 280 15 1 56396

BC-23 15000 3900 250 15 1 39709

BC-24 10000 2600 160 12 1 49180

BC-25 19000 4000 200 14 1 95693

BC-27 17585 8000 350 16 1 96286

BC-28 22000 5500 250 14 1 72175

BC-29 75000 15000 400 18 1 511328

BC-30 120000 22000 600 20 1 49180

BC-31 17000 4000 220 14 1 91124

BC-32 25000 5500 250 16 1 139583

BC-33 30000 6500 270 15 1 173797

Witczak Model

The Witczak models are developed **for**m **of** a sigmoid function. The basic **for**m **of** the

sigmoid function is shown in Equation 18 The shape **of** the sigmoid function is controlled by the

four fitting parameters: δ, α, β, and γ. In this function, δ is the smallest E* value. In a scenario

that HMA is subjected to a very high temperature and a slow moving traffic, the E* **of** the HMA

74

is very close to δ. In this situation, the stiffness **of** asphalt binder is very low which the stiffness

**of** HMA is governed by the aggregate and mixture volumetric properties. Equation 19 is the

developed **for**m **of** δ in the 1999 Witczak Model. In the 2006 Witczak Model, the **for**m **of** δ is

written as Equation 20 The value **of** δ + α is the theoretical largest E*. There**for**e, α represents

the largest change **of** E* that a HMA pavement can have. The developed **for**ms **of** α **for** 1999 and

2006 Witczak models are shown in Equation 21 and Equation 22, respectively. Parameter δ and

δ + α define the lower and upper bounds **of** the sigmoid curve. Parameter β and γ are empirical

constants that are used to define the shape **of** the curve.

| |

Equation 18

where | | = dynamic modulus,

reduced time, and

δ, α, β, γ = fitting parameters.

( )

where = percent mass **of** aggregates passing through a #200 sieve,

= cumulative percent mass **of** aggregates retained on a # 4 sieve,

= air voids, and

= effective binder content by volume **of** the mix.

Equation 19

75

(| | )

(

( ))

where | | = dynamic shear modulus **of** the binder,

= cumulative percent mass **of** aggregates retained on a 3/8” sieve, and

, , , and = as previously defined.

Equation 20

where

= cumulative percent mass **of** aggregates retained on a¾” sieve, and

, and = as previously defined.

Equation 21

( )

where , , , and = as previously defined.

Equation 22

The independent variable t r is the multiplicative inverse **of** the reduced frequency (f r ). The

reduced frequency is the equivalent frequency **of** an E* value at reference temperature. Reduced

frequency is calculated using the real frequency factored by a shift factor (a(T)) which is

determined by the binder rheological properties using the viscosity-temperature superposition

method. There**for**e, the variable t r represents the binder stiffness effect on the mixture stiffness.

Because the asphalt binder stiffness is dependent on temperature and loading frequency, t r is also

a simulation factor **for** the temperature and traffic loading rate. In the 1999 Witczak Model, t r is a

function **of** the loading rate and the binder viscosity as shown in Equation 23 In the 2006

Witczak Model, the stiffness **of** asphalt binder is calculated from the binder complex shear

modulus and phase angle by Equation 24 Substitute t r in Equation 18 by Equation 23 and

76

Equation 24, a general **for**m **of** the Witczak model can be obtained in Equation 25 The values **of**

parameter b, g 1 , and g 2 are equal to -0.604414, -0.313351, and -0.393532 **for** the 1999 Witczak

Model. In the 2006 Witczak Model, the values **of** the three parameters, b, g 1 , and g 2 , are -0.7814,

-0.5785, and 0.8834, respectively.

where f = loading frequency,

η = asphalt binder viscosity,

a, b = fitting parameters, and

t r = as previously defined.

Equation 23

| |

where Φ = phase angle,

a, b = fitting parameters, and

t r , |G*| = as previously defined.

Equation 24

| |

Equation 25

where x 1 = frequency in the 1999 Witczak Model or binder complex shear modulus in

the 2006 Witczak Model,

x 2 = binder viscosity in the 1999 Witczak Model or phase angle in the 2006 Witczak

Model,

b, g 1 , g 2 = fitting parameters, and

|E*|, δ, α = as previously defined.

There**for**e, dummy variables can be added to the δ, α, b, g 1 and g 2 terms to change the shape

**of** the sigmoid function to match the laboratory tested E* values. The E* values **of** the control

mixes which contain 0% RAS are used to determine the coefficients **of** the 0%-RAS-effect

77

calibration variable D IN, D IA , D MN , and D MO in Equation 26 After the coefficients **of** D IN, D IA ,

D MN , and D MO were determined, Equation 26 can be used to calculate the predicted E* which the

prediction accuracy variability from project differences is eliminated. The values **of** the

coefficients in Equation 26 are determined through non-linear multiple variable regression **of** the

lab data; and the results are listed in Table 20 **for** the 1999 Witczak Model and Table 21 **for** the

2006 Witczak Model.

| |

Equation 26

where D IN = 1 **for** Indiana mixes and 0 **for** others,

D IA = 1 **for** Iowa mixes and 0 **for** others,

D MN = 1 **for** Minnesota mixes and 0 **for** others,

D MO = 1 **for** Missouri mixes and 0 **for** others,

Cδ IN , Cδ IA , Cδ MN , Cδ MO , Cα IN , Cα IA , Cα MN , Cα MO , Cb IN , Cb IA , Cb MN , Cb MO , Cg 1IN ,

Cg 1IA , Cg 1MN , Cg 1MO , Cg 2IN , Cg 2IA , Cg 2MN , Cg 2MO = coefficient **of** the dummy variable

D IN , D IA , D MN , and D MO , and

δ,α,|E*|, x 1 , x 2 , |G b *|,b, g 1 , g 2 = as previously defined.

78

Table 20: Regression Results **of** 0%-RAS-Effect Calibration Parameters **for** the 1999

Witczak Model

Parameter Estimation Standard Error P-value

Cδ IN -2.4475 3.21572 0.4488

Cδ IA -2.4136 2.18329 0.2709

Cδ MN -0.3767 1.56535 0.8102

Cδ MO -2.1956 1.56179 0.1621

Cα IN 2.41062 3.25415 0.461

Cα IA 2.45945 2.25627 0.2776

Cα MN 0.30519 1.68828 0.8568

Cα MO 2.14614 1.5788 0.1763

Cb IN -0.8283 0.60855 0.1773

Cb IA -0.4255 0.42872 0.3228

Cb MN 0.10558 0.5454 0.8468

Cb MO -0.7409 0.31634 0.0206

Cg 1IN -0.0531 0.05045 0.2962

Cg 1IA -0.0357 0.0524 0.4972

Cg 1MN -0.1367 0.12542 0.2776

Cg 1MO -0.0674 0.02645 0.0120

Cg 2IN 0.02603 0.04846 0.5927

Cg 2IA 0.05663 0.0487 0.2469

Cg 2MN -0.0917 0.12768 0.4737

Cg 2MO -0.0144 0.02681 0.5923

79

Table 21: Regression Results **of** 0%-RAS-Effect Calibration Parameters **for** the 2006

Witczak Model

Parameter Estimation Standard Error P-value

Cδ IN -2.084 1.61254 0.2

Cδ IA -4.4766 3.35436 0.1843

Cδ MN -0.8869 0.39381 0.0259

Cδ MO -1.4828 1.05076 0.1605

Cα IN 2.32134 1.81791 0.2053

Cα IA 3.92956 3.41124 0.2514

Cα MN 0.52512 0.4388 0.2335

Cα MO 1.87323 1.31158 0.1556

Cb IN 0.09357 0.52829 0.8599

Cb IA -6.6804 0.5422

Modified Witczak Model Predicted

**Dynamic** **Modulus**, psi

Modified Witczak Model Predicted

**Dynamic** **Modulus**, log(psi)

7.5

7.0

6.5

6.0

5.5

5.0

4.5

4.0

Minnesota 0% RAS

Minnesota 5% RAS

Iowa 0% RAS

Iowa 4% RAS

Iowa 5% RAS

Iowa 6% RAS

Missouri 0% RAS

Missouri 5% RAS

Indiana 15% FRAP HMA

Indiana 3% RAS

Line **of** Equality

4 5 6 7 8

**Dynamic** **Modulus** Lab Results, log(psi)

Figure 41: Lab Tested vs. 1999 Witczak Model Predicted E* Values Calibrated **for** 0%-

RAS-Effect on Logarithm Scale

3500000

3000000

2500000

2000000

1500000

1000000

500000

Minnesota 0% RAS

Minnesota 5% RAS

Iowa 0% RAS

Iowa 4% RAS

Iowa 5% RAS

Iowa 6% RAS

Missouri 0% RAS

Missouri 5% RAS

Indiana 15% FRAP HMA

Indiana 3% RAS

Line **of** Equality

0

0 1000000 2000000 3000000 4000000

**Dynamic** **Modulus** Lab Results, psi

Figure 42: Lab Tested vs. the 1999 Witczak Model Predicted E* Values Calibrated **for** 0%-

RAS-Effect on Normal Scale

81

Modified Witczak Model Predicted

**Dynamic** **Modulus**, psi

Modified Witczak Model Predicted

**Dynamic** **Modulus**, log(psi)

7.5

7.0

6.5

6.0

5.5

5.0

Minnesota 0% RAS

Minnesota 5% RAS

Iowa 0% RAS

Iowa 4% RAS

Iowa 6% RAS

Missouri 0% RAS

Missouri 5% RAS

Indiana 15% FRAP HMA

Indiana 3% RAS

Line **of** Equality

4.5

4.0

4 5 6 7 8

**Dynamic** **Modulus** Lab Results, log(psi)

Figure 43: Lab Tested vs. the 2006 Witczak Model Predicted E* Values Calibrated **for** 0%-

RAS-Effect on Logarithm Scale

3500000

3000000

2500000

2000000

1500000

Minnesota 0% RAS

Minnesota 5% RAS

Iowa 0% RAS

Iowa 4% RAS

Iowa 6% RAS

Missouri 0% RAS

1000000

Missouri 5% RAS

500000

0

0 1000000 2000000 3000000 4000000

**Dynamic** **Modulus** Lab Results, psi

Figure 44: Lab Tested vs. the 2006 Witczak Model Predicted E* Values Calibrated **for** 0%-

RAS-Effect on Normal Scale

82

Modified Witczak Model Predicted

**Dynamic** **Modulus**, log(psi)

Let δ c , α c , b c , g 1c , and g 2c represent the calibrated δ, α, b, g 1 , and g 2 terms identified in

previous steps. Variables that represent different RAS contents are added to the δ c , α c , b c , g 1c , and

g 2c terms to simulate the effects **of** RAS content. Lab tested E* values **for** each level **of** RAS

content are used to determine the coefficients **of** the RAS effect variable D 3% , D 4% , D 5% , and D 6%

in Equation 27 The results **of** the regression analyses are shown in Table 22 and Table 23 **for** the

1999 and 2006 Witczak models, respectively. The prediction accuracies **of** modified Witczak

models are shown in Figure 45 through Figure 48 on both normal and logarithm scales. The

scatters on Figure 45 through Figure 48 are concentrated along the line **of** equality indicating the

modified models have high accuracy **of** prediction. The modified 1999 Witczak Model achieves

an R 2 value **of** 0.99 on a logarithm scale and 0.98 on a normal scale. The corresponding Se/Sy

values are 0.11 and 0.15 **for** the logarithm and normal scales, respectively. The R 2 **of** the

modified 2006 Witczak Model is 0.99 on a logarithm scale or 0.98 on a normal scale. The Se/Sy

value is 0.08. According to Table 10, both the modified 1999 and 2006 Witczak models arrive at

excellent goodness-**of**-fit.

7.5

7.0

6.5

6.0

5.5

5.0

Line **of** Equality

4.5

4.0

4 5 6 7 8

**Dynamic** **Modulus** Lab Results, log(psi)

Figure 45: Lab Tested vs. Modified 1999 Witczak Model Predicted E* Values on

Logarithm Scale

83

Modified Witczak Model

Predicted **Dynamic** **Modulus**,

log(psi)

Modified Witczak Model Predicted

**Dynamic** **Modulus**, psi

3500000

3000000

2500000

2000000

1500000

Line **of** Equality

1000000

500000

0

0 1000000 2000000 3000000 4000000

**Dynamic** **Modulus** Lab Results, psi

Figure 46: Lab Tested vs. Modified 1999 Witczak Model Predicted E* Values on Normal

Scale

7.5

7

6.5

6

5.5

Line **of** Equality

5

4.5

4

4 5 6 7 8

**Dynamic** **Modulus** Lab Results, log(psi)

Figure 47: Lab Tested vs. Modified 2006 Witczak Model Predicted E* Values on

Logarithm Scale

84

Modified Witczak Model Predicted

**Dynamic** **Modulus**, log(psi)

3500000

3000000

2500000

2000000

1500000

1000000

Line **of** Equality

500000

0

0 1000000 2000000 3000000 4000000

**Dynamic** **Modulus** Lab Results, log(psi)

Figure 48: Lab Tested vs. Modified 2006 Witczak Model Predicted E* Values on Normal

Scale

| |

Equation 27

where D 3% = 1 **for** mixes containing 3% RAS and 0 **for** others,

D 4% = 1 **for** mixes containing 4% RAS and 0 **for** others,

D 5% = 1 **for** mixes containing 5% RAS and 0 **for** others,

D 6% = 1 **for** mixes containing 6% RAS and 0 **for** others,

Cδ 3% , Cδ 4% , Cδ 5% , Cδ 6% , Cα 3% , Cα 4% , Cα 5% , Cα 6% , Cβ 3% , Cβ 4% , Cβ 5% , Cβ 6% , Cγ 3% ,

Cγ 4% , Cγ 5% , Cγ 6% , Cc 3% , Cc 4% , Cc 5% , Cc 6% = coefficient **of** the dummy variable D 3% ,

D 4% , D 5% , and D 6% , and

| |, | | δ α β γ as previously defined.

85

Table 22: Regression Results **of** RAS-Effect Calibration Parameters **for** the 1999 Witczak

Model

Parameter Estimation Standard Error P-value

Cδ 3% -1.6934 3.43166 0.6221

Cδ 4% 2.338807 0.346263

**of** the 1999 Witczak model. The p-values **of** the g 2 coefficients except **for** Cg2 4% are greater than

0.05. There is not an obvious trend in the p-values. Although the standard error is very small,

Cg2 5% is still not a significant factor. This indicates that the RAS content may not have an effect

on the parameter g 2 . The conclusions need to be verified by a larger sample space.

Table 23: Regression Results **of** RAS-Effect Calibration Parameters **for** the 2006 Witczak

Model

Parameter Estimation Standard Error P-value

Cδ 3% 1.56497 0.540942 0.0041

Cδ 4% 0.60657 1.63964 0.7120

Cδ 5% 0.83865 1.093461 0.4434

Cδ 6% 2.182726 0.907241 0.0175

Cα 3% -1.95661 0.618857 0.0017

Cα 4% -0.63047 1.672241 0.7068

Cα 5% -0.8366 1.116441 0.4539

Cα 6% -0.82806 0.230407 0.0005

Cb 3% -0.52857 1.046937 0.6141

Cb 4% -1.81861 1.567145 0.2479

Cb 5% 0.574334 0.99932 0.5657

Cb 6% 5.866697 1.676873 0.0006

Cg1 3% -0.17666 0.094207 0.0618

Cg1 4% -0.00774 0.970961 0.9937

Cg1 5% -0.06169 0.250851 0.8058

Cg1 6% -0.07247 1.35486 0.9574

Cg2 3% 0.848671 0.509028 0.0966

Cg2 4% 1.1913 0.97377 0.2233

Cg2 5% -0.01117 0.373595 0.9762

Cg2 6% -2.5251 0.569046 0.1099

Statistics in Table 23 show that the coefficients having a p-value greater than 0.05 include

Cδ 3% , Cδ 6% , Cα 3% , Cα 6% , and Cb 6% . The general p-value trend **for** the δ, α, and b coefficients are

87

decreasing with increasing RAS content. There are no distinct trends **for** the p-values **of** the g 1

and g 2 coefficients. This indicates that RAS content less than 5% may not result in significant

decrease in the prediction accuracy **of** the 2006 Witczak Model. Adding shingles to HMA may

not change the g 1 and g 2 parameters in the model.

Hirsch Model

The Hirsch model is developed from the Hirsch’s law **of** mixture. The basic equation is

Equation 28 The model contains four empirical constants, E a , p 0 , p 1 , and p 2 . The values **of** the

four constants determined by Christensen (2003) are 4,200,000, 20, 0.58, and 650 **for** E a , p 0 , p 1 ,

and p 2 , respectively. Dummy variables which are used to simulate different projects are added to

the four constants in order to match the lab testing results. The 0%-RAS-effect calibration

equations **for** E a , p 0 , p 1 , and p 2 are shown in Equation 29 through Equation 32 Lab tested E*

values **for** mixes containing 0% RAS are used to determine the value **of** each coefficient. The

regression results are shown in Table 24. Figure 49 shows the prediction accuracies **of** the

calibrated Hirsch Model. There are no distinct linear trend lines **for** different projects. Variables

are added to the calibrated E a , p 0 , p 1 , and p 2 to account **for** the effects **of** the RAS. The modified

predicted E* values are calculated by Equation 28 with modified E a , p 0 , p 1 , and p 2 as shown in

Equation 33 to Equation 36 Lab E* values **for** each RAS content are used **for** regression **of** the

modified Hirsch function. The coefficients **of** the dummy variables are determined and

summarized in Table 25. Figure 50 shows the lab tested E* vs. the predicted E* from the

modified Hirsch model. Data points on Figure 50 are concentrated along the line **of** equality. The

R 2 **of** the modified Hirsch model is 0.97 and the Se/Sy value is 0.19 on a normal scale. On a

logarithm scale, the model achieves R 2 value **of** 0.51 and Se/Sy value **of** 0.76. According to

Table 10, the goodness-**of**-fit **for** the modified Hirsch model is excellent on normal scale and fair

on logarithm scale.

Equation 28

88

where Ec = mixture modulus,

Ea = aggregate modulus,

Em = mastic modulus,

Va’ = volume fraction **of** aggregate excluding the contact volume and mineral filler,

Vm = volume fraction **of** mastic,

Vv = volume fraction **of** air voids,

VMA’ = voids in mineral aggregate,

VFM = voids filled by mastic, and

P 0 , P 1 , P 2 = empirical constant.

Equation 29

where Eac = 0%-RAS-effect calibrated Ea,

D IN = 1 **for** Indiana mixes and 0 **for** others,

D IA = 1 **for** Iowa mixes and 0 **for** others,

D MN = 1 **for** Minnesota mixes and 0 **for** others,

D MO = 1 **for** Missouri mixes and 0 **for** others, and

CEa IN , CEa IA , CEa MN , CEa MO = coefficient **of** the dummy variable D IN , D IA , D MN , and

D MO .

Equation 30

where P 0 c = 0%-RAS-effect calibrated P 0 ,

CEa IN , CEa IA , CEa MN , CEa MO = coefficient **of** the dummy variable D IN , D IA , D MN , and

D MO , and

D IN , D IA , D MN , D MO = as previously defined.

where P 1 c = 0%-RAS-effect calibrated P 1 ,

Equation 31

89

CP1 IN , CP1 IA , CP1 MN , CP1 MO = coefficient **of** the dummy variable D IN , D IA , D MN , and

D MO

D IN , D IA , D MN , D MO = as previously defined.

where P 2 c = 0%-RAS-effect calibrated P 2 ,

Equation 32

CP2 IN , CP2 IA , CP2 MN , CP2 MO = coefficient **of** the dummy variable D IN , D IA , D MN , and

D MO

D IN , D IA , D MN , D MO = as previously defined.

Table 24: Regression Results **of** 0%-RAS-Effect Calibration Parameters **for** Hirsch 2006

Model

Parameter Estimation Standard Error P-value

CEa IN 0.090722 584201.6 1

CEa IA -0.05654 571286.4 1

CEa MN -0.10356 424926.4 1

CEa MO 0.194212 276180.1 1

CP0 IN 249.0332 367.5947 0.4982

CP0 IA -23.3469 272.2187 0.9317

CP0 MN -3.91492 218.532 0.9857

CP0 MO 139.2855 240.595 0.5627

CP1 IN 0.012657 0.079471 0.8735

CP1 IA 0.100167 0.064257 0.1193

CP1 MN 0.133187 0.052335 0.0110

CP1 MO 0.074322 0.036013 0.0392

CP2 IN 69.14189 437.4 0.8744

CP2 IA 2063.315 1300.127 0.1127

CP2 MN 3078.152 1540.125 0.0458

CP2 MO 755.1289 396.8387 0.0573

90

Modified Witczak Model Predicted **Dynamic**

**Modulus**, log(psi)

3,000,000

2,500,000

2,000,000

1,500,000

1,000,000

500,000

0

0 1000000 2000000 3000000

**Dynamic** **Modulus** Lab Results, log(psi)

Minnesota 0% RAS

Minnestota 5% RAS

Iowa 4% RAS

Iowa 6% RAS

Missouri 0% RAS

Missouri 5% RAS

Indiana 15% FRAP HMA

Indiana 3% RAS

Indiana 3% RAS WMA

Line **of** Equality

Figure 49: Lab Tested vs. Hirsch Predicted E* Values Calibrated **for** 0%-RAS-Effect

Equation 33

where P 0 c’ = modified P 0 ,

modified Ea,

D 3% = 1 **for** mixes containing 3% RAS and 0 **for** others,

D 4% = 1 **for** mixes containing 4% RAS and 0 **for** others,

D 5% = 1 **for** mixes containing 5% RAS and 0 **for** others,

D 6% = 1 **for** mixes containing 6% RAS and 0 **for** others,

CP0 3% , CP0 4% , CP0 5% , CP0 6% = coefficient **of** the dummy variable D 3% , D 4% , D 5% ,

and D 6% , and

P 0 c as previously defined.

91

Equation 34.

where P 1 c = modified P 1 ,

CP1 3% , CP1 4% , CP1 5% , CP1 6% = coefficient **of** the dummy variable D 3% , D 4% , D 5% , and

D 6% , and

D 3% , D 4% , D 5% , D 6% , P 1 c = as previously defined.

Equation 35

where P 2 c = modified P 2 ,

CP2 3% , CP2 4% , CP2 5% , CP2 6% = coefficient **of** the dummy variable D 3% , D 4% , D 5% ,

and D 6% , and

D 3% , D 4% , D 5% , D 6% , P 1 c as previously defined.

Equation 36

where Eac’ = modified Ea,

CEa 3% , CEa 4% , CEa 5% , CEa 6% = coefficient **of** the dummy variable D 3% , D 4% , D 5% ,

and D 6% , and

D 3% , D 4% , D 5% , D 6% , Eac = as previously defined.

Table 25: Regression Results **of** RAS-Effect Calibration Parameters **for** Hirsch Model

Parameter Estimation Standard Error P-value

CEa 3% 0.852332 650984 1

CEa 4% 0.298186 885596.7 1

CEa 5% 0 356120.7 1

CEa 6% 0.400577 1623160 1

CP0 3% -53.876 486.252 0.9118

CP0 4% 0.73575 416.533 0.9986

CP0 5% 659.784 364.327 0.0704

92

Modified Witczak Model Predicted

**Dynamic** **Modulus**, log(psi)

CP0 6% 22.6821 589.209 0.9693

CP1 3% 0.1109 0.09217 0.2291

CP1 4% 0.02706 0.09873 0.7840

CP1 5% 0.12435 0.05287 0.0188

CP1 6% 0.01392 0.13396 0.9172

CP2 3% 2324.44 1288.15 0.0714

CP2 4% 910.952 2422.94 0.7070

CP2 5% 5513.72 3011.19 0.0673

CP2 6% 0.852332 650984 1

3500000

3000000

2500000

2000000

1500000

1000000

Line **of** Equality

500000

0

0 1000000 2000000 3000000 4000000

**Dynamic** **Modulus** Lab Results, log(psi)

Figure 50: Lab Tested vs. Predicted E* Values **of** Modified Hirsch Model

The p-values **of** Ea coefficients in Table 25 that are equal to 1 indicating the all Ea

coefficients are not significant factors. The estimations **of** coefficient values are very small

compared to the value **of** Ea which is 4,200,000. Parameter Ea is the assumed aggregate modulus.

The addition **of** shingles in HMA does not change the modulus **of** aggregate. There is only one p-

value in Table 25 that is less than 0.05 indicating that the coefficients to simulate the shingle

effects are not significant factors. A RAS content which is smaller than 6% may not result in bias

in the Hirsch prediction **of** E* values **of** RAS mixtures.

93

MODIFIED MODEL EVALUATION

The a**for**ementioned R 2 and Se/Sy values **of** the modified Witczak and Hirsch models

indicate the three E* predictive models achieve excellent goodness-**of**-fit **for** this database

containing 1701 data points. This section discusses the prediction efficiencies **of** modified

Witczak and Hirsch models in terms **of** model accuracy and reliability. **Dynamic** modulus master

curves and the plots **of** laboratory versus predicted E* are constructed to evaluate the model

accuracy. Statistics **of** the dummy variable coefficients are analyzed to discuss the reliability **of**

each parameter estimation and the correlations **of** parameters.

Model Efficiency Evaluation

Laboratory dynamic modulus values are tested at different temperatures and frequencies. In

this section, the accuracies **of** modified Witczak and Hirsch models are evaluated at the

corresponding temperatures and frequencies. **Dynamic** modulus master curves are **of**ten used to

simulate HMA E* behavior over a wide range **of** temperatures. There**for**e, master curves are used

to discuss the model accuracies at different temperatures. The lab vs. predictve plots are

developed at each loading frequency to evaluate the model accuracies at different frequencies.

Witczak Model

**Dynamic** modulus master curves are constructed **for** mixes containing shingles in order to

evaluate the prediction accuracy **of** the modified Witczak models. A typical E* master curve has

three components: upper tail, lower tail, and linear range. At the two tails **of** the curve, E* values

are approaching a constant simulating extreme climate and traffic loading. The upper tail

simulates HMA behavior under a fast moving traffic in a very cold winter day. The lower tail

simulates the opposite situation. The accuracies **of** the model predicted master curve on the upper

and lower tails are related to the accuracies **of** predicting HMA permanent de**for**mation and

thermal cracking, respectively. In between **of** the two tails, the slope **of** the master curve

approaches a constant. The E* is changing with a constant rate on log to log scale. The accuracy

**of** this range is related to the prediction accuracy **of** asphalt fatigue cracking. The original and

modified 2006 and 1999 Witczak master curves in Figure 51 to Figure 59 con**for**m very closely

to the lab master curves at the upper tail. The differences between the upper tails **of** the original

and modified 1999 Witczak models and the modified 2006 Witczak Model are very small. The

94

**Dynamic** modulus E*, psi

original 2006 Witczak Model tends to overestimate E* values at every range. The master curves

**of** the 1999 Witczak **Models** are closer to the lab master curves than the 2006 Witczak models.

Compared to the original Witczak models, the accuracies **of** modified models are increased at the

upper tail and the linear range. However, Figure 51 to Figure 59 show low model accuracies on

the lower tail. On the lower tail, the modified 1999 Witczak Model achieves better match with

the lab curve **for** mix BC25, 26, 32, and 33. For the 2006 Witczak Model, the modified model

has increased accuracy on the lower tail **for** mix BC29, 30, 32, and 33. For other mixes,

modifications **of** original models do not increase the model accuracies. It should be noticed that

E* values at the lower tail is very small. Small differences in two sets **of** E* values can cause

significant difference in the lower tails **of** the developed master curves. In testing E* at high

temperatures, the variability in test results is large and causes the inaccurate prediction **of** E* at

lower tail **of** master curve.

10000000

1000000

100000

10000

1000

1E-10 0.000001 0.01 100 1000000 1E+10

Reduced time, sec

Figure 51: Witczak Model Master Curves **for** Minnesota 5% Mfr. RAS Mix (Mix BC21)

95

**Dynamic** modulus E*, psi

**Dynamic** modulus E*, psi

10000000

1000000

100000

10000

1000

100

10

1

1E-10 0.000001 0.01 100 1000000 1E+10

Reduced time, sec

Figure 52: Witczak Model Master Curves **for** Minnesota 5% Tear-**of**f RAS Mix (Mix BC22)

10000000

1000000

100000

10000

1000

100

1E-10 0.000001 0.01 100 1000000 1E+10

Reduced time, sec

Figure 53: Witczak Model Master Curves **for** Iowa 4% RAS Mix (Mix BC25)

96

**Dynamic** modulus E*, psi

**Dynamic** modulus E*, psi

10000000

1000000

100000

10000

1000

100

1E-10 0.000001 0.01 100 1000000 1E+10

Reduced time, sec

Figure 54: Witczak Model Master Curves **for** Iowa 5% RAS Mix (Mix BC26)

10000000

1000000

100000

10000

1000

100

1E-10 0.000001 0.01 100 1000000 1E+10

Reduced time, sec

Figure 55: Witczak Model Master Curves **for** Iowa 6% RAS Mix (Mix BC27)

97

**Dynamic** modulus E*, psi

**Dynamic** modulus E*, psi

10000000

1000000

100000

10000

1000

100

1E-10 0.000001 0.01 100 1000000 1E+10

Reduced time, sec

Figure 56: Witczak Model Master Curves **for** Missouri 5% Fine RAS Mix (Mix BC29)

10000000

1000000

100000

10000

1000

100

1E-10 0.000001 0.01 100 1000000 1E+10

Reduced time, sec

Figure 57: Witczak Model Master Curves **for** Missouri 5% Coarse RAS Mix (Mix BC30)

98

**Dynamic** modulus E*, psi

**Dynamic** modulus E*, psi

10000000

1000000

100000

10000

1000

100

10

1E-10 0.000001 0.01 100 1000000 1E+10

Reduced time, sec

Figure 58: Witczak Model Master Curves **for** Indiana 3% RAS&HMA Mix (Mix BC32)

10000000

1000000

100000

10000

1000

100

10

1E-10 0.000001 0.01 100 1000000 1E+10

Reduced time, sec

Figure 59: Witczak Model Master Curves **for** Indiana 3% RAS&WMA Mix (Mix BC33)

99

Model Predicted E*, psi

Model Predicted E*, psi

Figure 60 includes nine individual plots **of** the tested results vs. the 1999 Witczak predictions

**of** E* **for** the nine loading frequencies in laboratory testing. The data are plotted on a normal

scale. The variability in predicting E* increases as the predicted E* increases. The scatters **for**

the modified 1999 Witczak Model are closely distributed along the line **of** equality. The spreads

**of** scatters **for** the original 1999 Witczak Model are wider indicating the variability in prediction

accuracy **for** the original model is larger than that **for** the modified model. The linear trend lines

**of** the original model predictions has a slope greater than 1 showing that the original model tends

to overestimate the E* value. There effects **of** different frequencies on the prediction accuracies

are not be able to visually identify from the plots in Figure 60.

2.E+06

0.1 Hz

2.E+06

0.2 Hz

0.E+00

0.E+00

Lab E*, psi

2.E+06

0.E+00

0.E+00

Lab E*, psi

2.E+06

100

Model Predicted E*, psi

Model Predicted E*, psi

Model Predicted E*, psi

Model Predicted E*, psi

2.E+06

0.5 Hz

3.E+06

1 Hz

0.E+00

0.E+00

Lab E*, psi

2.E+06

0.E+00

0.E+00

Lab E*, psi

3.E+06

3.E+06

2 Hz

3.E+06

5 Hz

0.E+00

0.E+00

Lab E*, psi

3.E+06

0.E+00

0.E+00

Lab E*, psi

3.E+06

101

Model Predicted E*, psi

Model Predicted E*, psi

Model Predicted E*, psi

3.E+06

10 Hz

3.E+06

20 Hz

0.E+00

0.E+00

Lab E*, psi

3.E+06

0.E+00

0.E+00

Lab E*, psi

3.E+06

3.E+06

25 Hz

0.E+00

0.E+00

Lab E*, psi

3.E+06

Figure 60: Lab E* vs. Predicted E* **of** Witczak 1999 Model

The lab vs. prediction plots are prepared **for** the 2006 Witczak Model in Figure 61. The data

are plotted on a normal scale. The variability in predicting E* increases as the predicted E*

102

Model Predicted E*, psi

Model Predicted E*, psi

increases. The original model obtains heavily biased E* values with large variability. Compared

to the original model, the modified model has higher accuracy and precision. There effects **of**

different frequencies on the prediction accuracies are not be able to visually identify from the

plots in Figure 61.

4.5E+06

0.1 Hz

5.E+06

0.2 Hz

0.0E+00

0.0E+00

Lab E*, psi

4.5E+06

0.E+00

0.E+00

Lab E*, psi

5.E+06

103

Model Predicted E*, psi

Model Predicted E*, psi

Model Predicted E*, psi

Model Predicted E*, psi

5.E+06

0.5 Hz

5.E+06

1 Hz

0.E+00

0.E+00

Lab E*, psi

5.E+06

0.E+00

0.E+00

Lab E*, psi

5.E+06

5.E+06

2 Hz

5.E+06

5Hz

0.E+00

0.E+00

Lab E*, psi

5.E+06

0.E+00

0.E+00

Lab E*, psi

5.E+06

104

Model Predicted E*, psi

Model Predicted E*, psi

Model Predicted E*, psi

5.E+06

10 Hz

5.E+06

20 Hz

0.E+00

0.E+00

Lab E*, psi

5.E+06

0.E+00

0.E+00

Lab E*, psi

5.E+06

5.E+06

25 Hz

0.E+00

0.E+00

Lab E*, psi

5.E+06

Figure 61: Lab E* vs. Predicted E* **of** Witczak 2006 Model

The R 2 values in Table 26 provide numerical evaluation **of** the model accuracies at each

frequency level. Negative R 2 value means the differences between predicted and tested E* values

105

are larger than the variability **of** the lab E*, which indicates the model is significantly biased.

There**for**e, the original 2006 Witczak Model has significantly biased predictions **of** E*. The R 2

**for** the original 1999 Witczak Model tends to be increased when the frequency increases.

Calibration **of** the original Witczak models significantly improves predicting accuracy and

precision. The R 2 values **for** the modified Witczak model are greater than 0.95 at every

frequency level.

Table 26: Coefficient **of** Determination **of** the Witczak **Models**

R 2 Values

Frequency Witczak

1999

Modified Witczak

1999

Witczak

2006

Modified Witczak

2006

0.1 0.78 0.97 * 7 0.96

0.2 0.77 0.98 * 0.97

0.5 0.8 0.98 * 0.98

1 0.83 0.98 * 0.98

2 0.84 0.98 * 0.95

5 0.86 0.98 * 0.99

10 0.87 0.98 * 0.99

20 0.96 0.98 * 0.98

25 0.88 0.98 * 0.98

Hirsch Model

The upper tails **of** the Hirsch model master curves in Figure 62 to Figure 68 con**for**ms very

closely to the lab master curves. At the linear range, the original Hirsch model tends to

overestimate E* values. The modified Hirsch model achieves improved accuracy **for** mix BC21,

25, 29, 30, 32, and 33. At the lower tail, the original Hirsch model has overwhelming biased

predictions which can be more than 1000 times the E* values estimated from lab master curves.

The modified Hirsch Model has more accurate predictions at the lower tail **for** mix BC25. For

other mixes, the prediction accuracy **of** the modified Hirsch Model is equal to, or lower than that

**of** the original model.

7 * represents a very low coefficient **of** determination that the model becomes extremely unreliable.

106

**Dynamic** modulus E*, psi

**Dynamic** modulus E*, psi

10000000

1000000

Lab Results

Hirsch

100000

Modified Hirsch

10000

1000

100

1E-10 0.000001 0.01 100 1000000 1E+10

Reduced time, sec

Figure 62: Hirsch Model Master Curves **for** Mix BC21

10000000

1000000

100000

Lab Results

Hirsch

Modified Hirsch

10000

1000

100

1E-10 0.000001 0.01 100 1000000 1E+10

Reduced time, sec

Figure 63: Hirsch Model Master Curves **for** Mix BC25

107

**Dynamic** modulus E*, psi

**Dynamic** modulus E*, psi

10000000

1000000

Lab Results

Hirsch

Modified Hirsch

100000

10000

1000

1E-10 0.000001 0.01 100 1000000 1E+10

Reduced time, sec

Figure 64: Hirsch Model Master Curves **for** Mix BC27

10000000

1000000

Lab Results

Hirsch

Modified Hirsch

100000

10000

1000

1E-10 0.000001 0.01 100 1000000 1E+10

Reduced time, sec

Figure 65: Hirsch Model Master Curves **for** Mix BC29

108

**Dynamic** modulus E*, psi

**Dynamic** modulus E*, psi

10000000

1000000

100000

Lab Results

Hirsch

Modified Hirsch

10000

1000

100

1E-10 0.000001 0.01 100 1000000 1E+10

Reduced time, sec

Figure 66: Hirsch Model Master Curves **for** Mix BC30

10000000

1000000

100000

Lab Results

Hirsch

Modified Hirsch

10000

1000

100

10

1

1E-10 0.000001 0.01 100 1000000 1E+10

Reduced time, sec

Figure 67: Hirsch Model Master Curves **for** Mix BC32

109

**Dynamic** modulus E*, psi

10000000

1000000

100000

Lab Results

Hirsch

Modified Hirsch

10000

1000

100

10

1

1E-10 0.000001 0.01 100 1000000 1E+10

Reduced time, sec

Figure 68: Hirsch Model Master Curves **for** Mix BC33

Hirsch model lab-prediction plots are prepared in Figure 69. The plots show accurate

prediction **for** the Hirsch model. Data **for** both original and modified models closely confirm the

line **of** equality indicating the bias **of** predicted E* is small. The modification does not

significantly improve the accuracy **of** the Hirsch model. R 2 values in Table 27 indicate that the

modified Hirsch model has slightly higher coefficient **of** determination. The improvement in

prediction accuracy is primarily from the calibration **of** the project effects. The influence **of**

loading frequency on model prediction accuracy and precision is not being able to visually

identify from Figure 69.

110

Model Predicted E*, psi

Model Predicted E*, psi

Model Predicted E*, psi

Model Predicted E*, psi

2.E+06

0.1 Hz

2.E+06

0.2 Hz

0.E+00

0.E+00

2.E+06

Lab E*, psi

Lab vs. Hirsch

Lab vs. Modified Hirsch

Line **of** Equality

0.E+00

0.E+00

2.E+06

Lab E*, psi

Lab vs. Hirsch

Lab vs. Modified Hirsch

Line **of** Equality

2.E+06

0.5 Hz

3.E+06

1 Hz

0.E+00

0.E+00

2.E+06

Lab E*, psi

Lab vs. Hirsch

Lab vs. Modified Hirsch

Line **of** Equality

0.E+00

0.E+00

3.E+06

Lab E*, psi

Lab vs. Hirsch

Lab vs. Modified Hirsch

Line **of** Equality

111

Model Predicted E*, psi

Model Predicted E*, psi

Model Predicted E*, psi

Model Predicted E*, psi

2.5E+06

2 Hz

3.E+06

5 Hz

0.0E+00

0.0E+00

Lab E*, psi

2.5E+06

0.E+00

0.E+00

Lab E*, psi

3.E+06

Lab vs. Hirsch

Lab vs. Hirsch

Lab vs. Modified Hirsch

Lab vs. Modified Hirsch

Line **of** Equality

Line **of** Equality

3.E+06

10 Hz

3.E+06

20 Hz

0.E+00

0.E+00

Lab E*, psi

3.E+06

0.E+00

0.E+00

Lab E*, psi

3.E+06

Lab vs. Hirsch

Lab vs. Modified Hirsch

Line **of** Equality

Lab vs. Hirsch

Lab vs. Modified Hirsch

Line **of** Equality

112

Model Predicted E*, psi

3.E+06

25 Hz

0.E+00

0.E+00

Lab E*, psi

3.E+06

Lab vs. Hirsch

Lab vs. Modified Hirsch

Line **of** Equality

Figure 69: Lab E* vs. Predicted E* **of** Hirsch Model

Table 27: Coefficient **of** Determination **of** the Hirsch Model

Frequency

R2 Values

Hirsch Modified Hirsch

0.1 0.89 0.95

0.2 0.89 0.96

0.5 0.89 0.97

1 0.89 0.97

2 0.89 0.98

5 0.9 0.98

10 0.9 0.97

20 0.91 0.96

25 0.85 0.91

Parameter Evaluation **of** **Models**

Witczak 1999 Model

Figure 70 indicates that an increased δ in the 1999 Witczak Model needs to be used to predict

E* when more than 4% RAS is added to HMA. The δ calibration coefficients are positive **for** 4%,

113

5%, and 6% RAS contents. The δ calibration coefficient **for** RAS content **of** 3% is negative.

However, the standard error **for** 3% RAS is large indicating 3% RAS content may not change the

δ parameter in the predictive equation. Figure 42 indicates that a decreased α in the 1999

Witczak Model needs to be used to predict E* when more than 4% RAS is added to HMA.

Negative α calibration coefficients are obtained **for** 4%, 5%, and 6% RAS contents. The α

calibration coefficient **for** RAS content **of** 3% is positive. However, the standard error **for** 3%

RAS is large indicating 3% RAS content may not change the α parameter in the predictive

equation. Figure 43 shows the b parameter in the 1999 Witczak Model needs to be increased to

predict E* when more than 4% RAS is added to HMA. Positive b calibration coefficients are

obtained **for** 4%, 5%, and 6% RAS contents. The b calibration coefficient **for** RAS content **of** 3%

is negative. However, the standard error **for** 3% RAS is large indicating 3% RAS content may

not change the b parameter in the predictive equation. The g 1 and g 2 calibration coefficients in

Figure 44 **for** 3%, 5%, and 6% RAS contents are positive. The g 1 and g 2 calibration coefficients

**for** 4% RAS are negative. The standard errors **of** g 1 and g 2 calibration coefficient **for** 3% and 6%

RAS contents are large. The effects **of** 3% and 6% RAS contents on g 1 and g 2 parameters are not

able to be identified. There**for**e, the addition **of** shingles in HMA results in increased δ and

decreased α parameters. The effects on the g 1 and g 2 parameters are not significant. **Modification**

**of** the 1999 Witczak Model is recommended when a 4% or more RAS content is used.

4

3

2

1

4% RAS

5% RAS

6% RAS

0

-1

-2

-3

-4

-5

-6

3% RAS

Figure 70: δ Calibration Coefficient **for** the 1999 Witczak Model

114

6

5

4

3

2

1

0

-1

-2

-3

-4

3% RAS

4% RAS

5% RAS

6% RAS

Figure 71: α Calibration Coefficient **for** the 1999 Witczak Model

1.4

1.2

1

0.8

0.6

0.4

0.2

0

-0.2

-0.4

-0.6

-0.8

3% RAS

4% RAS

5% RAS

6% RAS

Figure 72: b Calibration Coefficient **for** the 1999 Witczak Model

115

0.1

0.05

3% RAS

5% RAS

6% RAS

0

-0.05

-0.1

-0.15

4% RAS

Figure 73: g 1 Calibration Coefficient **for** the 1999 Witczak Model

0.1

0.05

0

-0.05

3% RAS

5% RAS

-0.1

-0.15

6% RAS

-0.2

-0.25

4% RAS

Figure 74: g 2 Calibration Coefficient **for** the 1999 Witczak Model

Table 28 shows the correlations between the calibration coefficients. The correlation between

two coefficients is represented by a number ranging from -1 to 1. The absolute value **of** the

correlation ratio represents the degree **of** the correlation. An absolute value **of** 1 means the

correlation between two coefficients is perfectly linear; and a value **of** 0 means the two

coefficients are independent. A positive number indicates one coefficient increases when the

116

other coefficient is increased; and a negative number indicates the opposite. The correlation

ratios **for** coefficients **of** different RAS contents in Figure 46 are equal to zero indicating the

calibration coefficients **of** different RAS contents are independent. Strong correlations are found

within coefficients at each RAS content level. High correlation ratios **of** the δ and α coefficients

indicate that δ and α are linearly correlated. The b, g 1 , and g 2 coefficients **for** 3%, 4%, and 6%

RAS have approximately perfectly linear correlations with absolute values **of** correlation ratios

greater than 0.95. For 5% RAS, the coefficients are still correlated with a much lower correlation

ratio. The chart also indicates that increase **of** δ will result in decreases **of** α, g 1 , and g 2 and

increase **of** b. An increase **of** α causes decreases **of** b and increases **of** g 1 and g 2 . An increase **of** b

will cause decreases **of** g 1 and g 2 . An increased g 1 will cause an increased g 2 .

117

Table 29: Coefficient Correlation Chart **for** the 1999 Witczak Model

Table 28: Coefficient Correlation Chart **for** the 1999 Witczak Model

Cδ 3% Cδ 4% Cδ 5% Cδ 6% Cα 3% Cα 4% Cα 5% Cα 6% Cb 3% Cb 4% Cb 5% Cb 6% Cg1 3% Cg1 4% Cg1 5% Cg1 6% Cg2 3% Cg2 4% Cg2 5% Cg2 6%

Cδ 3% 1.00 0.00 0.00 0.00 -1.00 0.00 0.00 0.00 1.00 0.00 0.00 0.00 -0.99 0.00 0.00 0.00 -0.98 0.00 0.00 0.00

Cδ 4% 1.00 0.00 0.00 0.00 -1.00 0.00 0.00 0.00 1.00 0.00 0.00 0.00 -0.97 0.00 0.00 0.00 -0.96 0.00 0.00

Cδ 5% 1.00 0.00 0.00 0.00 -0.95 0.00 0.00 0.00 0.81 0.00 0.00 0.00 -0.36 0.00 0.00 0.00 -0.55 0.00

Cδ 6% 1.00 0.00 0.00 0.00 -1.00 0.00 0.00 0.00 1.00 0.00 0.00 0.00 -0.98 0.00 0.00 0.00 -0.98

Cα 3% 1.00 0.00 0.00 0.00 -1.00 0.00 0.00 0.00 0.99 0.00 0.00 0.00 0.98 0.00 0.00 0.00

Cα 4% 1.00 0.00 0.00 0.00 -1.00 0.00 0.00 0.00 0.97 0.00 0.00 0.00 0.97 0.00 0.00

Cα 5% 1.00 0.00 0.00 0.00 -0.63 0.00 0.00 0.00 0.51 0.00 0.00 0.00 0.74 0.00

Cα 6% 1.00 0.00 0.00 0.00 -1.00 0.00 0.00 0.00 0.99 0.00 0.00 0.00 0.99

Cb 3% 1.00 0.00 0.00 0.00 -0.98 0.00 0.00 0.00 -0.98 0.00 0.00 0.00

Cb 4% 1.00 0.00 0.00 0.00 -0.96 0.00 0.00 0.00 -0.95 0.00 0.00

Cb 5% 1.00 0.00 0.00 0.00 -0.12 0.00 0.00 0.00 -0.31 0.00

Cb 6% 1.00 0.00 0.00 0.00 -0.98 0.00 0.00 0.00 -0.97

Cg13% 1.00 0.00 0.00 0.00 0.99 0.00 0.00 0.00

Cg14% 1.00 0.00 0.00 0.00 0.97 0.00 0.00

Cg15% 1.00 0.00 0.00 0.00 0.60 0.00

Cg16% 1.00 0.00 0.00 0.00 0.99

Cg23% 1.00 0.00 0.00 0.00

Cg24% 1.00 0.00 0.00

Cg25% 1.00 0.00

Cg26% 1.00

118

2006 Witczak Model

The δ calibration coefficients are all positive values as shown in Figure 75. The α calibration

coefficients are all negative values as shown in Figure 76. The absolute value **of** the δ coefficient

**for** 6% RAS is greater than other RAS contents, while the absolute value **of** α coefficient is

approximately the same as that **of** 4% RAS and 5% RAS. The coefficients **for** 4% and 5% RAS

contents have large standard errors compared to the value **of** the coefficients indicating the

effects **of** 4% and 5% RAS contents on the parameter δ and α are not significant. The b

calibration coeffcicients in Figure 77 **for** 3% and 4% RAS contents are negative. The coefficient

values at 3%, 4%, and 5% RAS contents are small compared to their standard errors. The 6%

RAS has a significant positive effect on the b parameter in the model. Figure 78 show very

small g 1 calibration coefficients at 4%, 5%, and 6% RAS contents compared to their standard

errors. Adding shingles to HMA may not cause changes in the g 1 parameter. Figure 79 indicates

the g 2 calibration coefficient **for** 5% RAS is almost zero. The 6% RAS has a significant larger

negative calibration coefficient than other RAS contents. To summarize, adding shingles to

HMA increases the δ and decreases the α values in the 2006 Witczak Model. The g 1 parameter

does not affected by addition **of** shingles in HMA. **Modification** **of** the original model is

recommended when 6% or more RAS is used.

3.5

3

2.5

2

3% RAS

4% RAS

5% RAS

6% RAS

1.5

1

0.5

0

-0.5

-1

-1.5

Figure 75: δ Calibration Coefficient **for** the 2006 Witczak Model

119

1.5

1

0.5

0

-0.5

-1

-1.5

6% RAS

-2

-2.5

-3

3% RAS

4% RAS

5% RAS

Figure 76: α Calibration Coefficient **for** the 2006 Witczak Model

10

8

6% RAS

6

4

2

5% RAS

0

-2

-4

3% RAS 4% RAS

Figure 77: b Calibration Coefficient **for** the 2006 Witczak Model

120

1.5

1

0.5

0

-0.5

-1

-1.5

3% RAS

4% RAS

5% RAS

6% RAS

-2

Figure 78: g 1 Calibration Coefficient **for** the 2006 Witczak Model

3

2

1

3% RAS

4% RAS

0

-1

5% RAS

-2

-3

-4

6% RAS

Figure 79: g 2 Calibration Coefficient **for** the 2006 Witczak Model

Table 30 shows that the δ and α calibration coefficients are strongly correlated. An increased

δ will result in a decreased α. The δ coefficient is negatively correlated to the b coefficient. The α

coefficient is positively correlated to the g 1 coefficient. The coefficient b is negatively correlated

to the g 2 coefficient. Coefficients **of** different RAS contents are independent to each other.

121

Table 31: 2006 Witczak **Modification** Coefficient Correlation Table

Table 30: 2006 Witczak **Modification** Coefficient Correlation Table

Cδ 3% Cδ 4% Cδ 5% Cδ 6% Cα 3% Cα 4% Cα 5% Cα 6% Cb 3% Cb 4% Cb 5% Cb 6% Cg1 3% Cg1 4% Cg1 5% Cg1 6% Cg2 3% Cg2 4% Cg2 5% Cg2 6%

Cδ 3% 1.00 0.00 0.00 0.00 -0.99 0.00 0.00 0.00 0.33 0.00 0.00 0.00 -0.95 0.00 0.00 0.00 0.08 0.00 0.00 0.00

Cδ 4% 1.00 0.00 0.00 0.00 -1.00 0.00 0.00 0.00 0.26 0.00 0.00 0.00 -0.90 0.00 0.00 0.00 0.33 0.00 0.00

Cδ 5% 1.00 0.00 0.00 0.00 -0.96 0.00 0.00 0.00 0.44 0.00 0.00 0.00 -0.59 0.00 0.00 0.00 -0.29 0.00

Cδ 6% 1.00 0.00 0.00 0.00 -1.00 0.00 0.00 0.00 -0.14 0.00 0.00 0.00 -0.99 0.00 0.00 0.00 0.87

Cα 3% 1.00 0.00 0.00 0.00 -0.19 0.00 0.00 0.00 0.92 0.00 0.00 0.00 -0.23 0.00 0.00 0.00

Cα 4% 1.00 0.00 0.00 0.00 -0.25 0.00 0.00 0.00 0.89 0.00 0.00 0.00 -0.35 0.00 0.00

Cα 5% 1.00 0.00 0.00 0.00 -0.55 0.00 0.00 0.00 0.70 0.00 0.00 0.00 0.41 0.00

Cα 6% 1.00 0.00 0.00 0.00 0.21 0.00 0.00 0.00 0.99 0.00 0.00 0.00 -0.91

Cb 3% 1.00 0.00 0.00 0.00 -0.53 0.00 0.00 0.00 -0.91 0.00 0.00 0.00

Cb 4% 1.00 0.00 0.00 0.00 -0.64 0.00 0.00 0.00 -0.82 0.00 0.00

Cb 5% 1.00 0.00 0.00 0.00 -0.97 0.00 0.00 0.00 -0.98 0.00

Cb 6% 1.00 0.00 0.00 0.00 0.11 0.00 0.00 0.00 -0.60

Cg13% 1.00 0.00 0.00 0.00 0.14 0.00 0.00 0.00

Cg14% 1.00 0.00 0.00 0.00 0.09 0.00 0.00

Cg15% 1.00 0.00 0.00 0.00 0.92 0.00

Cg16% 1.00 0.00 0.00 0.00 -0.86

122

Hirsch Model

Regression statistics in Table 25 show that values **of** the Ea calibration coefficients are very

small with significantly large standard errors. The absolute values **of** the coefficients are less

than 1. Considering the value **of** Ea is 4,200,000 in the original Hirsch model, addition **of**

shingles in HMA does not change the assumed aggregate modulus. The p 0 calibration coefficient

**for** 5% RAS in Figure 80 is positive. However, the coefficients **for** other RAS contents are very

small. Figure 81 and Figure 82 show RAS has positive effects on the p 1 and p 2 parameters. The

effects are very small at 6% RAS content. To summarize, the addition **of** RAS in HMA does not

significantly decrease the prediction accuracy **of** the original Hirsch model.

1500

1000

500

0

-500

4% RAS

5% RAS

6% RAS

-1000

3% RAS

Figure 80: p 0 Calibration Coefficient **for** the Hirsch Model

0.25

0.2

0.15

3% RAS

4% RAS

5% RAS

6% RAS

0.1

0.05

0

-0.05

-0.1

-0.15

Figure 81: p 1 Calibration Coefficient **for** the Hirsch Model

123

10000

8000

6000

4000

3% RAS 4% RAS

5% RAS

2000

0

-2000

-4000

Figure 82: p 2 Calibration Coefficient **for** the Hirsch Model

124

CHAPTER 5: CONCLUSIONS AND RECOMMENDATIONS

The research was conducted to evaluate the accuracies **of** the commonly used dynamic

modulus (E*) predictive models when recycled asphalt shingles are used in producing asphalt

mixtures. The E* predictive models evaluated in this research are the 1999 Witczak Model, the

2006 Witczak Model, and the Hirsch Model. **Modification**s were proposed **for** the Witczak

models. Model parameter statistics indicate that the Hirsch Model is not sensitive to mixtures

RAS containing and thus modification **of** the Hirsch model is not necessary.

The mixes tested in this study were procured from demonstration projects **of** the National

Pooled Fund Study #1208 which was conducted **for** the purpose **of** evaluating the effects **of** RAS

on laboratory testing properties and field per**for**mances **of** asphalt mixtures. In the study, thirteen

mixes were produced **for** four different demonstration projects constructed by state agencies

including Indiana, Iowa, Minnesota, and Missouri. The Indiana mixes include two three percent

RAS mixes **of** which one **of** them used a foaming warm mix asphalt technology and a control

mix which contains 15 percent FRAP. The Iowa mixes include a control mix which does not

contain any RAS and three experimental mixes with four, five, and six percent RAS contents.

The Minnesota mixes include a control mix containing 30 percent FRAP, and two experimental

mixes containing five percent manufactured and tear-**of**f RAS, respectively. The Missouri mixes

include a control mix containing 15 percent RAP, a mix containing ten percent RAP and five

percent fine ground RAS, and a Mix containing ten percent RAP and five percent coarse ground

RAS. The asphalt used in the Missouri demonstration project contains ground tire rubber and a

vestenamer polymer to improve the binder per**for**mance grade from 64-22 to 70-22. Loose

mixtures were obtained in the field and compacted to test cylinders in the laboratory **for** dynamic

modulus testing. **Asphalt**s were recovered from the field mixes through a centrifugal extraction

method **for** the DSR tests. The DSR tests results were used to estimate the values **of** input

parameters regarding binder rheological properties. The laboratory E* values were compared

with the calculated E* values from the predictive models. A statistical analysis was per**for**med on

the accuracies **of** the models to determine if there were significant differences in mixes

containing different percentages **of** RAS from different demonstration projects. **Modification**s **of**

the original predictive models were made to change the empirically determined coefficients by

introducing dummy variables to consider the use **of** RAS. Non-linear multiple variable

regressions based on the least square method were per**for**med to determine the coefficients **of** the

125

dummy variables. A statistical analysis was conducted to evaluate the effectiveness **of** the

coefficients and their correlations. Based on the a**for**ementioned analysis, the following

conclusions are drawn in the ensuing sections.

Prediction Accuracies **of** the Original E* **Predictive** **Models**

The 1999 Witczak Model

The 1999 Witczak Model tends to overestimate E* values **for** mixes containing RAS. The

master curves constructed on the model predicted E* values closely confirm the master curves

constructed on the laboratory tested E* values at the low temperatures, while the master curves

diverge at the high temperatures. These results are in agreement with Clyne et al. [29] and Kim

et al. [30]. Birgisson et al. [31] indicated in their study on the influences **of** different binder

viscosity measuring methods on the accuracy **of** the 1999 Witczak Model leads to

underestimating E* values. However, this research shows a disagreement as the predictive

accuracy **of** the 1999 Witczak Model is significantly affected by the projects, RAS contents, and

environmental condition. Statistically significant differences were detected between every pair **of**

projects and RAS contents suggesting modification is needed to account **for** the effects **of** the

projects and shingles. Loading condition does not affect the model’s prediction accuracy. The

overall goodness-**of**-fit is statistically considered good.

The 2006 Witczak Model

The 2006 Witczak Model tends to overestimate the E* values. The master curves constructed

on the model predicted E* values show the E* values are overestimated at every temperature

range. The goodness-**of**-fit **of** the 2006 Witczak Model is fair. Statistically significant differences

in predicting accuracies were detected between every pair **of** projects. The statistical analysis

indicates the model has the same accuracy level **of** predicting E* values **for** mixes containing 0

percent RAS and four or five percent RAS. However, the predictive accuracy **for** mixes

containing four percent RAS is significantly different from mixes containing five percent RAS.

The predictive accuracy level **for** mixes containing six percent RAS is found to be the same as

mixes containing three or five percent RAS. However, significant difference in model accuracies

was detected between mixes containing three and five percent RAS. Significant differences were

found **for** other comparisons. Failure to detect significant differences in the a**for**ementioned

126

comparisons may be a result from variability in lab testing results. However, modification is

needed to account **for** the effects **of** RAS and projects.

The Hirsch Model

The Hirsch Model tends to overestimate the E* values at the high temperatures. Master

curves constructed by the Hirsch Model predictions closely con**for**m to the laboratory data at low

temperatures and diverge at high temperatures. The goodness-**of**-fit **of** the Hirsch Model is

excellent. Demonstration project factor is a significant factor affecting the predicting accuracy **of**

the model. Statistical differences in model accuracies **of** the Hirsch Model were detected between

mixes containing zero and four percent RAS, zero and five percent RAS, three and five percent

RAS, and four and five percent RAS. There is not a rational relationship between the prediction

accuracy and RAS content **for** the Hirsch Model.

Modified E* **Predictive** **Models**

The three modified E* predictive models have high accuracies **of** predicting at low and

intermediate temperatures and considerably lower accuracies at high temperatures. The modified

models have the same level **of** predictive accuracies under different loading rates.

The Modified 1999 Witczak Model

The calibrated modified 1999 Witczak Model is presented in Equation 37. The values **of** the

introduced parameters are listed in Table 32 and Table 33. The R 2 value **of** the model is

improved from 0.87 to 0.99 on a logarithm scale by the calibration.

| |

( )

Equation 37

127

Table 32: Project Effect Calibration Parameters **for** the Modified 1999 Witczak Model

Project δ α b g1 g2

Indiana -2.4475 2.41062 -0.8283 -0.0531 0.02603

Iowa -2.4136 2.45945 -0.4255 -0.0357 0.05663

Minnesota -0.3767 0.30519 0.10558 -0.1367 -0.0917

Missouri -2.1956 2.14614 -0.7409 -0.0674 -0.0144

Table 33: RAS Content Calibration Parameters **for** the Modified 1999 Witczak Model

RAS% δ α b g1 g2

0 0 0 0 0 0

3 -1.6934 1.7359 -0.0558 0.02851 0.0244

4 2.33881 -2.5261 0.63665 -0.0927 -0.2008

5 1.29883 -1.2563 0.48735 0.0227 0.01138

6 2.37178 -2.3721 0.91856 0.01253 -0.0229

The Modified 2006 Witczak Model

The calibrated modified 2006 Witczak Model is presented in Equation 38. The values **of** the

introduced parameters are listed in Table 34 and Table 35. The R 2 value **of** the model is

improved from 0.75 to 0.99 on a logarithm scale by the calibration.

(| | )

(

( ))

( )

| |

Equation 38

128

Table 34: Project Effect Calibration Parameters **for** the Modified 2006 Witczak Model

Project δ α b g1 g2

Indiana -2.084 2.32134 0.09357 0.16969 -0.4511

Iowa -4.4766 3.92956 -6.6804 0.3434 2.86933

Minnesota -0.8869 0.52512 -3.5158 0.04846 2.00793

Missouri -1.4828 1.87323 1.72603 0.08525 -1.012

Table 35: RAS Content Calibration Parameters **for** the Modified 2006 Witczak Model

RAS% δ α b g1 g2

0 0 0 0 0 0

3 1.56497 -1.9566 -0.5286 -0.1767 0.84867

4 0.60657 -0.6305 -1.8186 -0.0077 1.1913

5 0.83865 -0.8366 0.57433 -0.0617 -0.0112

6 2.18273 -0.8281 5.8667 -0.0725 -2.5251

The Modified Hirsch Model

The finalized modified Hirsch Model is presented in Equation 39 and Equation 40. The

values **of** the introduced parameters are listed in Table 36 and Table 37. The calibration **of** the

model improves the R 2 value from 0.90 to 0.97. The improvement **of** the R 2 value is primarily

from calibrations addressing the project effects.

| | [ ( )

| | ( )]

| |

| |

Equation 39

| |

Equation 40

129

Table 36: Project Effect Calibration Parameters **for** the Modified Hirsch Model

Project Ea p0 p1 p2

Indiana 0.09072 249.033 0.01266 69.1419

Iowa -0.0565 -23.347 0.10017 2063.32

Minnesota -0.1036 -3.9149 0.13319 3078.15

Missouri 0.19421 139.286 0.07432 755.129

Table 37: RAS Content Calibration Parameters **for** the Modified Hirsch Model

RAS% Ea p0 p1 p2

0 0 0 0 0

3 0.85233 -53.876 0.1109 2324.44

4 0.29819 0.73575 0.02706 910.952

5 0 659.784 0.12435 5513.72

6 0.40058 22.6821 0.01392 0.85233

Influences **of** RAS on Parameters **of** the E* **Predictive** **Models**

Adding Shingles to asphalt mixtures requires an increase in δ and b values and a decrease in

the α value in the 1999 and 2006 Witczak models **for** improved prediction **of** E* values. Strong

linear correlations exist in parameter δ, α and b. There are no rational relationships between the

RAS content and the parameters g1 and g2. Shingles do not have significant effects on the

parameter Ea, p0, p1, and p2 in the Hirsch Model.

Recommendations

A low RAS content **of** less than three percent does not require modification **of** the 1999

Witczak Model. When a RAS content **of** four percent or higher is used, it is recommended to

use the modified 1999 Witczak Model.

The modified 2006 Witczak Model is recommended to use when a mix contains six percent

RAS or more.

The δ term in the Witczak models should be increased and α term should be decreased

correspondently when RAS is used in asphalt mixture.

The b constant in the Witczak models should be increased **for** RAS.

The g1 and g2 constants in the Witczak models do not need to be modified **for** RAS.

130

The Hirsch Model does not need to be modified **for** shingles’ effects.

Different projects affect the calibration coefficients and need to be developed if the modified

models are used **for** other projects.

The modified models were developed from a limited database containing 13 different mixes.

The experiments were not specifically designed **for** the purposes **of** this research. Mixes

containing certain percentages **of** RAS such as three percent, four percent, and six percent

can be only found in one project. The mutual variability **of** the project and the certain RAS

contents cannot be determined. Future research should be conducted to verify the effects **of**

RAS on the 1999 and 2006 Witczak models as well as other E* predictive models that are

not included in this research. In addition, comprehensive research should be conducted to

investigate the accuracies **of** the E* predictive models when different methods are used to

obtain values **of** the input parameters such as the binder shear modulus, phase angle, and

viscosity. This includes developing a standardized procedure to calibrate the model input

parameters.

131

REFERENCES

[1] New Hampshire Department **of** Transportation, "Construction cost index,". vol. 2011,

2011.

[2] Pennsylvania Department Of Transportation, "Strategic recycling program fact sheet".

vol. 2011, 2006.

[3] D. W. Janisch and C. M. Turgeon, "Minnesota’s Experience Using Shingle Scrap in

Bituminous Pavements," Final Report, Minnesota Department **of** Transportation, Minnesota,

1996.

[4] J. D. Brock, From Ro**of**ing Shingles to Roads: Astec, 1998.

[5] Cali**for**nia Department Of Resources Recycling And Recovery, "**Asphalt** Ro**of**ing

Shingles Recycling,". vol. 2011, 2006.

[6] Ohio Department Of Transportation, "Revisions to the 2010 Construction & Material

Specifications,". vol. 2011, 2011.

[7] Construction Materials Recycling Association and U. S. Environmental Protection

Agency, "State Experience in Recycling **Asphalt** Shingles,". vol. 2011, 2011.

[8] J. Mallela, L. T. Glover, M. I. Darter, H. Von Quintus, A. Gotlif, M. Stanley, and S.

Sadasivam, "Guidelines **for** implementing NCHRP 1-37A ME design procedures in Ohio:

volume 1-summary **of** findings, implementation plan, and next steps," Columbus: Ohio

Department **of** Transportation, 2009-01-01 2009.

[9] J. Bari and M. W. Witczak, "Development **of** a New Revised Version **of** the Witczak E*

**Predictive** Model **for** Hot Mix **Asphalt** Mixtures," Journal **of** the Association **of** **Asphalt** Paving

Technologists, p. 385, 2006.

[10] D. W. Christensen, T. Pellinen and R. F. Bonaquist, "Hirsch Model **for** Estimating the

**Modulus** **of** **Asphalt** Concrete," Journal **of** the Association **of** **Asphalt** Paving Technologists,

2003.

[11] D. E. Newcomb, M. D. O. T. Administration, U. O. M. D. Civil, and M. Engineering,

Influence **of** Ro**of**ing Shingles on **Asphalt** Concrete Mixture Properties: Minnesota Dept. **of**

Transportation, Office **of** Research Administration, 1993.

[12] D. C. Trumbore, "Magnitude and source **of** air emissions from asphalt blowing

operations," Environmental Progress, vol. 17, pp. 53-59, 1998.

[13] J. Cory, "Shingle recycling slow to come: few ro**of**ing companies have the opportunity to

recycle shingles at an af**for**dable price," Remodeling, vol. 11, p. 120, 2003.

132

[14] D. Krivit, "Recycling Tear-Off **Asphalt** Shingles: Best Practices Guide," Construction

Materials Recycling Association (CMRA) 2007.

[15] United States. Environmental Protection Agency. Emission Standards And Engineering

Division, Standards support document, promulgated amendments to the national emission

standard **for** asbestos. Research Triangle Park, N.C.

Springfield, Va.: U.S. Environmental Protection Agency, Office **of** Air and Waste Management

National Technical In**for**mation Service [distributor, 1978.

[16] D. E. Watson, A. Johnson and H. R. Sharma, "Georgia's experience with recycled ro**of**ing

shingles in asphaltic concrete," Transportation Research Record: Journal **of** the Transportation

Research Board, vol. 1638, pp. 129--133, 1998.

[17] J. W. Button, D. Williams and J. A. Scherocman, "Ro**of**ing Shingles and Toner in

**Asphalt** Pavements," 1996.

[18] M. J. Watson, J. McGraw, E. Johnson, D. Linell, and S. Dai, "The effect **of** recycled

asphalt materials on hot mixed asphalt pavement per**for**mance," in Green Streets and Highways

2010: An Interactive Conference on the State **of** the Art and How to Achieve Sustainable

Outcomes - Proceedings **of** the Green Streets and Highways 2010 Conference Denver, CO,

United states, 2010, pp. 323-336.

[19] A. A. Cascione, R. Christopher Williams, W. G. Buttlar, S. Ahmed, B. Hill, D. S.

Haugen, and S. Gillen, "Laboratory Evaluation **of** Field Produced Hot Mix **Asphalt** Containing

Post-Consumer Recycled **Asphalt** Shingles and Fractionated Recycled **Asphalt** Pavement,"

**Asphalt** Paving Technology-Proceedings Association **of** **Asphalt** Technologists, vol. 80, p. 377,

2011.

[20] T. V. Scholz, "Preliminary Investigation **of** RAP and RAS in HMAC," 2010.

[21] C. W. Schwartz, "Evaluation **of** the Witcak **Dynamic** **Modulus** Prediction Model," in 84th

Annual Meeting **of** the Transportation Research Board Washington D.C., 2005.

[22] M. W. Witzcak, Simple per**for**mance test **for** superpave mix design: Transportation

Research Board, 2002.

[23] G. Garcia and M. Thompson, "HMA DYNAMIC MODULUS PREDICTIVE MODELS-

-AReview," Urbana, vol. 51, p. 61801, 2007.

[24] C. E. Dougan, C. D. O. T. Research, Materials, C. T. Institute, and U. O. C. S.

Engineering, E*-dynamic **Modulus**: Test Protocol: Problems and Solutions: Connecticut

Transportation Institute, School **of** Engineering, University **of** Connecticut, 2003.

[25] American Association **of** State Highway And Transportation Officials, "Standard Method

**of** Test **for** Determining **Dynamic** **Modulus** **of** Hot Mix **Asphalt** (HMA)," in AASHTO TP62-07,

2009.

133

[26] D. W. Christen and D. A. Anderson, "Interpretation **of** **Dynamic** Mechanical Test Data

**for** Paving Grade **Asphalt** Cements," Journal **of** the Association **of** **Asphalt** Paving Technologists,

1992.

[27] T. K. Pellinen and M. W. Witczak, "Stress Dependent Master Curve Construction **for**

**Dynamic** (Complex) **Modulus**," Journal **of** the Association **of** **Asphalt** Paving Technologists, p.

287, 2002.

[28] M. W. Mirza and M. W. Witczak, "Development **of** a Global Aging System **for** Short and

Long Term Aging **of** **Asphalt** Cements," Journal **of** the Association **of** **Asphalt** Paving

Technologists, 1995.

[29] T. R. Clyne, X. Li, M. O. Marasteanu, and E. L. Skok, "**Dynamic** and Resilient **Modulus**

**of** MN/DOT **Asphalt** Mixtures," University **of** Minnesota, Minneapolis MN/RC – 2003-09,

2003.

[30] Y. R. Kim, M. Momen and M. King, "Typical **Dynamic** Moduli **for** North Carolina

**Asphalt** Concrete Mixtures," North Carolina State University, Raleigh FHWA/NC/2005-03,

2005.

[31] B. Birgisson, G. Sholar and R. Roque, "Evaluation **of** a Predicted **Dynamic** **Modulus** **for**

Florida Mixtures," in 84th Annual Meeting **of** the Transportation Research Board Washington

D.C.: Transportation Research Board, 2005.

[32] F. O. Martinez and S. M. Angelone, "Evaluation **of** Different **Predictive** **Dynamic**

**Modulus** **Models** **of** **Asphalt** Mixtures Used in Argentina," in 88th Annual Meeting **of** the

Transportation Research Board Washington D.C., 2009.

[33] J. P. Serfass and J. Samanos, "Fiber-Modified **Asphalt** Concrete Characteristics,

Applications and Behavior," Journal **of** the Association **of** **Asphalt** Paving Technologists, p. 193,

1996.

[34] S. Wu, Q. Yue, N. Li, and H. Yue, "Effects **of** Fibers on the **Dynamic** Properties **of**

**Asphalt** Mixtures," Journal **of** Wuhan University **of** Technology(Materials Science Edition), pp.

733-736, 2007.

[35] D. Haugen, "National Pooled Fund Study #1208 Field Notes,", 2010.

[36] Li, X. and R. Christopher Williams, "A Practical **Dynamic** **Modulus** Testing Protocol,"

Journal **of** Testing and Evaluation, vol.40, 2012.

[37] N. Tran and K Hall, "Evaluating the **Predictive** Equation in Determining **Dynamic**

Moduli **of** Typical **Asphalt** Mixtures Used in Arkansas," Journal **of** the Association **Asphalt**

Paving Technologists, vol. 74, pp. 1-17, 2005.

134

APPENDIX A: DYNAMIC MODULUS RESULTS

Table 38: **Dynamic** **Modulus** Test Results **for** Mix BC-21

**Dynamic** **Modulus**, kPa

Mix BC-21, Minnesota Demonstration Project, 5% Mfr. RAS

Temp., C Freq., Hz Sample 1 Sample 2 Sample 3 Sample 4 Sample 5 CV, %

4 25 15763 15688 15505 15636 15745 0.66

4 20 15299 15365 15089 15291 15320 0.70

4 10 14228 14260 13929 14180 14304 1.04

4 5 13165 13172 12786 13075 13259 1.40

4 2 11760 11688 11342 11703 11929 1.83

4 1 10728 10734 10223 10672 10936 2.47

4 0.5 9727 9702 9188 9732 10005 3.07

4 0.2 8470 8528 7884 8549 8784 3.96

4 0.1 7600 7662 6984 7745 7907 4.65

21 25 7192 7118 7708 6544 6938 5.95

21 20 6828 6795 7301 6146 6656 6.14

21 10 5851 5784 6280 5230 5741 6.47

21 5 4985 4960 5345 4407 4886 6.83

21 2 3982 3991 4291 3479 3889 7.45

21 1 3355 3361 3590 2864 3214 8.16

21 0.5 2724 2767 3021 2386 2678 8.36

21 0.2 2210 2164 2347 1813 2033 9.56

21 0.1 1771 1767 1972 1508 1646 9.91

37 25 2412 2409 2514 2460 2246 4.16

37 20 2302 2277 2320 2235 2109 3.75

37 10 1847 1845 1816 1718 1652 4.88

37 5 1407 1413 1476 1374 1337 3.68

37 2 1042 1049 1069 974 947 5.18

37 1 833 842 778 689 680 10.04

37 0.5 632 622 651 576 574 5.63

37 0.2 519 493 461 404 399 11.70

37 0.1 382 451 350 303 298 17.69

135

Table 39: **Dynamic** **Modulus** Test Results **for** Mix BC-22

**Dynamic** **Modulus**, kPa

Mix BC-22, Minnesota Demonstration Project, 5% Tear-**of**f

Temp., C Freq., Hz Sample 1 Sample 2 Sample RAS 3 Sample 4 Sample 5 CV, %

4 25 16508 16642 16825 15743 16480 2.51

4 20 16040 16195 16390 15322 16050 2.53

4 10 14833 14682 15126 14278 14831 2.10

4 5 13569 13655 13692 13053 13523 1.91

4 2 11914 12004 11967 11557 11938 1.53

4 1 10704 10772 10679 10423 10768 1.34

4 0.5 9533 9521 9498 9371 9550 0.75

4 0.2 8009 8110 7965 7970 8137 1.00

4 0.1 6928 7000 6959 7050 7055 0.80

21 25 7280 6288 7217 8057 7211 8.70

21 20 6884 5751 7486 7390 6892 10.02

21 10 5949 4807 6360 6315 5931 10.69

21 5 5040 4222 5269 5282 5068 8.76

21 2 3985 3313 4150 4215 4035 9.19

21 1 3335 2744 3404 3496 3294 9.08

21 0.5 2598 2336 2816 2936 2791 8.69

21 0.2 2054 2048 1985 2124 2160 3.31

21 0.1 1636 1760 1594 1698 1785 4.76

37 25 2485 2137 2744 2482 2478 8.76

37 20 2345 2010 2558 2374 2335 8.51

37 10 1875 1477 1960 1840 1847 10.36

37 5 1410 1059 1530 1397 1461 13.28

37 2 954 687 1069 1034 965 15.95

37 1 651 449 726 728 745 18.65

37 0.5 488 337 604 540 547 20.14

37 0.2 351 253 427 356 357 17.85

37 0.1 197 136 266 341 342 35.16

136

Table 40: **Dynamic** **Modulus** Test Results **for** Mix BC-23

**Dynamic** **Modulus**, kPa

Mix BC-23, Minnesota Demonstration Project, 30% RAP

Temp., C Freq., Hz Sample 1 Sample 2 Sample 3 Sample 4 Sample 5 CV, %

4 25 15865 15771 15857 15846 15862 0.25

4 20 15390 15126 15480 15476 15434 0.96

4 10 14105 13937 14145 14127 14086 0.59

4 5 12807 12596 12811 12876 12825 0.85

4 2 11143 10937 11188 11145 11201 0.96

4 1 9909 9831 9908 9918 9897 0.36

4 0.5 8713 7737 9630 8720 8751 7.69

4 0.2 7325 5935 7694 7303 7951 10.76

4 0.1 6269 5072 6609 6244 6816 10.89

21 25 6421 5339 7141 6397 6386 10.15

21 20 6486 5070 6480 6137 6131 9.59

21 10 5551 4101 5459 5114 5087 11.36

21 5 4611 3434 4408 4217 4175 10.70

21 2 3524 2456 3354 3184 3230 12.99

21 1 2789 1866 2691 2547 2563 14.58

21 0.5 2064 1499 2226 2005 2012 13.94

21 0.2 1563 1146 1438 1506 1445 11.34

21 0.1 1215 891 1122 1173 1106 11.36

37 25 1711 1792 1812 1890 1870 3.90

37 20 1651 1654 1662 1781 1718 3.31

37 10 1274 1222 1264 1269 1316 2.63

37 5 912 828 958 952 1019 7.52

37 2 592 510 670 723 638 12.87

37 1 372 305 441 475 493 18.63

37 0.5 249 206 366 415 367 27.71

37 0.2 190 151 269 261 254 23.01

37 0.1 150 121 214 169 187 20.93

137

Table 41: **Dynamic** **Modulus** Test Results **for** Mix BC-24

**Dynamic** **Modulus**, kPa

Mix BC-24, Iowa Demonstration Project, 0% RAS

Temp., C Freq., Hz Sample 1 Sample 2 Sample 3 Sample 4 Sample 5 CV, %

4 25 15407 15309 15380 15385 15412 0.27

4 20 14990 14978 14997 14998 14990 0.05

4 10 13741 13961 13861 13865 13870 0.56

4 5 12853 12608 12724 12723 12692 0.69

4 2 11261 11157 11235 11242 11269 0.40

4 1 10158 10042 10131 10130 10166 0.49

4 0.5 9061 8987 9044 9047 9065 0.35

4 0.2 7674 7674 7685 7684 7673 0.08

4 0.1 6708 6709 6706 6709 6681 0.18

21 25 6426 7088 6687 7096 6091 6.49

21 20 6047 6689 6318 6715 5788 6.38

21 10 5097 5703 5348 5708 4872 6.91

21 5 4251 4826 4493 4819 4054 7.62

21 2 3280 3806 3502 3792 3111 8.80

21 1 2640 3131 2851 3123 2496 9.98

21 0.5 2110 2538 2306 2546 1991 10.85

21 0.2 1543 1931 1712 1919 1447 12.73

21 0.1 1203 1545 1355 1537 1122 14.15

37 25 2237 2782 2567 2814 2416 9.53

37 20 2098 2611 2340 2619 1995 12.29

37 10 1613 2040 1802 2042 1504 13.57

37 5 1218 1575 1382 1575 1132 14.71

37 2 820 1099 952 1093 776 15.83

37 1 576 793 680 786 537 17.37

37 0.5 435 596 512 588 413 16.52

37 0.2 295 407 359 403 282 16.81

37 0.1 219 297 262 294 212 15.67

138

Table 42: **Dynamic** **Modulus** Test Results **for** Mix BC-25

**Dynamic** **Modulus**, kPa

Mix BC-25, Iowa Demonstration Project, 4% RAS

Temp., C Freq., Hz Sample 1 Sample 2 Sample 3 Sample 4 Sample 5 CV, %

4 25 15336 15378 14973 15501 15570 1.51

4 20 15018 15082 14548 15084 15198 1.69

4 10 13813 13948 13393 14048 14318 2.45

4 5 13007 12921 12173 12959 13124 2.95

4 2 11521 11558 10721 11656 11849 3.78

4 1 10492 10452 9543 10577 11149 5.52

4 0.5 9480 9462 8716 9404 10236 5.69

4 0.2 8249 8275 7560 8710 8225 5.02

4 0.1 7387 7340 6549 7983 7323 6.97

21 25 7113 7027 7209 6477 6974 4.09

21 20 6948 6635 6689 6094 6633 4.72

21 10 5967 5704 5718 5129 5667 5.46

21 5 5175 4871 4783 4293 4812 6.63

21 2 4164 3883 3817 3327 3817 7.94

21 1 3532 3161 3210 2731 3162 9.03

21 0.5 2716 2627 2489 2506 2694 4.03

21 0.2 1992 2052 1833 2000 2059 4.59

21 0.1 1625 1639 1494 1694 1655 4.67

37 25 2161 2083 2100 1822 2161 6.80

37 20 1984 2001 2019 1734 1946 6.01

37 10 1539 1593 1515 1289 1587 8.30

37 5 1188 1184 1164 1046 1218 5.74

37 2 830 854 780 753 849 5.50

37 1 601 670 511 540 607 10.64

37 0.5 462 486 406 453 470 6.63

37 0.2 327 399 268 301 331 14.85

37 0.1 221 284 230 249 249 9.81

139

Table 43: **Dynamic** **Modulus** Test Results **for** Mix BC-26

**Dynamic** **Modulus**, kPa

Mix BC-26, Iowa Demonstration Project, 5% RAS

Temp., C Freq., Hz Sample 1 Sample 2 Sample 3 Sample 4 Sample 5 CV, %

4 25 12702 14036 12711 13034 12360 4.95

4 20 12391 13579 12348 12669 11917 4.93

4 10 11326 12446 11353 11675 11086 4.57

4 5 10766 11813 10009 10620 9653 7.83

4 2 9652 10391 8787 9303 8380 8.37

4 1 8723 9246 7643 8456 7787 7.94

4 0.5 7961 7805 7126 7562 7008 5.55

4 0.2 6757 6164 6131 6413 6379 3.94

4 0.1 5932 5294 5328 5573 5674 4.73

21 25 6276 5692 6891 6341 6258 6.76

21 20 6290 5347 6322 6063 5886 6.63

21 10 5128 4518 5582 5190 5182 7.47

21 5 4376 4032 4797 4427 4190 6.61

21 2 3502 3362 3577 3516 3521 2.29

21 1 2921 2769 2996 2938 2981 3.09

21 0.5 2396 2190 2355 2433 2781 8.90

21 0.2 2194 1836 1629 1947 1843 10.86

21 0.1 1823 1515 1292 1605 1542 12.23

37 25 2146 2181 2496 2297 2333 6.05

37 20 2158 2035 2332 2146 2008 6.00

37 10 1704 1604 1776 1785 1597 5.32

37 5 1341 1194 1403 1342 1420 6.64

37 2 969 811 981 1052 1051 10.09

37 1 748 592 681 818 814 13.07

37 0.5 544 416 609 588 732 19.71

37 0.2 430 330 417 446 509 15.11

37 0.1 290 248 380 401 353 19.08

140

Table 44: **Dynamic** **Modulus** Test Results **for** Mix BC-27

**Dynamic** **Modulus**, kPa

Mix BC-27, Iowa Demonstration Project, 6% RAS

Temp., C Freq., Hz Sample 1 Sample 2 Sample 3 Sample 4 Sample 5 CV, %

4 25 12559 13694 13249 13307 13248 3.10

4 20 12254 13312 12849 12930 12826 2.95

4 10 11141 12251 11824 11832 11848 3.39

4 5 10478 11439 10823 10758 10250 4.17

4 2 9310 10104 9552 9522 8774 5.07

4 1 8358 9042 8541 8503 8067 4.17

4 0.5 7746 7801 7467 7609 7342 2.51

4 0.2 6586 6279 6388 6489 6641 2.27

4 0.1 5805 5502 5540 5775 5873 2.93

21 25 5404 5597 5654 5655 5651 1.93

21 20 5142 5402 5352 5323 5319 1.85

21 10 3926 4506 4503 4588 4972 8.32

21 5 3425 3809 3872 3874 4027 5.92

21 2 2489 3021 3053 3052 3466 11.51

21 1 1984 2501 2510 2585 2891 13.10

21 0.5 1437 2070 2068 2072 2644 20.74

21 0.2 1437 1777 1346 1699 1740 12.16

21 0.1 1245 1316 1113 1383 1520 11.55

37 25 1708 2266 2277 2285 2489 13.27

37 20 1872 1894 2196 2127 2063 7.03

37 10 1582 1549 1706 1658 1730 4.73

37 5 1277 1208 1382 1370 1362 5.67

37 2 885 884 993 1054 1053 8.76

37 1 755 721 757 783 786 3.48

37 0.5 544 522 658 699 650 12.60

37 0.2 445 426 467 516 503 8.02

37 0.1 320 347 433 402 422 12.71

141

Table 45: **Dynamic** **Modulus** Test Results **for** Mix BC-28

**Dynamic** **Modulus**, kPa

Mix BC-28, Missouri Demonstration Project, 15% RAP

Temp., C Freq., Hz Sample 1 Sample 2 Sample 3 Sample 4 Sample 5 CV, %

4 25 18977 18985 19308 18392 18813 1.76

4 20 18550 18611 18962 18062 18482 1.74

4 10 17611 17598 17883 17100 17635 1.62

4 5 16667 16673 16713 16427 16447 0.82

4 2 15296 15336 15446 15205 15062 0.95

4 1 14296 14279 14254 14137 14307 0.48

4 0.5 13279 13302 13239 12852 13509 1.80

4 0.2 11935 12013 11691 11723 12256 1.94

4 0.1 11011 11038 10734 10817 11334 2.12

21 25 11121 10608 11851 11160 11270 3.96

21 20 10901 10278 11157 10762 10821 2.97

21 10 9420 9182 10151 9774 9746 3.83

21 5 8420 8314 8964 8651 8642 2.91

21 2 7019 7377 7465 7337 7388 2.36

21 1 6152 6504 6599 6472 6441 2.61

21 0.5 5248 5715 5757 5638 5640 3.62

21 0.2 4774 4667 4362 4666 4678 3.37

21 0.1 4149 4014 3750 4002 4043 3.68

37 25 5043 5033 5073 5016 4968 0.77

37 20 4845 4725 4873 4813 4791 1.17

37 10 4011 3964 3990 4011 3895 1.22

37 5 3278 3135 3333 3281 3189 2.45

37 2 2478 2376 2498 2469 2379 2.38

37 1 1894 1879 1934 1901 1791 2.84

37 0.5 1480 1430 1513 1486 1479 2.03

37 0.2 1169 1055 1095 1091 1012 5.35

37 0.1 914 809 934 847 712 10.55

142

Table 46: **Dynamic** **Modulus** Test Results **for** Mix BC-29

**Dynamic** **Modulus**, kPa

Missouri Demonstration Project, 5% Fine RAS/10% RAP

Temp., C Freq., Hz Sample 1 Sample 2 Sample 3 Sample 4 Sample 5 CV, %

4 25 17163 17080 16865 17084 17131 0.68

4 20 16765 16774 16384 16755 16747 1.01

4 10 15961 15923 15723 15955 15943 0.63

4 5 15140 15152 14959 15151 15142 0.56

4 2 14163 14132 13858 14097 14108 0.87

4 1 13339 13341 13094 13289 13323 0.79

4 0.5 12501 12537 11550 13250 12541 4.85

4 0.2 11511 11459 10320 12331 11505 6.27

4 0.1 10666 10636 9622 11580 10635 6.52

21 25 9988 9986 9784 10042 10038 1.06

21 20 9626 9615 9460 9670 9626 0.84

21 10 8785 8785 8425 8761 8690 1.76

21 5 7895 7915 7557 7912 7917 2.02

21 2 6815 6852 6623 6888 6860 1.56

21 1 6153 6102 5873 6163 6110 1.95

21 0.5 5435 5491 5166 5481 5396 2.46

21 0.2 4681 4679 4260 4675 4659 4.03

21 0.1 4091 4140 3781 4128 4103 3.73

37 25 4817 5058 5014 5043 5063 2.08

37 20 4828 4607 4729 4858 4791 2.08

37 10 4210 3969 3939 4155 4143 2.96

37 5 3613 3299 3415 3556 3595 3.85

37 2 2916 2723 2793 2888 2852 2.73

37 1 2456 2291 2288 2431 2450 3.61

37 0.5 2013 1906 2005 2050 2112 3.73

37 0.2 1646 1544 1590 1638 1630 2.63

37 0.1 1308 1239 1373 1365 1403 4.85

143

Table 47: **Dynamic** **Modulus** Test Results **for** Mix BC-30

**Dynamic** **Modulus**, kPa

Missouri Demonstration Project, 5% Coarse RAS/10% RAP

Temp., C Freq., Hz Sample 1 Sample 2 Sample 3 Sample 4 Sample 5 CV, %

4 25 15651 15919 15953 16073 15933 0.97

4 20 15318 15629 15601 15679 15588 0.91

4 10 14365 14721 14685 14748 14804 1.18

4 5 13800 13817 13864 13869 13484 1.17

4 2 12691 12657 12669 12746 12268 1.52

4 1 11744 11766 11746 11734 11628 0.47

4 0.5 10900 10986 10954 10369 11291 3.06

4 0.2 9810 9864 9822 9356 10167 2.96

4 0.1 9134 9156 9158 8514 9343 3.50

21 25 9935 9827 10019 10077 10014 0.97

21 20 9773 9508 9725 9581 9727 1.17

21 10 8617 8708 8717 8806 8736 0.78

21 5 7735 7926 7918 7730 7904 1.29

21 2 6539 7179 6825 6527 6773 3.92

21 1 5775 6403 6084 5772 6025 4.34

21 0.5 4878 5613 5383 5293 5397 5.08

21 0.2 4421 4578 4555 4353 4512 2.11

21 0.1 3831 3971 4010 3813 3997 2.41

37 25 3958 5002 4629 4548 4628 8.27

37 20 3966 4592 4429 4499 4428 5.53

37 10 3340 3906 3728 3764 3772 5.77

37 5 2801 3232 3225 3246 3129 6.00

37 2 2224 2472 2532 2628 2490 6.06

37 1 1807 2035 2063 2123 2100 6.27

37 0.5 1503 1701 1699 1836 1697 7.03

37 0.2 1171 1336 1400 1329 1346 6.54

37 0.1 911 1106 1138 1086 1121 8.59

144

Table 48: **Dynamic** **Modulus** Test Results **for** Mix BC-31

**Dynamic** **Modulus**, kPa

Indiana Demonstration Project, 15%

Temp., C Freq., Hz Sample 1 RAP/HMA Sample 2 Sample 3 CV, %

4 25 18757 19174 18262 2.44

4 20 18453 18775 17958 2.24

4 10 17317 17568 16913 1.91

4 5 16163 16395 15669 2.31

4 2 14513 14772 14217 1.92

4 1 13390 13405 13104 1.28

4 0.5 12182 12125 12058 0.51

4 0.2 10692 10500 10755 1.25

4 0.1 9733 9437 9735 1.78

21 25 11111 10925 11085 0.91

21 20 10562 10308 10527 1.31

21 10 9245 9123 9298 0.97

21 5 8396 8243 8330 0.92

21 2 7135 7150 6973 1.39

21 1 6179 6231 6084 1.21

21 0.5 5345 5322 5257 0.85

21 0.2 4381 4207 4380 2.31

21 0.1 3758 3512 3760 3.89

37 25 5002 4869 4964 1.38

37 20 4762 4610 4878 2.84

37 10 3977 3801 3937 2.36

37 5 3210 3031 3296 4.26

37 2 2452 2251 2485 5.27

37 1 1872 1793 1950 4.18

37 0.5 1493 1361 1610 8.38

37 0.2 1179 975 1141 9.91

37 0.1 945 690 917 16.42

145

Table 49: **Dynamic** **Modulus** Test Results **for** Mix BC-32

**Dynamic** **Modulus**, kPa

Indiana Demonstration Project, 3% RAS/HMA

Temp., C Freq., Hz Sample 1 Sample 2 Sample 3 Sample 4 Sample 5 CV, %

4 25 17301 16961 16421 16994 16946 1.87

4 20 16764 16419 15978 16473 16435 1.72

4 10 15458 15271 14876 15299 15291 1.42

4 5 14371 14095 13576 14176 14166 2.12

4 2 12675 12453 11849 12413 12528 2.54

4 1 11526 11281 10839 11198 11074 2.27

4 0.5 10621 10113 9541 10101 9965 3.84

4 0.2 9342 8735 8262 8708 8492 4.62

4 0.1 8399 7827 7421 7818 7521 4.89

21 25 9152 9141 8644 9190 9390 3.03

21 20 8827 8793 8400 8785 9047 2.66

21 10 7770 7721 7443 7958 7688 2.39

21 5 6782 6841 6592 6891 6619 1.98

21 2 5668 5658 5396 5495 5629 2.14

21 1 4855 4849 4637 4706 4797 1.99

21 0.5 4104 4116 3817 4082 4178 3.45

21 0.2 3335 3273 3167 3242 3201 2.01

21 0.1 2771 2720 2667 2715 2705 1.37

37 25 3776 3803 3545 3850 3815 3.24

37 20 3627 3619 3475 3639 3608 1.87

37 10 2933 3015 2688 2962 3004 4.59

37 5 2444 2419 2083 2387 2416 6.41

37 2 1800 1769 1529 1749 1755 6.32

37 1 1370 1328 1168 1339 1337 6.12

37 0.5 1069 1022 926 1027 1025 5.20

37 0.2 760 723 587 819 724 11.82

37 0.1 588 481 570 624 465 12.67

146

Table 50: **Dynamic** **Modulus** Test Results **for** Mix BC-33

**Dynamic** **Modulus**, kPa

Indiana Demonstration Project, 3% RAS/WMA

Temp., C Freq., Hz Sample 1 Sample 2 Sample 3 Sample 4 Sample 5 CV, %

4 25 18962 19192 19175 19209 19145 0.52

4 20 18604 18766 18786 18738 18751 0.39

4 10 17460 17626 17633 17639 17613 0.43

4 5 16286 16460 16541 16467 16469 0.58

4 2 14710 14986 14993 15022 14940 0.85

4 1 13580 13766 13804 13843 13842 0.80

4 0.5 12689 12424 12631 12677 12615 0.85

4 0.2 11455 10675 11131 11174 11143 2.52

4 0.1 10383 9542 10017 10096 10033 3.02

21 25 9329 9796 10026 9866 9868 2.70

21 20 9024 9497 9614 9460 9482 2.41

21 10 8163 8292 8326 8296 8342 0.85

21 5 6999 7293 7307 7333 7291 1.91

21 2 5747 6081 6072 6031 6022 2.31

21 1 4975 5181 5226 5144 5156 1.86

21 0.5 4251 4373 4361 4435 4371 1.53

21 0.2 3227 3554 3580 3488 3562 4.22

21 0.1 2659 2955 3000 2951 2979 4.85

37 25 3382 4233 4015 4091 4235 8.85

37 20 3581 3923 3938 3926 3887 3.96

37 10 2962 3208 3192 3148 3161 3.17

37 5 2428 2502 2560 2565 2540 2.25

37 2 1804 1817 1867 1871 1851 1.63

37 1 1313 1303 1496 1457 1415 6.16

37 0.5 1035 928 1161 1154 1093 8.97

37 0.2 721 674 828 842 782 9.28

37 0.1 609 487 617 579 588 9.04

147

APPENDIX B: DSR TEST RESULTS

Table 51: DSR Test Results

Temperature, C

58 64 70 76 82

Mix Test δ, ° G*, Pa δ, ° G*, Pa δ, ° G*, Pa δ, ° G*, Pa δ, ° G*, Pa

1 72.44 12510 75.31 5654 78.11 2624 80.54 1302

BC21 2 72.62 11980 75.50 5468 78.19 2619 80.68 1266

3 72.91 11715 75.68 5374 78.39 2531 80.80 1248

1 74.95 12460 78.00 5399 80.78 2436 83.15 1157

BC22 2 74.11 14170 77.22 6223 80.07 2858 82.58 1349

3 74.26 13350 77.30 5914 80.15 2693 82.61 1275

1 78.54 9254 81.41 4001 83.87 1795

BC23 2 78.73 8641 81.60 3724 84.00 1683

3 78.71 9429 81.59 4044 84.00 1835

1 75.72 18190 78.98 7790 81.90 3391 84.29 1563

BC24 2 75.84 17800 79.15 7505 82.00 3340 84.40 1527

3 76.06 18340 79.34 7680 82.17 3377 84.51 1554

1 70.07 21240 73.48 9534 76.80 4396 79.78 2095

BC25 2 69.95 21400 73.29 9722 76.59 4515 79.57 2160

3 69.90 21220 73.16 9733 76.47 4489 79.51 2106

1 64.50 35160 67.71 16510 71.20 7800 74.60 3790 77.73 1846

BC26 2 64.30 36700 67.50 17340 71.02 8194 74.51 3921 77.65 1950

3 64.22 37660 67.38 18060 70.86 8586 74.31 4130 77.54 2018

1 60.80 51000 63.50 25230 66.74 12420 70.22 6085 73.65 3054

BC27 2 60.77 48100 63.60 23440 66.80 11525 70.24 5660

3 60.19 59140 62.92 29180 66.13 14295 69.54 7052 73.02 3489

1 72.62 30580 75.76 13120 78.83 5736 81.50 2632 83.76 1261

BC28 2 72.57 30460 75.74 13045 78.82 5685 81.52 2587 83.79 1230

3 72.51 31060 75.63 13320 78.69 2616 81.42 2616 83.70 1242

1 61.83 52200 64.52 25720 67.65 12590 71.03 6160

BC29 2 62.72 39360 65.30 20620 68.38 10150 71.70 4930

3 62.92 44720 65.45 22170 68.38 11060 71.47 5567

1 64.76 35600 67.63 17295 70.96 8326 74.29 4100

BC30 2 64.67 36600 67.53 17840 70.98 8470 74.01 4265

3 64.72 36300 67.07 18790 70.51 8942 72.85 4755

1 75.23 24370 78.21 10795 81.20 4608 83.63 2090

BC31 2 75.03 23100 78.30 9720 81.27 4185 83.67 1936

3 74.90 25450 78.22 10595 81.20 4580 83.65 2110

1 70.33 33500 73.61 14945 76.95 6718 80.01 3082 82.54 1462

BC32 2 70.32 34140 73.68 15060 77.07 6683 80.05 3130 82.64 1461

3 70.45 31900 73.85 13910 77.18 6238 80.19 2874 82.75 1375

1 71.19 29220 74.59 12785 77.95 5677 80.79 2652 83.22 1239

BC33 2 71.02 30870 74.50 13300 77.84 5992 80.75 2780 83.16 1317

3 70.81 32380 74.31 14045 77.72 6205 80.75 2804 83.04 1386

148

149

APPENDIX C: DSR FREQUENCY SWEEP TEST RESULTS

Table 52: DSR Frequency Sweep Test Results **for** Mixes BC-21, 23, 24, and 25

Mix

Temp. Freq. BC-21 BC-23 BC-24 BC-25

C Hz G*, Pa Φ G*, Pa Φ G*, Pa Φ G*, Pa Φ

9 0.100 7336000 46.40 12250000 42.00 8991000 40.52

9 0.126 8288000 45.62 13610000 41.29 9933000 39.95

9 0.158 9327000 44.92 15150000 40.55 11070000 39.34

9 0.200 10530000 44.19 16830000 39.84 12220000 38.82

9 0.251 11800000 43.51 18720000 39.13 13370000 38.35

9 0.316 13210000 42.83 20690000 38.45 14740000 37.84

9 0.398 14730000 42.17 22710000 37.82 16160000 37.36

9 0.501 16310000 41.56 25000000 37.17 17850000 36.85

9 0.631 18160000 40.91 27530000 36.53 19760000 36.32

9 0.794 20170000 40.26 30160000 35.90 21720000 35.82

9 1.000 22300000 39.65 33020000 35.29 23580000 35.40

9 1.259 24710000 39.02 36080000 34.69 25780000 34.95

9 1.585 27210000 38.42 39450000 34.07 28210000 34.48

9 1.995 29940000 37.81 42990000 33.48 30680000 34.04

9 2.512 32890000 37.23 46870000 32.90 33460000 33.58

9 3.162 36190000 36.62 50860000 32.36 36510000 33.08

9 3.981 39720000 36.04 55220000 31.80 39720000 32.62

9 5.012 43480000 35.47 59810000 31.25 43100000 32.18

9 6.310 47440000 34.90 64710000 30.71 46790000 31.74

9 7.943 51770000 34.32 70050000 30.17 50760000 31.29

9 10.000 56520000 33.65 75760000 29.75 54970000 30.80

9 12.590 61590000 32.95 81150000 29.08 59340000 30.30

9 15.849 67090000 32.66 87560000 28.45 64070000 29.97

9 19.953 72850000 31.96 94160000 28.03 69070000 29.56

9 25.121 79150000 31.38 100900000 27.55 74450000 29.26

9 31.623 85730000 30.71 108300000 27.01 80060000 28.70

9 39.809 92550000 30.18 116000000 26.38 86220000 28.16

9 50.000 99780000 29.56 123900000 25.77 92680000 27.72

13 0.100 3495000 47.50 3767000 50.44 6696000 45.85 4899000 44.25

13 0.158 4420000 46.22 4934000 48.99 8541000 44.32 6194000 43.04

13 0.251 5622000 45.00 6251000 47.70 10640000 42.94 7633000 41.97

13 0.398 7048000 43.87 7926000 46.39 13140000 41.62 9397000 40.91

13 0.631 8827000 42.73 10030000 45.07 16230000 40.30 11530000 39.88

13 1.000 10970000 41.60 12600000 43.78 19890000 39.02 14100000 38.87

13 1.585 13510000 40.55 15750000 42.49 24220000 37.76 17170000 37.86

13 2.512 16580000 39.39 19480000 41.23 29220000 36.60 20770000 36.85

13 3.981 20210000 38.24 24000000 39.99 35180000 35.44 24970000 35.90

13 6.310 24630000 37.19 29350000 38.73 41890000 34.31 30000000 34.91

13 10.000 29680000 36.15 35550000 37.40 49690000 33.07 35730000 34.07

150

Mix

Temp. Freq. BC-21 BC-23 BC-24 BC-25

C Hz G*, Pa Φ G*, Pa Φ G*, Pa Φ G*, Pa Φ

13 15.849 35510000 35.14 42970000 36.32 58730000 32.13 42460000 32.91

13 25.121 42360000 34.14 51690000 35.23 69200000 31.00 50100000 32.19

13 39.809 50300000 33.16 61750000 33.84 80790000 29.78 59200000 31.23

13 50.000 54710000 32.68 67230000 33.13 86980000 29.26 63950000 30.71

21 0.100 900600 54.09 896400 58.12 1732000 54.14 1364000 50.91

21 0.158 1184000 53.02 1193000 56.91 2287000 52.66 1766000 49.78

21 0.251 1555000 51.94 1602000 55.63 2989000 51.21 2273000 48.69

21 0.398 2023000 50.86 2126000 54.38 3859000 49.81 2914000 47.61

21 0.631 2621000 49.77 2798000 53.12 4967000 48.42 3708000 46.56

21 1.000 3377000 48.64 3650000 51.88 6349000 47.07 4691000 45.52

21 1.585 4332000 47.52 4736000 50.65 8041000 45.76 5901000 44.48

21 2.512 5504000 46.45 6118000 49.40 10120000 44.52 7385000 43.46

21 3.981 6956000 45.39 7859000 48.04 12630000 43.28 9209000 42.43

21 6.310 8746000 44.34 9963000 46.74 15650000 41.94 11440000 41.48

21 10.000 10970000 43.51 12670000 45.53 19350000 40.54 14090000 40.63

21 15.849 13600000 42.20 15950000 44.20 23810000 39.61 17290000 39.34

21 25.121 16830000 41.08 19950000 42.97 29070000 38.19 21050000 38.55

21 39.809 20770000 40.08 24810000 41.55 35290000 37.00 25640000 37.64

21 50.000 22960000 39.57 27580000 40.88 38760000 36.38 28160000 37.08

29 0.100 222100 59.43 200100 64.71 417000 61.15 373200 56.44

29 0.158 299800 58.55 281000 63.46 570400 59.85 498700 55.30

29 0.251 404800 57.70 386000 62.39 774400 58.55 662300 54.23

29 0.398 544200 56.82 528200 61.34 1041000 57.29 870800 53.20

29 0.631 728000 55.86 720500 60.25 1393000 56.01 1137000 52.20

29 1.000 969300 54.87 976200 59.13 1852000 54.73 1483000 51.24

29 1.585 1284000 53.89 1315000 58.02 2444000 53.47 1924000 50.32

29 2.512 1688000 52.97 1759000 56.93 3199000 52.22 2481000 49.43

29 3.981 2207000 52.03 2343000 55.75 4160000 50.95 3189000 48.49

29 6.310 2865000 51.02 3097000 54.37 5366000 49.58 4049000 47.48

29 10.000 3715000 50.03 4111000 53.28 6903000 48.13 5180000 46.60

29 15.849 4784000 49.12 5389000 51.97 8824000 47.05 6564000 45.62

29 25.121 6162000 48.08 7038000 50.66 11200000 45.76 8281000 44.63

29 39.809 7850000 47.03 9086000 49.34 14110000 44.59 10400000 43.69

29 50.000 8842000 46.67 10340000 48.76 15830000 43.86 11630000 43.31

37 0.100 57080 64.64 44810 70.91 98940 67.16 101800 61.71

37 0.158 79240 63.37 64880 69.55 139400 65.88 139100 60.55

37 0.251 110500 62.29 91900 68.34 195100 64.65 189000 59.47

37 0.398 149700 61.37 128600 67.19 269600 63.50 255000 58.46

37 0.631 204400 60.71 179700 66.20 373100 62.34 343100 57.50

37 1.000 280300 59.81 252600 65.23 511200 61.21 460100 56.55

37 1.585 379800 59.00 355700 64.18 695300 60.10 613600 55.65

37 2.512 509400 58.24 493800 63.19 941500 59.00 811400 54.82

151

Mix

Temp. Freq. BC-21 BC-23 BC-24 BC-25

C Hz G*, Pa Φ G*, Pa Φ G*, Pa Φ G*, Pa Φ

37 3.981 685100 57.44 678100 62.18 1265000 57.85 1071000 53.98

37 6.310 916400 56.63 927400 60.96 1699000 56.60 1408000 53.06

37 10.000 1223000 55.65 1271000 60.13 2269000 55.41 1847000 52.23

37 15.849 1623000 54.86 1718000 59.11 2999000 54.27 2409000 51.39

37 25.121 2153000 54.02 2321000 58.21 3951000 53.00 3136000 50.53

37 39.809 2840000 53.24 3113000 57.38 5181000 51.90 4050000 49.89

37 50.000 3261000 52.89 3591000 56.92 5926000 51.27 4584000 49.55

Table 53: DSR Frequency Sweep Test Results **for** Mixes BC-27, 28, 29, and 30

Mix

Temp. Freq. BC-27 BC-28 BC-29 BC-30

C Hz G*, Pa Φ G*, Pa Φ G*, Pa Φ G*, Pa Φ

9 0.100

9 0.126 22950000 33.58 26650000 28.45 26540000 28.34

9 0.158 28720000 28.02 28770000 27.90

9 0.200 26950000 32.52 30950000 27.60 30870000 27.52

9 0.251 33200000 27.22 33020000 27.17

9 0.316 31750000 31.48 35310000 26.89 35570000 26.80

9 0.398 37900000 26.53 37950000 26.47

9 0.501 37230000 30.49 40790000 26.17 40720000 26.14

9 0.631 43580000 25.84 43470000 25.83

9 0.794 43320000 29.57 46640000 25.53 46410000 25.53

9 1.000 49890000 25.22 49400000 25.25

9 1.259 50300000 28.68 53250000 24.92 52610000 24.98

9 1.585 56630000 24.64 56180000 24.70

9 1.995 58140000 27.82 60510000 24.37 59860000 24.44

9 2.512 64330000 24.10 63630000 24.17

9 3.162 66840000 27.01 68480000 23.84 67650000 23.92

9 3.981 72680000 23.61 71960000 23.75

9 5.012 76530000 26.20 77110000 23.41 76530000 23.51

9 6.310 81800000 23.16 81110000 23.29

9 7.943 87530000 25.43 86540000 22.91 86000000 23.05

9 10.000 91540000 22.50 90930000 22.65

9 12.590 99470000 24.49 97250000 22.27 96760000 22.56

9 15.849 102900000 22.22 102500000 22.28

9 19.953 112200000 24.17 109200000 21.90 108300000 22.06

9 25.121 115300000 21.69 114900000 21.89

9 31.623 127400000 22.90 122100000 21.27 121800000 21.57

9 39.809 128900000 21.05 128500000 21.18

9 50.000 134200000 22.65 135800000 20.78 135300000 20.91

13 0.100 5389000 38.64 11470000 38.40 16110000 31.34 16250000 31.06

152

Mix

Temp. Freq. BC-27 BC-28 BC-29 BC-30

C Hz G*, Pa Φ G*, Pa Φ G*, Pa Φ G*, Pa Φ

13 0.158 6545000 37.70 14100000 37.04 19080000 30.37 19240000 30.15

13 0.251 7912000 36.81 16860000 35.89 22110000 29.56 22220000 29.41

13 0.398 9542000 35.97 20110000 34.78 25540000 28.80 25800000 28.68

13 0.631 11450000 35.19 23860000 33.73 29510000 28.10 29850000 27.99

13 1.000 13710000 34.46 28340000 32.69 34060000 27.42 34340000 27.36

13 1.585 16260000 33.77 33270000 31.73 39130000 26.80 39470000 26.75

13 2.512 19280000 33.09 38990000 30.79 44790000 26.22 45090000 26.22

13 3.981 22830000 32.41 45520000 29.88 51140000 25.72 51600000 25.67

13 6.310 26860000 31.77 52840000 29.01 58160000 25.23 58730000 25.23

13 10.000 31510000 31.22 61270000 28.22 65890000 24.55 66630000 24.75

13 15.849 36750000 30.53 70590000 27.31 74910000 24.19 75520000 24.33

13 25.121 42930000 29.99 81160000 26.45 84800000 23.69 85390000 23.74

13 39.809 50080000 29.29 92660000 25.60 95710000 23.09 96450000 23.07

13 50.000 53910000 28.99 98710000 25.15 101400000 22.81 102100000 22.84

21 0.100 1802000 44.18 3316000 47.12 5934000 37.41 5956000 36.99

21 0.158 2258000 43.18 4220000 45.62 7161000 36.28 7159000 36.01

21 0.251 2826000 42.21 5314000 44.19 8617000 35.23 8612000 35.07

21 0.398 3488000 41.35 6625000 42.86 10280000 34.30 10260000 34.22

21 0.631 4299000 40.50 8219000 41.57 12220000 33.42 12160000 33.43

21 1.000 5274000 39.70 10130000 40.35 14460000 32.63 14390000 32.68

21 1.585 6447000 38.93 12410000 39.18 17050000 31.87 16970000 31.96

21 2.512 7843000 38.19 15090000 38.03 20010000 31.16 19920000 31.28

21 3.981 9510000 37.48 18260000 36.90 23400000 30.55 23300000 30.63

21 6.310 11500000 36.80 21990000 35.83 27230000 29.94 27190000 30.00

21 10.000 13880000 36.22 26320000 34.85 31610000 29.19 31610000 29.41

21 15.849 16630000 35.40 31330000 33.79 36750000 28.78 36690000 28.80

21 25.121 19890000 34.72 37070000 32.92 42500000 28.21 42470000 28.35

21 39.809 23830000 34.12 43970000 31.93 49090000 27.59 49020000 27.64

21 50.000 25970000 33.80 47570000 31.34 52640000 27.30 52590000 27.42

29 0.100 580900 49.25 836800 55.58 1990000 43.55 1971000 43.37

29 0.158 749100 48.21 1114000 54.06 2492000 42.26 2455000 42.25

29 0.251 956500 47.26 1466000 52.60 3083000 41.10 3036000 41.21

29 0.398 1217000 46.36 1913000 51.17 3803000 40.00 3739000 40.20

29 0.631 1540000 45.51 2474000 49.79 4661000 38.98 4577000 39.25

29 1.000 1939000 44.69 3174000 48.44 5665000 38.05 5569000 38.35

29 1.585 2432000 43.90 4047000 47.13 6861000 37.18 6754000 37.50

29 2.512 3038000 43.14 5129000 45.86 8283000 36.44 8157000 36.70

29 3.981 3777000 42.41 6459000 44.60 9968000 35.70 9809000 35.96

29 6.310 4676000 41.70 8060000 43.40 11840000 35.05 11750000 35.24

29 10.000 5768000 40.94 10040000 42.09 14140000 34.21 14040000 34.52

29 15.849 7111000 40.29 12430000 41.14 16880000 33.66 16710000 33.88

29 25.121 8724000 39.57 15330000 39.82 20000000 33.06 19880000 33.22

153

Mix

Temp. Freq. BC-27 BC-28 BC-29 BC-30

C Hz G*, Pa Φ G*, Pa Φ G*, Pa Φ G*, Pa Φ

29 39.809 10710000 38.96 18770000 38.81 23660000 32.45 23510000 32.54

29 50.000 11810000 38.64 20760000 38.28 25650000 32.16 25570000 32.25

37 0.100 189600 53.75 199300 62.80 629000 49.70 605200 49.60

37 0.158 251000 52.62 278400 61.45 811600 48.38 779700 48.43

37 0.251 328400 51.64 372500 60.31 1033000 47.21 991800 47.33

37 0.398 426400 50.73 504700 58.87 1313000 46.09 1259000 46.28

37 0.631 552400 49.89 679200 57.52 1655000 45.03 1593000 45.25

37 1.000 710800 49.11 907700 56.20 2073000 44.02 2004000 44.26

37 1.585 909300 48.35 1207000 54.90 2587000 43.06 2506000 43.33

37 2.512 1163000 47.61 1591000 53.60 3208000 42.12 3118000 42.46

37 3.981 1479000 46.92 2096000 52.27 3982000 41.02 3854000 41.66

37 6.310 1879000 46.24 2717000 51.02 4909000 40.18 4746000 40.85

37 10.000 2369000 45.40 3506000 49.65 5993000 39.38 5820000 39.96

37 15.849 2989000 44.87 4524000 48.39 7325000 38.61 7137000 39.23

37 25.121 3763000 44.24 5788000 47.05 8915000 37.87 8727000 38.49

37 39.809 4713000 43.57 7377000 45.73 10810000 37.19 10620000 37.84

37 50.000 5282000 43.29 8326000 45.19 11910000 36.88 11690000 37.56

Table 54: DSR Frequency Sweep Test Results **for** Mixes BC-31, 32, and 33

Mix

Temp. Freq. BC-31 BC-32 BC-33

C Hz G*, Pa Φ G*, Pa Φ G*, Pa Φ

9 0.100

9 0.126 15000000 39.38 21390000 36.47 16400000 37.53

9 0.158 16630000 38.67 23510000 35.87 18190000 36.87

9 0.200 18300000 38.01 25810000 35.28 19890000 36.32

9 0.251 20200000 37.35 28100000 34.76 21840000 35.74

9 0.316 22210000 36.70 30710000 34.22 23940000 35.17

9 0.398 24300000 36.09 33470000 33.71 26150000 34.63

9 0.501 26700000 35.46 36410000 33.21 28570000 34.09

9 0.631 29200000 34.86 39670000 32.70 31220000 33.55

9 0.794 32000000 34.25 43200000 32.21 33940000 33.04

9 1.000 34840000 33.68 46900000 31.73 36920000 32.53

9 1.259 38030000 33.10 50740000 31.28 40180000 32.02

9 1.585 41210000 32.57 55030000 30.81 43600000 31.53

9 1.995 44840000 32.00 59480000 30.35 47180000 31.07

9 2.512 48610000 31.47 64180000 29.91 50970000 30.64

9 3.162 52580000 30.94 69170000 29.46 55290000 30.20

9 3.981 56870000 30.41 74620000 29.01 59600000 29.77

9 5.012 61440000 29.88 80330000 28.57 64260000 29.39

9 6.310 66100000 29.38 86370000 28.14 69170000 28.94

154

9 7.943 71090000 28.87 92630000 27.72 74340000 28.51

9 10.000 76730000 28.35 99330000 27.29 79780000 28.09

9 12.590 82220000 27.78 106400000 26.86 85710000 27.69

9 15.849 88180000 27.28 113900000 26.47 91780000 27.23

9 19.953 94450000 26.86 121600000 26.05 98660000 26.66

9 25.121 101000000 26.34 130000000 25.60 105800000 26.30

9 31.623 108100000 25.77 139000000 25.11 113100000 25.75

9 39.809 115600000 25.24 148200000 24.57 120800000 25.38

9 50.000 122900000 24.63 157200000 24.05 128000000 24.82

13 0.100 7531000 44.11 11320000 40.51 8534000 41.61

13 0.158 9462000 42.65 13890000 39.31 10660000 40.31

13 0.251 11700000 41.30 16900000 38.18 12980000 39.16

13 0.398 14410000 39.99 20420000 37.08 15790000 38.03

13 0.631 17610000 38.72 24620000 36.01 19100000 36.93

13 1.000 21280000 37.51 29550000 34.98 22990000 35.86

13 1.585 25710000 36.30 35240000 33.98 27570000 34.82

13 2.512 30820000 35.13 41690000 33.03 32840000 33.88

13 3.981 36660000 34.02 49150000 32.08 38950000 33.00

13 6.310 43560000 32.89 57810000 31.16 45860000 32.09

13 10.000 51370000 31.78 67700000 30.35 53720000 30.93

13 15.849 60330000 30.73 78570000 29.41 63070000 30.25

13 25.121 70420000 29.59 90850000 28.44 73620000 29.33

13 39.809 81800000 28.49 105100000 27.49 85260000 28.33

13 50.000 87840000 27.92 112700000 27.03 91580000 27.83

21 0.100 2039000 52.57 3296000 48.16 2433000 49.17

21 0.158 2646000 51.16 4186000 46.91 3133000 47.88

21 0.251 3437000 49.73 5303000 45.68 3993000 46.65

21 0.398 4414000 48.34 6686000 44.47 5046000 45.46

21 0.631 5635000 46.97 8348000 43.33 6346000 44.32

21 1.000 7139000 45.62 10390000 42.20 7928000 43.20

21 1.585 8965000 44.30 12850000 41.09 9850000 42.13

21 2.512 11210000 42.99 15810000 39.99 12170000 41.04

21 3.981 13920000 41.69 19300000 38.91 14970000 39.95

21 6.310 17150000 40.43 23500000 37.84 18310000 38.92

21 10.000 20990000 39.19 28380000 36.78 22230000 37.66

21 15.849 25610000 37.86 34210000 35.72 26930000 36.66

21 25.121 31030000 36.72 40890000 34.75 32450000 35.70

21 39.809 37350000 35.54 48960000 33.83 38960000 34.75

21 50.000 40810000 34.90 53260000 33.33 42540000 34.24

29 0.100 489800 60.08 901400 54.80 622600 56.56

29 0.158 664500 58.82 1189000 53.59 833700 55.36

29 0.251 897500 57.54 1567000 52.39 1108000 54.05

29 0.398 1197000 56.27 2041000 51.24 1461000 52.78

29 0.631 1594000 54.97 2643000 50.11 1909000 51.57

29 1.000 2113000 53.64 3404000 48.98 2477000 50.44

155

29 1.585 2773000 52.32 4360000 47.85 3185000 49.37

29 2.512 3616000 50.96 5549000 46.74 4083000 48.28

29 3.981 4681000 49.63 7032000 45.62 5203000 47.18

29 6.310 6009000 48.31 8851000 44.54 6595000 46.00

29 10.000 7657000 47.08 11060000 43.30 8309000 44.63

29 15.849 9714000 45.52 13800000 42.26 10460000 43.77

29 25.121 12220000 44.32 17080000 41.21 13100000 42.63

29 39.809 15310000 43.02 21130000 40.21 16250000 41.55

29 50.000 17060000 42.38 23370000 39.64 18070000 41.06

37 0.100 114000 66.38 240500 60.65 157600 62.64

37 0.158 158000 65.26 330000 59.35 215600 61.44

37 0.251 219900 64.12 447300 58.26 298300 60.17

37 0.398 305200 62.97 602500 57.23 401300 59.22

37 0.631 421600 61.80 801500 56.20 538500 58.17

37 1.000 578000 60.65 1064000 55.16 723700 57.23

37 1.585 782300 59.51 1411000 54.10 975200 56.11

37 2.512 1060000 58.32 1855000 53.08 1296000 55.02

37 3.981 1424000 57.12 2423000 52.06 1716000 53.94

37 6.310 1901000 55.92 3151000 51.00 2246000 52.89

37 10.000 2517000 54.59 4080000 50.03 2937000 51.62

37 15.849 3327000 53.22 5257000 48.77 3823000 50.66

37 25.121 4361000 51.95 6741000 47.82 4927000 49.46

37 39.809 5680000 50.55 8582000 46.69 6353000 48.53

37 50.000 6484000 49.88 9648000 46.20 7184000 48.11

156